serviceability analysis of reinforced concrete
TRANSCRIPT
Research Collection
Doctoral Thesis
Serviceability analysis of reinforced concrete based in thetension chord model
Author(s): Burns, Clare
Publication Date: 2011
Permanent Link: https://doi.org/10.3929/ethza007179384
Rights / License: In Copyright  NonCommercial Use Permitted
This page was generated automatically upon download from the ETH Zurich Research Collection. For moreinformation please consult the Terms of use.
ETH Library
DISS. ETH NO. 19979
SERVICEABILITY ANALYSIS OF REINFORCED CONCRETE
BASED ON THE TENSION CHORD MODEL
A dissertation submitted to
ETH ZURICH
for the degree of
Doctor of Sciences
presented by
CLARE BURNS
Dipl. Bauingenieur ETH
born on the 25 July 1977
citizen of Effingen, AG
accepted on the recommendation of
Prof. Dr. Peter Marti, examiner
Prof. Dr. György L. Balázs, coexaminer
2011
Preface
"Structural Engineering is the art of moulding materials we do not wholly understand into
shapes we cannot precisely analyse, so as to withstand forces we cannot really assess, in such
a way that the community at large has no reason to suspect the extent of our ignorance."
Dykes (1978)
This quotation refers to the complex and hardly predictable load sequences and the highly variable concrete properties, which limit the accuracy of serviceability limit state deformation predictions in particular. Nevertheless, practical applications require reasonably reliable estimates of both integral and local deformations under service loads.
The present thesis illustrates how the Tension Chord Model can be used to estimate the serviceability limit state behaviour of tensile and bending members. The Tension Chord Model is an analytical model that was developed within Prof. Marti's group at the Institute of Structural Engineering (IBK) of ETH Zurich. During the past twenty years it has been used to model the deformation behaviour of tensile ties and beams. Even though most previous applications were focused on ultimate limit state solutions, the model was also found to give good crack width and deflection predictions under service loads. This is why the present PhD thesis work was initiated with the aim of systematically applying the Tension Chord Model for serviceability design and verifying its prediction quality.
The scope of the theoretical work summarized in Chapter 4 was guided by a number of questions, which arose during the course of the work. At the beginning, a discussion (Burns et al. 2008) written in response to a technical note on tension stiffening (Gilbert 2007) initiated the work on bending members and led to the transformed section propertydependent tension stiffening and cracking equations. In a next step, the tension stiffening equations were combined with Ghali's creep and shrinkage curvature coefficients (Burns 2008). However, as a result of subsequent parameter studies, the much simpler Effective Modulus Method was used for further longterm deflection calculations. At this point, the topic of low shrinkage concrete directed the work towards shrinkage cracking, leading to the discussion on restraintinduced cracking under different boundary conditions. Finally, the calculations for the ConCrack prediction contest led to the endrestraint cracking approach being extended to account for elastic restraint conditions and the simultaneous presence of shrinkage and coolinginduced strains.
This research work could not have been carried out had it not been for my supervisor Prof. Dr. Peter Marti, who gave me the opportunity to be part of his research group at the Institute of Structural Engineering of ETH Zurich. I am also much obliged to Prof. Dr. György L. Balázs for being my cosupervisor and inviting me to join the fib Serviceability Models Task Group 4.1. My greatest thanks are reserved for my wonderful colleagues, who shared my time at IBK. I would like to particularly thank Stephan Etter, Hans Seelhofer and Patrick Fehlmann for their much appreciated technical advice, Andreas Galmarini for making sure this work got written and Almut Pohl for helping me prepare the presentations. Last but not least, I would like to express my gratitude to my parents and my husband Rodrigo Pérez for their support and understanding.
Zurich, September 2011 Clare Burns
Abstract
In the present thesis the Tension Chord Model is applied to describe the deformation behaviour of reinforced concrete (RC) tensile and bending members in the serviceability limit state.
After an introduction (Chapter 1), the most frequently used crack width and deflection approaches are described in Chapter 2. The two different concepts of transfer length adopted by the slippingbond and concretecover crack width approaches are compared in the first part of the chapter. The second part of the chapter discusses the tension stiffening models of Branson and Rao, which differ especially for low reinforcement ratios. Further, global deflection approaches are compared.
Chapter 3 contains the basic principles required for the crack width and deflection approaches presented in Chapter 4. The first two parts of the chapter summarise the concrete and steel material properties used for the serviceability limit state. The third part of the chapter deals with approaches for determining the State I and II section deformations under sustained and variable loads. It is shown that the AgeAdjusted Effective Modulus Method (AAEMM) and the Effective Modulus Method (EMM) provide similar deformations for ordinary RC sections under sustained loads. In the fourth part of the chapter the Tension Chord Model is presented and its two main assumptions, which are the rigidperfectly plastic bond stressslip relation and the constant tensile strength, are discussed.
The first part of Chapter 4 provides expressions for considering tension stiffening in bending members under shortterm and sustained loads as well as during unloading. The momentinduced crack width equations given in the second part of the chapter are functions of the transformed section properties. They are followed by a discussion on restraintinduced cracking due to uniform cooling and shrinkageinduced strains. Besides spantodepth ratios, the third section of the chapter illustrates systemdependent interpolation coefficients for global deflection calculations.
In Chapter 5 the approaches discussed in Chapter 4 are verified with a selection of test series from various research institutions. The test data comparisons show that the State II section approach (cracked elastic state neglecting tension stiffening) leads to consistent upper limit predictions for the local and integral deformations of members with constant moment distributions. In combination with the Tension Chord Model the State II section approach provides good lower limit deformation predictions. In most cases, the Tension Chord Model gives a good estimate of the maximum crack spacing. However, both the deformation and crack width comparisons show that the effective deformations vary arbitrarily between the lower (considering tension stiffening) and upper (no tension stiffening) limits. Further, the support moments predicted for the twospan beams are all larger than the measured values.
Chapter 6 discusses the approaches illustrated in Chapter 4. It is shown that lightly (strongly) reinforced endrestrained tensile members are characterized by widely (closely) spaced cracks with large (small) crack openings. The cracking behaviour of bending members is strongly dependent on the effective reinforcement ratio of the tension chord. Moment redistributions have a large influence on beam deflections, while the relative influence of tension stiffening decreases with increasing load level and time.
The overall conclusions are summarized in Chapter 7.
Kurzfassung
Die vorliegende Arbeit zeigt, wie das Verformungsverhalten von Zuggliedern und Balken mit dem Zuggurtmodell modelliert werden kann. Nach einer Einführung (Kapitel 1) werden in Kapitel 2 häufig verwendete Berechnungsmodelle für Rissbreiten und Durchbiegungen betrachtet. Im ersten Teil des Kapitels werden zwei unterschiedliche Rissmodelle verglichen. Im ersten Modell wird der Rissabstand unter Annahme eines verschieblichen Verbundes berechnet, während im zweiten Modell die Betonüberdeckung dazu benützt wird. Der zweite Teil des Kapitels beinhaltet Raos und Bransons Modelle zur Berücksichtigung der Zugversteifung. Insbesondere bei tiefen Bewehrungsgehalten liefern die beiden Modelle unterschiedliche Resultate. Am Schluss des Kapitels werden globale Durchbiegungsmodelle verglichen.
Kapitel 3 beinhaltet die Grundlagen der Berechnungsmodelle in Kapitel 4. Die ersten beiden Kapitelteile geben einen Überblick über das Materialverhalten von Stahl und Beton unter Gebrauchslasten. Im dritten Teil des Kapitels werden Berechnungsmodelle für Querschnittsverformungen unter Langzeit und veränderlichen Lasten besprochen. Es wird gezeigt, dass die Annahme eines wirksamen Elastizitätsmoduls (EMM) und das Verfahren von Trost (AAEMM) ähnliche Verformungen für gewöhnliche Stahlbetonquerschnitte unter Langzeitbiegung ergeben. Im vierten Kapitelteil werden das Zuggurtmodell vorgestellt und seine beiden Hauptannahmen erläutert. Es handelt sich dabei um die starrideal plastische VerbundschubspannungsSchlupfBeziehung und die konstante Betonzugfestigkeit.
Im ersten Teil von Kapitel 4 werden Ansätze für die Berücksichtigung der Zugversteifung in Biegeträgern unter Langzeitlasten und während der Entlastung präsentiert. Im zweiten Teil des Kapitels werden die Biegerissbreiten mit ideellen Querschnittswerten berechnet. Es folgt eine Diskussion über das Rissverhalten von beidseitig eingespannten Zuggliedern infolge gleichmässig verteilter temperatur und schwindinduzierter Dehnungen. Der dritte Teil des Kapitels beinhaltet Biegeschlankheiten sowie Interpolationskoeffizienten für globale Durchbiegungsberechnungen.
In Kapitel 5 werden die Berechnungsmodelle aus Kapitel 4 mit Versuchsdaten von verschiedenen Forschungsinstituten verifiziert. Die Nachrechnungen zeigen, dass Verformungsberechnungen an Querschnitten im Zustand II (gerissen elastisches Materialverhalten ohne Zugversteifung) zuverlässige obere Grenzwerte der lokalen und integralen Verformungen liefern. Wird zusätzlich mit dem Zuggurtmodell die Zugversteifung berücksichtigt, entstehen gute untere Grenzwerte. Das Zuggurtmodell liefert auch einen guten Richtwert für den maximalen Rissabstand. Es ist aber zu beachten, dass die gemessenen Rissbreiten und Verformungen beliebig zwischen den oberen (ohne Zugversteifung) und unteren (mit Zugversteifung) Grenzwerten liegen. Des Weiteren werden die Stützmomente bei den Zweifeldträgern rechnerisch überschätzt.
In Kapitel 6 werden die Berechnungsmodelle aus Kapitel 4 diskutiert. Es wird gezeigt, dass bei beidseitig eingespannten Zuggliedern eine schwache (starke) Bewehrung zu grossen (kleinen) Rissabständen und entsprechend grossen (kleinen) Rissbreiten führt. Das Rissverhalten von Biegeträgern ist stark vom effektiven Bewehrungsgehalt im Zuggurt abhängig. Momentenumlagerungen haben einen grossen Einfluss auf die integralen Verformungen, während der relative Einfluss der Zugversteifung mit zunehmender Last und Zeit abnimmt. Kapitel 7 beinhaltet Schlussfolgerungen.
i
Content
1 Introduction 1
1.1 Background 1 1.2 Aims 1 1.3 Research Significance 1 1.4 Overview 2 1.5 Limitations 3
2 State of the Art 5
2.1 Crack Width 5 2.1.1 SlippingBond Approach 5 2.1.2 ConcreteCover Approach 7
2.2 Deflections 9 2.2.1 Section Level 9 2.2.2 Member Level 11
2.3 Summary 12
3 Basic Principles 13
3.1 Concrete Material Behaviour 13 3.1.1 ShortTerm 13 3.1.2 LongTerm 14
3.2 Steel Material Behaviour 23 3.3 Uncracked and Cracked Elastic State Section Behaviour 24
3.3.1 ShortTerm Loads 25 3.3.2 Sustained Loads 26 3.3.3 Sustained and Variable Loads 31
3.4 Tension Chord Model 32 3.4.1 Basic Assumptions 32 3.4.2 Tensile Members 34
3.5 Summary 36
4 Tension Chord Model for Serviceability Problems 37
4.1 Tension Stiffening 37 4.1.1 ShortTerm 37 4.1.2 LongTerm 39 4.1.3 Unloading 41
4.2 Crack Width 42 4.2.1 Bending 43 4.2.2 Restrained Deformations 45 4.2.3 Imposed Deformations 53
4.3 Deflections 54 4.3.1 Interpolation Equations 56 4.3.2 Influence of Reinforcement Detailing 59 4.3.3 SpantoDepth Ratios 61
ii
4.4 Summary 62
5 Verification 65
5.1 Tensile Members 65 5.1.1 Loss of Tension Stiffening 65 5.1.2 Restrained Deformations 66 5.1.3 Imposed Deformations 70
5.2 Beams 73 5.2.1 Statically Determinate Beams 73 5.2.2 Statically Indeterminate Beams 97
5.3 Slabs 104 5.4 Summary 111
6 Discussion 113
6.1 Crack Width 113 6.1.1 Tensile Members 113 6.1.2 Bending Members 118
6.2 Deflections 120 6.2.1 Section Level 120 6.2.2 Member Level 124
6.3 Summary 127
7 Conclusions and Outlook 129
7.1 Conclusions 129 7.2 Outlook 130
Notation 131
Literature 135
Appendix A – Test Data Used in Chapter 5 141
Tensile Tests 141 Bending Tests 143
1
1 Introduction
1.1 Background
The Tension Chord Model (TCM) was developed within the framework of the research project Deformation Capacity of Structural Concrete that was carried out between 1992 and 2002 at the Institute of Structural Engineering (IBK, ETH Zurich) within the group led by Prof. Marti. Sigrist (1995) developed the Tension Chord Model for the purpose of determining the deformation capacity of plastic hinges in reinforced concrete (RC) bending members. Alvarez (1998) formulated the complete stressstrain relationship for a reinforced and prestressed tension tie under load and restraint. He applied the model to determine the amount of minimal reinforcement necessary for limiting crack widths and preventing brittle failure at first cracking. Kaufmann (1998) developed the Cracked Membrane Model based on the basic principles of the Tension Chord Model. Fürst (2001) used the Tension Chord Model to discuss the behaviour of prestressed tension ties subjected to loading cycles, drawing conclusions concerning fatigue. Kenel (2002) implemented fracture mechanics aspects into the model. Pfyl (2003) combined the Tension Chord Model with the Fibre Effectiveness Model in order to describe the deformation behaviour of tensile and bending members made of steel fibre reinforced concrete and steel reinforcing bars. Thoma (2004) developed a stochastic model for prestressed tensile ties based on the Tension Chord Model. Heinzmann (Heinzmann 2006) incorporated the influence of selfequilibrating stresses due to shrinkage. The steel strains and integral deformations predicted by the Tension Chord Model show a good agreement with the measured values obtained in large scale tests (Sigrist 1995; Alvarez 1998; Kenel 2002).
1.2 Aims
Following up on the previous work outlined above, the present thesis was initiated with the aim of verifying the applicability of the Tension Chord Model for serviceability design. The work was carried out with the following goals:
1. to discuss and extend the Tension Chord Model crack width and deformation approach for tensile and bending members under shortterm and sustained service loads.
2. to validate the resulting approach with test data from short and longterm tensile and bending tests from various research institutes.
3. to compare the resulting approach with other crack width and deflection equations.
4. to evaluate the decisive input parameters for serviceability limit state predictions.
1.3 Research Significance
Due to the requirements for modern buildings concerning aesthetics, functionality and durability a number of deformationsensitive solutions such as hightech cladding, exposed concrete and white
Introduction
2
tank waterproofing (see Fig. 1.1) are becoming increasingly popular. At the same time, demanding cost and construction time limitations, paired with a constant increase in material strengths, favour slender, monolithically connected members with rapid construction schedules, which all together result in less favourable conditions for serviceability.
As a consequence, serviceability design is becoming an increasingly important aspect of building construction. Regardless of this tendency most codes still treat serviceability as a secondary issue (Beeby 1999) and their prediction models differ considerably (see Chapter 2). The Tension Chord Model represents a consistent tool for modelling both the cracking and deformation behaviour of tension ties and oneway bending members.
costsdeadlines
materialscienceutilisation
sensitivecladdings
exposedconcrete
monolithicconstruction
shortconstruction
restraint higherstress levels
earlyageloading
more demanding circumstancesstricter requirements
durabilityaesthetics
for serviceability design for serviceability design
waterproofconcrete periods
slendermembers
Fig. 1.1 Significance of Serviceability Design.
1.4 Overview
Chapter 2 of this work summarizes the predominant crack width and deflection prediction approaches. The first part of the chapter discusses the basic principles behind the slippingbond and concretecover crack width approaches. The second part of the chapter provides an overview of the most wellknown tension stiffening and deflection prediction approaches for bending members.
Chapter 3 contains the basic principles used for the crack width and deflection approaches provided in Chapter 4. The chapter is divided into four parts. The first part discusses the concrete material parameters relevant for serviceability. The second part on reinforcement behaviour is very short, because elastic steel behaviour is assumed under service loads. The third part deals with different approaches for quantifying the State I and II section behaviour under sustained moments. Finally, the fourth part of the chapter illustrates the basic principles and assumptions behind the Tension Chord Model.
Chapter 4 is one of the two core chapters of this work. The first part of the chapter deals with tension stiffening in bending members, under sustained loads and during unloading. The second and
Limitations
3
third parts contain a selection of consistent crack width and deflection prediction equations, derived based on the State I and II deformation behaviour combined with the Tension Chord Model.
Chapter 5 is the second core chapter of this work. A selection of test series from various research institutions is used to validate the serviceability approaches described in Chapter 4. The first part of the chapter contains three series of small tensile elements with sustained axial loads, eight shrinkage specimens and a selection of deformationcontrolled tensile tests. The second part contains three series of fourpoint bending tests (two of them with sustained loads), a series of simple beams under sustained uniformly distributed loads, the two ConCrack fourpoint bending tests and three series of twospan beams. The last part of the chapter contains four experimental campaigns with simply supported slabs as well as corner, edge and internal flatslab panels under sustained loads.
Chapter 6 contains a discussion involving parameter studies carried out for the Tension Chord Model crack and deflection equations (Chapter 4), as well as comparisons with the models discussed in Chapter 2.
Overall conclusions are provided in Chapter 7.
1.5 Limitations
The present work is limited to steel reinforced concrete tension ties and tension chords in oneway bending members with uniaxial stress states. The crosssections are rectangular and the material behaviour is assumed elastic. Second order effects, shear deformations, nonlinear creep and differential shrinkage/temperature effects are not considered. When not stated otherwise, average material properties are used. Cyclic loading is not considered.
5
2 State of the Art
The two main concerns of serviceability design of reinforced concrete (RC) structures consist in limiting crack widths and deflections. This chapter summarizes the most wellknown approaches currently used for these purposes. Section 2.1 discusses the basic principles behind the crack width prediction equations based on the slippingbond approach and the concretecover approach. Section 2.2 summarizes the most used approaches for considering tension stiffening at section level for the purpose of determining deflections at member level.
2.1 Crack Width
In a cracked tension chord the strain difference between the ductile steel (with service strains up to 2 ‰) and the brittle concrete (with tensile strains below 0.1 ‰) is absorbed by the cracks. The transfer length l0 (also referred to as transmission length) defines the straindifference gathering length belonging to each crack, which corresponds to the length on each side of a crack, which is affected by the crack. Since the concrete surface stresses are reduced within the transfer length, new cracks form outside the transfer length, leading to a final crack spacing sr between once and twice the transfer length (Base et al. 1966; Broms 1965). The corresponding crack widths are
dxr
s c r sm cmsw s (2.1)
Under shortterm loads the strain in the concrete is small and often ignored. There are different approaches for determining the transfer length l0 and the development of the steel (and concrete) strains on either side of the crack. Both depend on the model used to describe the load transfer between the steel and the concrete through mechanical interlock.
Besides the purely empirical crack width equations (e.g. Gergely and Lutz 1968) there are two main approaches for modelling the load transfer between the steel and concrete and accommodating the strain incompatibility. The first approach based on Saliger (1936), Kuuskoski (1950) and Rehm (1961) assumes a slipping bond at the interface between the two materials. In this case the transfer length is defined as the length necessary to introduce the force Fc = fct Ac into the concrete and depends on the bond stress, the reinforcement ratio and the bar diameter. The second approach based on Base et al. (1966) and Broms (1965) assumes a transfer length defined by the concrete cover. The traditional (Continental) European code equations are based on the former, while the bar spacing limit in ACI 318 (2008) is derived from the latter approach. A comprehensive summary of the individual crack width equations is given in Borosnyói and Balázs (2005).
2.1.1 SlippingBond Approach
The slippingbond approach models the load transfer between the steel and the concrete with fictitious bond stresses at the interface between the two materials. The strain incompatibility is accommodated by slip (relative displacement between steel and concrete). The distribution of bond stresses on either side of the cracks was initially assumed to be a function of the ultimate bond stress (Con
State of the Art
6
sidère 1902; Saliger 1936) and later determined from the differential equation of slipping bond (Kuuskoski 1950; Rehm 1961). In the first case (Saliger 1936) the transfer length
0,max
ct
b
fl k
(2.2)
is defined by the ratio of tensile and bond strength and the assumed bond stress distribution factor k. In the second case, the slip (x) and shear stress b(x) distributions on either side of a crack are obtained by solving the differential equation of slipping bond
2
2
4 1 1
1b
s
nd
Edx
(2.3)
for a given bond stress  slip relationship, e.g.
b C (2.4)
Eq. (2.4) leads to analytical solutions for initial cracking (0 < (Noakowski 1985; Balázs 1993) and the limiting cases of = 0 and 1 (e.g. Rehm 1961). More complex bond stress – slip relationships usually require numerical solutions. The reinforcement ratio refers to As/(bh) for uniformly reinforced tension ties and As/(bhef) for tension chords in bending elements. The tensile concrete stresses are assumed to be uniformly distributed over the tension chord, implying plane concrete sections and leading to equal crack widths from the bar to the concrete surface.
Analytical crack width approaches based on Eq. (2.3) usually adopt Eq. (2.4) with = 0 and an average bond stress C = b (Watstein and Parsons 1943; Bachmann 1967; König and Fehling 1988; Sigrist 1995; Alvarez 1998; Marti et al. 1998). This solution also provides the basis for the Model Code 1990 (Comité EuroInternational du Béton 1993), Model Code 2010 (Fédération Internationale du Béton 2010b) and Eurocode 2 (Part 1) (European Committee for Standardization 2004) transfer length
0 1 22 2ct
b
fcl
(2.5)
and load crack width
,IImax 0 3 4
12 s ct
shs s
f nw l
E E
(2.6)
as well as for the Eurocode 2 (Part 3) (European Committee for Standardization 2011) end restraint crack width equation
max 0
12
2ct
cs
f nw l k k
E
(2.7)
The code equations differ from the strictly analytical solution (1 = 0, 2 = 3 = 0.5, 4 = 0/1, kc = k = 1) in an attempt to incorporate the influence of cover, curvature, different bond conditions and shrinkage strains. Eurocode 2 (EC 2) suggests 1 = 3.4, 2 ≈ 0.61/0.30 (tension/bending for b = 1.8 fct), 3 = 0.6/0.4 (short/longterm), 4 = 0, k = 1/0.65 (h ≤ 300 mm/h ≥ 800 mm) and kc = 0.5...1 (1 for pure tension). Model Code 2010 (MC 2010) adopts 1 = 0, 2 = 0.5, 3 = 0.6/0.4 (short/longterm) and 4 = 0/1 and additionally provides a multiplier for large concrete covers. Except for longterm loading during the crack formation phase, the bond stress b = 1.8 fct.
Crack Width
7
Both codes use Schiessl's (1989) effective reinforcement ratio
II
3
2.5s s
ef
A A
b h d b h x
(2.8)
for RC bending elements.
2.1.2 ConcreteCover Approach
In this case the transfer length is defined by the controlling concrete cover. Broms (1965) distinguishes between internal and visible cracks and uses load spreading circles inscribed between two neighbouring cracks to check if a new intermediate crack in a onebar tensile tie (Fig. 2.1 (a – c)) reaches the concrete surface or not. He considers a new crack short enough to remain invisible if it forms between cracks spaced closer than sr = 2 (c + /2) (Fig. 2.1 (b)), making
0 2l c
(2.9)
the transfer length for visible cracks in circular singlebar tension ties. Similarly, for their so called "nonslip" approach, Base et al. (1966) use an elastic theory solution to show that a length approximately equal to the concrete cover c is necessary to distribute concentrated tensile stresses to the concrete surface in a onebar tensile tie. They consider the sum of the microcrack widths at the steelconcrete interface to amount to similar values as the sum of the surface crack widths. Neither approach considers if the concrete tensile stresses that reach the member surface are large enough to cause cracking.
crack
2
CL
c
crack CL crack CL
(a)
crack CLcrack CL crack CL
(b) (c)
(d) (e) (f)
Ø+
c Ø+ 2 2c Ø+c Ø+ 42
Fig. 2.1 Circular singlebar tensile tie between two cracks illustrating Broms' (1965) load spreading circlesand the corresponding strut and tie models.
For a multiplebar tension chord Broms assumes that the local cracks at each reinforcement bar join and reach the surface if they occur between two existing cracks, which are spaced at a distance larger than the bar spacing and larger than twice the transfer length according to Eq. (2.9). He suggests a
State of the Art
8
visible crack spacing between once and twice the transfer length of a single bar and an average (not maximum) surface crack width equal to
,II2 2avg sw c
(2.10)
Based on their theoretical consideration and on test data comparisons Base et al. suggest a maximal crack width
IImax ,II
II
3.3 s
h xw c
d x
(2.11)
corresponding to a maximal crack spacing of 3.3 c.
000
max
00000
w
200 300 400 500 600
[MPa]σs,II
[mm
]
0.2
0.4
0.6
0.8
1.0
0
1000
250 16
MC 2010
Frosch
250
0α =10.5α =2
EC 23.4α =10.3α =2
(a)
Ø
200 300 400 500 600
[MPa]σs,II
1000
10
Frosch
100
EC 23.4α =10.3α =
Ø
MC 20100α =10.5α =2
250
2
(b)
16Ø 10Ø
Fig. 2.2 Maximum crack widths according to Frosch's Eqs. (2.12) and (2.13) and the EC 2 and MC 2010versions of Eqs. (2.6) and (2.5) with 3 = 0.6, 4 = 0 and b = 1.8 fct: (a) 16 mm @ 250 mm ( =0.4 %.); (b) 10 mm @ 100 mm ( = 0.5 %.). Note that fct = 2 MPa, n = 6, Es = 205 GPa, c = 30mm. The dimensions are in [mm].
The current (since the 2005 edition) ACI 318 (ACI Committee 318 2008) maximal bar spacing for crack width limitation is derived from Frosch's (1999) bottom face maximum crack width equation
,II IImax 0
II
2 s
s
h xw l
E d x
(2.12)
which is directly based on Eq. (2.10) with a bottom face transfer length
2 2
0 2 2b
sl c
(2.13)
This bottom face transfer length corresponds to the maximum distance between a point on the bottom beam face and the centre of the nearest reinforcing bar (controlling concrete cover), which increases with increasing bar spacing s. For bottom fibre side crack widths Frosch (1999) suggests a transfer length of
2 2
0 2 2b sl c c
(2.14)
Deflections
9
Fig. 2.2 illustrates Frosch's Eqs. (2.12) and (2.13) together with the EC 2 and MC 2010 versions of Eqs. (2.6) and (2.5). Despite the additional cover term, the EC 2 version (1 = 3.4, 2 = 0.3) predicts lower maximum crack widths than the original MC 2010 version (1 = 0, 2 = 0.5).
2.2 Deflections
The general way to determine deflections of beams and oneway slab strips is to integrate the curvatures determined at each section (x), by applying the principle of virtual work
0
dl
a x M x x (2.15)
By this means axial forces and variable stiffnesses (e.g. due to cracking or curtailed reinforcement) can be considered and longterm effects and tension stiffening can be dealt with at section level.
h
M
Δχts
q
l
χMr
2x
χχII
x( )
x( )
I
χII
Fig. 2.3 Schematic illustration of the moment and curvature distributions in a partially cracked beam.
2.2.1 Section Level
The two most used models for incorporating tension stiffening at section level in bending elements were developed in the 1960's by Branson and Rao. Branson (see Branson 1977) empirically derived an effective moment of inertia
I II1m m
r ref
M MI I I
M M
(2.16)
used with m = 4 for considering tension stiffening at section level. Reference is given to his book (Branson 1977) because the author does not hold the original paper (Branson 1963). Eq. (2.16) can be rearranged to
II
4IIII I II
1tscmr
I M
E II M M I I
(2.17)
State of the Art
10
Rao (1966) derived the semiempirical expression
,II,
,II
0.18s r ctts
s s
f
E
(2.18)
for the average steel strain reduction due to tension stiffening in cracked flexural elements subjected to pure bending. According to Mourachev (Mourachev et al. 1971), the quotient in the brackets corresponds to the empirical tension stiffening factor found by Nemirovsky (1949) [not cited, as the original publication is not available]. The second part of the equation, as shown by Rostásy et al. (1976), who extended the equation to other load cases, corresponds to the sudden increase in steel strains upon cracking.
Rao's tension stiffening factor is implicitly included in the EC 2 (2004) and the MC (2010b) interpolation equation
2 2
,II, ,II,I II
,II ,II
1s r s r
s s
(2.19)
For pure bending elements (s,II,r/s,II) can be replaced with (Mr/M) and Eq. (2.19) can be rearranged to
II I
r r rts
cm cm
M M M
M E I E I
(2.20)
Factor is equal to and for shortterm and longterm/cyclic loading, respectivelyFig. 2.4 compares Branson's and Rao's equations. The agreement between the models depends on the load level and reinforcement ratio.
0
0.2
0.4
0.6
0.8
1.0
χ Δts
0031.5 2 2.51
0
χ II
MrM
Rao 1β =
Branson 4m =
0.2 %ρ =
31.5 2 2.51
1.0 %ρ =
Branson 4m =
Rao 1β =
(a) (b)
MrM
Fig. 2.4 Related tension stiffening curvature reductions according to Branson with Eq. (2.17) and Rao withEq. (2.20): (a) = 0.2 %; (b) = 1.0 %. Note that ' = 0, d/h = 0.85 and n = 6. The curves are cutoff at M = My.
Deflections
11
2.2.2 Member Level
In order to avoid curvature integrations as in Eq. (2.15), global stiffness
I II1ef I II I I (2.21)
or global deflection
I II1a aa a a (2.22)
interpolation coefficients I ora can be used. Besides tension stiffening, these have to account for a nonuniform stiffness (cracked and uncracked regions).
Branson (1977) suggested the same interpolation coefficient he derived at section level (Eq. (2.16)) to be used at member level, but with a power m = 3. This equation is given in ACI 318 (2008) together with a global multiplier (Branson 1971) for longterm effects, leading to
2
11 50
a
ef c
kM la
I E
(2.23)
where depends on the load duration and k is the integration factor.
EC 2 and MC 2010 both refer to the direct interpolation of deflections with the same interpolation coefficient
2
ra
a
M
M
(2.24)
used for curvatures (Eq. (2.19)) as the simplest method of deflection prediction. For sustained loads they use the effective modulus method (see Eq. (3.65)) with a shrinkage curvature equation (Trost and Mainz 1968).
method variable stiffness tension stiffening creep & shrinkage
ACI 31808
3
rI
a
M
M
implicit 01 50ta a
EC 2
MC 2010
2
ra
a
M
M
implicit
,
st sh ef
ef c ef ef
M Sn
I E I
Bilinear Method
ra
a
M
M
implicit 0
sht shk k
d
MC 90 simplified
3
1 20g
ha a
d
implicit creep implicit
Table 2.1 Global deflection prediction approaches for pure bending.
The bilinear method (Favre et al. 1981) interpolates the deflections with a lower power version
ra
a
M
M
(2.25)
of Rao's section level interpolation coefficient (due to the integration) and uses Trost and Mainz' (1968) interpolation coefficients (see Chapter 3.3.2) to account for longterm effects. The MC 90
State of the Art
12
(Comité EuroInternational du Béton 1993) deflection equation is a simplified version of the bilinear method. Table 2.1 gives an overview of the global deflection approaches at member level.
2.3 Summary
This chapter gives an overview of the mostused crack width and deflection equations.
For determining the crack spacing Model Code and Eurocode suggest Eq. (2.5), which is a modified version of the slippingbond transfer length. The ACI Building Code Requirements for Structural Concrete implicitly use Eq. (2.13), which is based on Broms's load spreading circles.
For considering the influence of tension stiffening at section level Model Code and Eurocode suggest Rao's Eq. (2.20), while the ACI Building Code Requirements for Structural Concrete suggest Branson's Eq. (2.17). At cracking both approaches provide curvature reductions equal to the full difference between the State I and II curvature, which are then reduced towards zero with increasing load levels. However, between these two points, especially for low reinforcement ratios, the two approaches differ (see Fig. 2.4).
For determining the global deflections of partially cracked beams Model Code and Eurocode interpolate the deflections with Eq. (2.22)), while the ACI Building Code Requirements for Structural Concrete interpolate the stiffnesses with Eq. (2.21). The interpolation coefficients are given in Table 2.1. Tension stiffening is considered implicitly within the interpolation.
13
3 Basic Principles
The first two sections of this chapter summarize the concrete (Section 3.1) and steel (Section 3.2) material behaviour required for short and longterm serviceability design. The next two sections contain the two basic approaches combined in Chapter 4 to form the short and longterm crack width and deflection equations. The first approach (Section 3.3) describes the short and longterm section behaviour in bending of uncracked (State I) and cracked (State II, fct = 0) sections. The second approach refers to the Tension Chord Model used to model the interaction between steel and concrete between the cracks in cracked tension chords (Section 3.4). A summary of the chapter is given in Section 3.5.
3.1 Concrete Material Behaviour
Traditionally, the average 28day concrete compressive strength is used to describe all other concrete properties. It is usually obtained from tests on 300 mm tall, 150 mm diameter cylinders (fcm) or cubes with 150 mm side lengths. Mainly due to the smaller aspect ratio, the latter is slightly larger (fcm,cube ≈ 1.25 fcm). The current European code equations use the characteristic (5% fractile) cylindrical compressive strength
28 [N/mm ]ck cmf f (3.1)
while the ACI codes refer to the specified cylindrical compressive strength fc', which is an average
value.
The cement classes S, N and R refer to slow, normal and rapid strength development rates. According to the EN 197 (European Committee for Standardization 2000) classification, S includes CEM 32.5N (fc,7d ≥ 16 MPa), N includes CEM 32.5R and 42.5N (fc,2d ≥ 10 MPa) and R includes CEM 42.5R and 52.5N (fc,2d ≥ 20 MPa and 30 MPa) as well as 52.5R (fc,2d ≥ 30 MPa).
3.1.1 ShortTerm
Under service conditions it is common praxis to assume linear elastic material behaviour to describe the instantaneous deformations
00
0
cc
c
tt
E t
(3.2)
in tension and compression. Alternatively, Sargin's (1971) stressstrain relationship
2
with and 1 2
c c cuc cm
cu cm
k Ef k
k f
(3.3)
in [‰ and MPa] describes the shortterm behaviour of concrete in compression below the compressive strength, where the failure strains are approximately
Basic Principles
14
1
30.6 [in ‰ and MPa]cu cmf (3.4)
The concrete tensile strength is a decisive parameter for serviceability design. Besides defining the cracking loads, the concrete tensile strength also influences the deformation behaviour of cracked tension chords. Most current (European) cracking models are based on the average direct tensile strength, which requires a demanding test setup. This is why the tensile strength is often obtained from splitting tensile tests, where
,0.7...1.0ct ct spf f (3.5)
or flexural tensile tests, where
0.7
,0.7
1.5 100 mm
1 100 mmct ct fl
hf f
h
(3.6)
As indicated in Eq. (3.2), the stresses, strains and material properties in Eqs. (3.2) to (3.6) apply to the concrete age t0 when the stress is applied. In the absence of material tests, the average 28day elastic modulus (Fédération Internationale du Béton 2010a)
1/3
0 [ in MPa]10
cmc E cm
fE E f
(3.7)
and the average direct tensile strength
2/30.3 [in MPa]ct ckf f (3.8)
can be determined from the 28day compressive strength. E0 = 21.5GPa and E = 0.7 to 1.2 (1 for quartzite aggregates). The compressive strength
cm cmf t t f (3.9)
and elastic modulus
m
c cE t t E (3.10)
at loading ages other than 28 days can be estimated with the time factor
28exp 1t
t
(3.11)
where = [0.38/0.25/0.20] for cement types [S/N/R] and m is between 0.5 (Fédération Internationale du Béton 2010a) and 1 (European Committee for Standardization 2004). Eq. (3.11) is not usually used for the concrete tensile strength because its development is sensitive to many hardtoquantify parameters.
3.1.2 LongTerm
The concrete strains under sustained loads increase due to creep, while the concrete stresses under sustained deformations decrease due to relaxation. Further concrete shrinks due to loss of water and cement hydration. For service compressive stresses below approximately 0.4 fcm it is common practice to treat concrete as an aging, linear viscoelastic material where the strain at time t
Concrete Material Behaviour
15
0 0,ct t J t t (3.12)
due to a sustained stress applied at t0 is defined by the compliance function J (t, t0). Accordingly the stress at time t
0 0,c ct t R t t (3.13)
due to a sustained strain applied at t0 is defined by the relaxation function R (t, t0). The compliance function is either determined experimentally or with empirical expressions for (t, t0) (see Section "Creep Coefficient" below) according to
0 00
0 0
1 , ,1, or
c c c
t t t tJ t t
E t E t E
(3.14)
depending on whether (t, t0) is related to the elastic modulus at the age of loading or at 28 d. As relaxation tests are not feasible, the relaxation function is derived from the compliance function, making use of the fact that the two functions are related mathematically (see Section "Aging Coefficient" below).
According to Boltzmann's (1874) principle of superposition for viscoelastic materials, strains due to stresses applied either suddenly at t0 or gradually over a period of time between t0 and t, as well as shrinkage or temperatureinduced strains (ci) can be determined individually and added together. Assuming the first definition of given in Eq. (3.14)
0
00 0
0
1 , 1 , d ,
tc
c c cic ct
t t tdt t t
E t d E
(3.15)
In practice gradual concrete stress variations occur e.g. due to internal stress redistributions between the steel and concrete caused by creep and shrinkage. By introducing the aging coefficient (Trost 1967) and assuming Ec () = Ec (t0), the integral term in Eq. (3.15) can be simplified according to
0 00 0
0 0
1 , 1 ,,c c c ci
c c
t t t tt t t t
E t E t
(3.16)
The aging coefficient takes into account that c (t) = c (t) – c (t0) is applied gradually to an aging concrete.
Eq. (3.16) leads to
0
0 , 0 00
1 ,,c c c a c c ci
c
t tt t E t t t
E t
(3.17)
where
0
,01 ,
cc a
E tE
t t
(3.18)
denotes the ageadjusted effective modulus. Eqs. (3.17) and (3.18) belong to the ageadjusted effective modulus method (AAEMM), named this way by Bažant (1972), because he found the aging coefficient to be strongly dependent on the age of the concrete when the load is applied. The input parameters of Eqs. (3.17) and (3.18) are the temperature and shrinkageinduced strains ci ci (t, t0), the creep coefficient (t, t0) and the aging coefficient . The free shrinkage strains sh, the creep coefficient and the aging coefficient are discussed in the following three sections.
Basic Principles
16
Free Shrinkage Strains
It is usually assumed that the total free shrinkage strains are composed of drying sh,d (loss of water) and autogenous sh,a (cement hydration) shrinkage strains. The total and autogenous shrinkage strains can be determined experimentally. If the shrinkage specimens are not the same size as the corresponding concrete member, the size dependent development rate of the drying shrinkage strains needs to be taken into account, for example with Eq. (3.21) given below.
There are a wide range of empirical shrinkage equations
, , ,, ,sh s s sh d sh at t t t t (3.19)
for estimating the shrinkage strains. They usually contain a drying shrinkage term composed of a final value and a time function (first term) and in some cases an autogenous shrinkage term (second term). The shrinkage equations are based on the concrete compressive strength even though shrinkage is only indirectly related to the compressive strength over the watertocement ratio, which directly influences both the drying (water) and autogenous (cement) shrinkage. A selection of shrinkage equations is given here and illustrated in Fig. 3.1. When not stated otherwise, the input variables are to be inserted in the following units: the relative humidity RH as a percentage, the notional size of the member h0 = 2·V/S = 2Ac/u in [mm], the concrete properties fcm and Ec in [MPa], the shrinkage duration t–ts in [d] and the end of curing (= beginning of shrinkage) ts in [d]. The equation versions given here apply to a relative humidity (RH) between approximately 0.4 and 0.9. V/S stands for the volume to surface ratio.
CEB Model:
The original CEB shrinkage approach (version MC 90) was developed by Task Group 9 (Müller and Hilsdorf 1990) especially for Model Code 90 (Comité EuroInternational du Béton 1993). The approach contains a final drying shrinkage value of
6 3, , 1.55 10 1 RH 160 10 9 0.1sh d cmf
(3.20)
with = [4/5/8] for [S/N/R] cement and a time factor
0.5
20
,0.035
ss
s
t tt t
h t t
(3.21)
For the current fib (Fédération Internationale du Béton 1999; 2010a) approach (version MC 2010), an autogenous shrinkage term
2.5
6 0.2,
0.110 1
6 0.1tcm
sh a ascm
ft e
f
(3.22)
and additional factors for considering the cement type in the drying shrinkage term
26 3, , 11.55 10 1 RH 220 110 cm dsf
sh d ds e (3.23)
were added. Factors [as/ds1/ds2] are equal to [800/3/0.013] for S type cement, [700/4/0.012] for N type cement and [600/6/0.012] for R type cement.
The EC 2 (European Committee for Standardization 2004) shrinkage equation includes a reduction factor 0.85 kh for the final drying shrinkage strains
26 3, , 11.55 10 1 RH 220 110 0.85cm dsf
sh d ds he k (3.24)
Concrete Material Behaviour
17
and uses a different power of h0 in the time factor
0.5
1.50
,0.04
ss
s
t tt t
h t t
(3.25)
as well as a slightly simpler expression for the autogenous shrinkage strains
6 0.2, 2.5 10 10 1 t
sh a ckt f e (3.26)
The type of cement is considered with the coefficients ds1 and ds2 defined above. Factor kh = [1/0.85/0.75/0.7] considers the notional sizes h0 = [100/200/300/≥500 mm].
ACI 209:
The ACI (ACI Committee 209 1992) shrinkage strains consider the experimentally determined final shrinkage value sh,∞ = 780 106 and time factor (Branson and Christiason 1971)
,35
ss
s
t tt t
t t
(3.27)
for standard conditions (RH = 0.4 and havg = 150 mm). For nonstandard conditions 150 mm ≤ havg ≤ 300 mm empirical correction factors apply, leading to
,
1.23 0.00150 for 360 d, , 1.4 RH
1.17 0.00114 for 360 d
avg s
sh s sh s
avg s
h t tt t t t
h t t
(3.28)
According to Branson and Christiason (1971), the empirical correction factors were derived by Christiason in his MS thesis in 1970.
GL 2000 Model:
Gardner and Lockman's (2001) model considers final shrinkage strains
6 4,
301000 10 1 1.18 RHsh
cmf
(3.29)
and the CEB time factor
0.5
2,
0.15
ss
s
t tt t
V S t t
(3.30)
with V/S instead of h0. The model was derived with test specimens with h0 < 38 mm. Factor is equal to [1/0.7/1.15] for ASTM C150 (American Society for Testing and Materials 2011) Portland cement types [I/II/III], where type I is a general purpose cement with fc,3d = 12 MPa, type II features a moderate sulphate resistance with fc,3d = 10 MPa and type III is characterized by a relatively high early strength with fc,3d = 24 MPa.
Basic Principles
18
Full B3 Model:
The most complex shrinkage equation (Bažant and Baweja 1995) does not explicitly consider autogenous shrinkage. It considers final shrinkage strains
0.5
6 2 2.1 0.28 3, 1 2
607 4 0.8510 1.9 10 270 1 RH
4 0.85 607s sh
sh cms sh
tw f
t
(3.31)
and the time factor
, tanh s
ssh
t tt t
(3.32)
with
20.08 0.2508.5sh s cm st f k h (3.33)
Factor 1 = [1/0.85/1.1] for cement types [I/II/III], factor 2 = [0.75/1.2/1] for curing conditions steam/normal/RH 100% and factor ks = [1; 1.15; 1.25; 1.3; 1.55] for an [infinite slab; infinite cylinder; infinite square; prism; cube]. w is the water content in [kg/m3] and h0 in [cm].
0
0.2
0.4
0.6
0.8
1.0
ε
0010001
010 100
[d]tts
sh[
]
10000 100000
80 years
MC 90MC 2010
EC 2
ACI 209
GL 2000
B3
Fig. 3.1 Predicted free shrinkage strains for a 320 mm thick slab strip (havg = h0 = 2·V/S = 320 mm) madeof C25/35 concrete with fcm = 33 MPa (fck = 25 MPa). The slab strip is located in a RH = 40 %ambient and moist cured for ts = 7 days. Further a class N, type I cement and a water content of150 kg/m3 are assumed.
Fig. 3.1 illustrates the shrinkage equations for a 320 mm thick slab strip made from normal strength concrete. The difference between the MC 90 and MC 2010 curves illustrates the influence of the autogenous shrinkage term. Extensive test data comparisons carried out by Gardner (2004) for all four models show that the CEB (version MC 2010), B3 and GL2000 models underestimate on average the measured values, while the ACI 209 model underestimates again at earlyages, is neutral or overestimates at durations below 1000 days and underestimates at later durations. For shrinkage predictions based solely on the concrete tensile strength, Gardner (2004) found variation coefficients between 25 % (GL 2000) and 34 % (ACI 209). For shrinkage durations above 3000 days the variation coefficients dropped to values between 15 % (GL 2000) and 30 % (ACI 209). This coincides with Müller and Hilsdorf (1990) who evaluated a variance coefficient for the CEB model equal to 33% for general and 19 % for final shrinkage predictions.
Concrete Material Behaviour
19
Creep Coefficient
If the compliance function is determined experimentally from length measurements on creep specimens, the creep coefficient results from
0 0, 1cE t J t t (3.34)
or
00
, cc
c
EE J t t
E t (3.35)
depending on its definition. ACI 209 (1992) and the B3 model (Bažant and Baweja 1995) adopt Eq. (3.34), while the CEB (Comité EuroInternational du Béton 1993; Fédération Internationale du Béton 1999; European Committee for Standardization 2004; Fédération Internationale du Béton 2010a) and GL 2000 (Gardner and Lockman 2001) models adopt Eq. (3.35).
Similar to the shrinkage strains, there is a wide range of empirical creep prediction equations. The most wellknown expressions are summarized here and illustrated in Fig. 3.2. When not stated otherwise, the input variables are to be inserted in the following units: the relative humidity RH as a percentage, the notional size of the member h0 = 2·V/S = 2Ac/u in [mm], the concrete properties fcm and Ec in [MPa] and t and t0 in [d].
CEB model:
The CEB creep coefficient
0,t t (3.36)
was developed by Task Group 9 (Müller and Hilsdorf 1990) especially for MC 90 (Comité EuroInternational du Béton 1993) and consists of a final creep coefficient
2
1 0.230 0
16.8 1 RH1
0.1 0.1cmh f t
(3.37)
and a time factor
0.3
00
0
,H
t tt t
t t
(3.38)
where
18
0 3 31.5 1 1.2 RH 250 1500H h (3.39)
The factors
0.7 0.2 0.5
1 2 335 ; 35 ; 35cm cm cmf f f (3.40)
considering the concrete strength were added for the current fib (Fédération Internationale du Béton 2010a; Fédération Internationale du Béton 1999) and EC 2 (European Committee for Standardization 2004) versions (they are equal to 1 in the MC 90 version).
ACI 209 Model:
The ACI (ACI Committee 209 1992) creep coefficient (Eq. (3.34)) is based on an experimentally determined (Branson and Christiason 1971) final creep coefficient ∞ = 2.35 and a time factor
Basic Principles
20
0.6
00 0.6
0
,10
t tt t
t t
(3.41)
for standard conditions (t0 = 7d, RH = 0.4 and havg = 150 mm). For nonstandard conditions empirical correction factors apply, leading to
00.1180 0
0
1.14 0.00092 for 360 d , 1.25 1.27 0.67 RH
1.10 0.00067 for 360 d
avg
avg
h t tt t t
h t t
(3.42)
According to Branson and Christiason (1971) the empirical correction factors were derived by Christiason in his MS thesis. The havg correction factor is valid for havg between 150 and 380 mm.
GL 2000 Model:
Gardner and Lockman's (2001) creep coefficient considers basic and drying creep
0.50.50.3
0 0 020.3 2
0 0 0 00
2 72.5 1 1.086 RH
7 0.1514
t t t t t t
t t t t t t V St t
(3.43)
and accounts for drying before loading (if t0 ≥ ts) with the factor
0.50.5
02
0
10.15
s
s
t t
t t V S
(3.44)
Full B3 Model:
Bažant and Baweja's (1995) creep coefficient results with Eq. (3.34) from the compliance function
0 1 0 0, , , ,basic drying sJ t t J t t J t t t (3.45)
The compliance function considers instantaneous strain 1 due to a unit stress (determined with the asymptotic modulus), the theoretical basic creep compliance
0.1
2 3 0 40
ln 1 lnbasic
tJ Q t t
t
(3.46)
and the drying creep compliance (if t0 ≥ ts)
0
0.60.5, 8 87.57 ssh H t H t
dryingcm
J e ef
(3.47)
Q stands for a binominal integral, approximated by
0.12 0.12
0 0
1
1.7 8 1.7 812/9 4/91 0 02/9 4/9
0 0 0.10.50 0
0.086 1.21 0.086 1.21 1
ln 1
t t
t tQ t t
t t t
(3.48)
Concrete Material Behaviour
21
The additional empirical factors are
4 0.760.9
1 2 3 2 4
0.6 10185.4 0.29 20.3cm
c
w ac f
E c c
(3.49)
and
20.08 0.25
0
1 1 tanh8.5
s
s cm s
t tH t RH
t f k h
(3.50)
The input variables are inserted in the following units: h0 in [cm], water and cement content w and c in [kg/m3], water to cement ratio w/c in [] and aggregate to cement (weight) ratio a/c (e.g. 7) in []. Time t0s in [d] is the major of t0 (concrete age at loading) and ts (concrete age at end of curing). The shrinkage parameters sh,∞ (Eq. (3.31)) and ks are defined in the shrinkage section above.
Fig. 3.2 illustrates the different creep equations. So they can be compared, the creep coefficients based on Eq. (3.35) are multiplied with Ec (t0)/ Ec. The kink in the ACI 209 curve is caused by the change in Eq. (3.42) at t – t0 = 360 days. The same test comparison referred to above for shrinkage (Gardner (2004)) contains compliance comparisons illustrating variation coefficients between 26 % (GL 2000) and 37 % (CEB) for test data comparisons based solely on the measured concrete compression strength. All four models have a tendency to underestimate the creep compliance (especially the ACI 209 model). Müller and Hilsdorf (Müller and Hilsdorf 1990) found a 20 % variation coefficient for the CEB model.
0
ϕ
0010001
010 100
[d]tt0
10000 100000
80 years
MC 90
0
4
3
2
1
MC 2010
ACI 209
GL 2000B3
& EC 2
Fig. 3.2 Creep coefficients for a 320 mm thick slab strip (havg = h0 = 2·V/S = 320 mm) made of C25/35concrete with fcm = 33 MPa and Ecm = 32 GPa. The slab strip is located in a RH = 40 % ambientand loaded at t0 = 7 days. For the B3 model a type I cement with w = 150 kg/m3, w/c = 0.5 anda/c = 7 is assumed.
Aging Coefficient
Inserting c (t0) = c Ec (t0) (Eq. (3.2)) and c (t) = c R (t, t0) (Eq. (3.13)) into Eq. (3.16) with c (t) = c (t) – c (t0) and solving for (Ghali and Favre 1986) leads to
0
0 0 0
1
, ,c
c
E t
E t R t t t t
(3.51)
Basic Principles
22
where R(t, t0) is the relaxation function, defined as the stress at age t due to a unit strain introduced at age t0. This means that the aging coefficient can be determined from the relaxation function. The relaxation function is obtained by numerically solving the Volterra Integral
0
00 0 0
,, , dt 1
t
c
t
R t tE t J t t J t t
t
(3.52)
which mathematically links the relaxation and compliance functions and is derived by inserting c (t) = c R (t, t0) into Eq. (3.15) and dividing by c.
Ghali & Favre (1986) provide a stepbystep analysis to numerically determine R(t, t0) according to Eq. (3.52). They divide the time period between t0 to t of a given timestress function into i intervals and apply the stress increments (c)i at the middle of the intervals. In this case, Eq. (3.15) can be written as
1
, ,,
1
1 , 1 ,
ii end j i end i
c i end c cj ij c ic j
t t t tt
E tE t
(3.53)
if the last term of the summation is written separately and zero shrinkage is assumed. While ti refers to the middle of the interval, ti,end refers to the end of the interval. Assuming c (ti,end) = c = constant and equal to 1 during all i intervals, solving Eq. (3.53) for
1
,
,1,
1 , 1 ,
ii end jc i
c c i end ci jji end i c j
t tE tt
t t E t
(3.54)
leads to the (c)i values for i = 1, 2,..., which can be added up to give the relaxation function
, 01
1,
i
i end c jjc
R t t
(3.55)
at the end of the ith interval.
Example 1
This example illustrates the stepbystep analysis for determining the aging coefficient. Thereto the linear timestress curve illustrated in
Fig. 3.3 is divided into 6 intervals with i = 1 to 6 (the first interval contains the sudden stress application at ti = 28 d).
σc [MPa]
15
10
t [d]28 84 140 196 252 30856 112
i = 6i = 1
168 224 280
i = 5i = 4i = 3i = 2
Fig. 3.3 Adopted timestress diagram for Example 1.
Steel Material Behaviour
23
Eqs. (3.10) and (3.11) are used to determine the elastic modulus
0.5
28exp 0.25 1c cE t E
t
with Ec = 30 GPa, while Eq. (3.38) is used to determine the creep coefficient
0.3
00 0.23
00
1 0.4 16.8 1, 1
302.50.1 35 35 0.1
t tt t
t tt
with h0 = 35 mm, fcm = 35 MPa, RH = 0.4 and H = 302.5.
The stress increments belonging to a constant unit strain are determined with Eq. (3.54) in the units [GPa and days]
1
2 1
3 1 2
4 1 2 3
2830
1 28,28
56 1 84,281 26.526
1 84,56 28
112 1 140,28 1 140,561 0.718
1 140,112 28 56
168 1 196,28 1 196,56 1 1961
1 196,168 28 56
c
c
c
c
c c
c
c c
E
E
E
E
E E
E
E E
5 1 2 3 4
6 1 2 3
,1120.286
112
224 1 252,28 1 252,56 1 252,112 1 252,1681 0.245
1 252,224 28 56 112 168
280 1 308,28 1 308,56 1 308,1121
1 308,280 28 56
c
c
c c c c
c
c c
E
E
E E E E
E
E E E
4 5
1 308,168 1 308,2240.196
112 168 224c c cE E
Adding up the above values according to Eq. (3.55) leads to R = 3.465 GPa. Thus, Eq. (3.51) with (308d, 28d) = 3.16 and Ec (28d) =
30 GPa leads to
30 GPa 10.81
30 GPa 3.46 GPa 3.16
According to Eq. (3.16), this means that = 3.16 applies to the 10 MPa introduced suddenly at 28 days, while = 2.56 applies to the 5
MPa introduced gradually.
Trost (1967) found the practical range of to be between 0.8 and 0.9, so that often a constant value of 0.8 is used.
3.2 Steel Material Behaviour
All of the service design models and approaches given in this thesis are based on the assumption of elastic steel behaviour
0s s s siE (3.56)
where s0stands for initial stresses andsi stands for induced steel strains (e.g. temperatureinduced). When not stated otherwise, the reinforcement steel is assumed to have an elastic modulus of 205 GPa up until the yield limit.
Basic Principles
24
3.3 Uncracked and Cracked Elastic State Section Behaviour
0.7
4.4

25
238
163
2.0
7.8

16

264
259
7.4
2.8

0.6
9.5

17.6
256
294
4.3 230
425
500
2%
20016
325
9
2.0
7.7

17
261
260
6.3
[MPa]
1.4 425
260
0.6
[ ]
(b)
ε σ [MPa][ ]ε σ
(c)
(d)
(e)
(a)
2%
Fig. 3.4 Example of a State II section with M = 150 kNm: (a) = sh = 0; (b) Eqs. (3.58) and (3.59) with= 3, sh = 0, = 0.8; (c) Eqs. (3.58) and (3.59) with = 3, sh = – 0.6 ‰, = 0.8;(d) EMM (Eq.(3.66)) with = 3, sh = 0; (e) shrinkage alone (M = 0) with sh = – 0.6 ‰Note that fct = 0 MPa,Es = 205 GPa, n = 6, lengths in [mm] and curvatures in [mrad/m].
It is common practice to determine the inservice section deformations of RC crosssections (notation see Fig. 3.5) assuming plane sections
0 z (3.57)
elastic steel and concrete behaviour and Mörsch's (1908) simplified design concept for cracked sections. According to Mörsch's simplified design concept, once the concrete tensile strength is reached in the extreme fibres, the section is assumed to reach the cracked elastic state, where fct = 0 is adopted. This is equivalent to assuming an infinitely small crack spacing. In this work the uncracked elastic state is referred to as State I, while the cracked elastic state is referred to as State II. With these assumptions
2
0.5 0.52d
h
c s s c s s cz d h z d hhN b z A A
(3.58)
Uncracked and Cracked Elastic State Section Behaviour
25
and
2
0.5 0.52d
2 2
h
c s s c s s cz d h z d hh
h hM zb z d A d A
(3.59)
can be solved for State I and State II sections.
h
ε
+
χ
d
d’
b
A’
z
y
ε 0,II
MNx
cs
As
ε
+
χ
ε 0,I
c
I
III
II
(a) (c)(b) (d)
2
h2
zh2
h2
+
A’
z
y
s
As
Fig. 3.5 Notation for Eqs. (3.57) to (3.59): (a) crosssection; (b) stress resultants (c) State I strains; (d) StateII strains.
3.3.1 ShortTerm Loads
As a consequence of setting fct = 0 after cracking, the State II momentcurvature relation of bending elements is linear (like the State I relation), as long as the depth of the compression zone remains constant. This is the case for shortterm bending without axial force.
Thus, with N = 0 and the shortterm elastic concrete behaviour (Eq. (3.2)), the equilibrium Eqs. (3.58) and (3.59) lead to the well known loadindependent transformed State I and II section properties used to determine the deformations of uncracked and cracked sections, respectively. For a rectangular section the section properties are summarized in Table 3.1 and their quotient is illustrated in Fig. 3.6. The figure illustrates the importance of correctly locating the cracked regions in lightly reinforced elements (e.g. < 0.5 %).
State I State II
x
21 1 2
I1
0.5 1
1 1
nh h f
n
22 3 2 II2d b b b d f
2 1b n n and 3 3 1b n n
A 11 1bh n II 2bd f b
I 2 2 23 3I 1 1 I I 2 I1 12 0.5 1bh f n f f bh g
32 2II3 3
II II 3 II1 13
fbd n f n f bd g
Table 3.1 State I and II section properties for rectangular crosssections with = As/(bd), ' = As'/(bd) 1 = d/h, 2 = d'/h and 3 = d'/d.
Basic Principles
26
Example 2
In this example the State II curvatures and steel stresses illustrated in Fig. 3.4 (a) are calculated. Although not needed here, the State I
section properties are also determined, as they are used in Example 7. With n = 6, = 2%, ' = 0 and d/h = 0.85, the equations in Table 3.1
lead to the shortterm section parameters
2
I
2
II
0.5 24 1 0.85 2 %0.527
1 0.85 2 % 24 1
24 2 % 2 24 2 % 24 2 % 0.384
f
f
and
22
I
32
II
1 10.527 0.85 6 1 2 % 0.85 0.527 0.0929
12 2
0.3846 2 % 1 0.384 0.0644
3
g
g
As a consequence for h = 0.5 m the section properties
I
II
0.5 m 0.527 264 mm
0.85 0.5 m 0.384 163 mm
x
x
and
3 3 2I
3 3 2II
34 GPa 1 m 0.5 m 0.0929 79378 kN m
34 GPa 1 m (0.85 0.2) m 0.0644 33787 kN m
c
c
E I
E I
are obtained. They define the cracked section curvature
II 2
150 kNm4.4 mrad/m
33787 kN m
and the steel stress
,II 2
150 kNm205 GPa 0.425 m 0.163 m 238 MPa
33787 kN ms
illustrated in Fig. 3.4 (a).
1 2 3
5
10
15
6=n
d/h 0.9=d /h 0.1=’
1
ρ =’
[%]ρ[%]ρ
ρ
I IE
I II
Ecc
0
= 0
Fig. 3.6 Stiffness ratio of a rectangular crosssection.
3.3.2 Sustained Loads
For sustained loads Trost's (1967) Eq. (3.17) expresses the concrete behaviour. With Eq. (3.17), Eqs. (3.58) and (3.59) lead to the section deformations illustrated in Fig. 3.4 (b) and (c) for the example section used in Example 2.
Uncracked and Cracked Elastic State Section Behaviour
27
AgeAdjusted Effective Modulus Method (AAEMM)
Once longterm effects such as creep and shrinkage are involved, the depth of the compression concrete becomes timedependent, leading to a nonlinear State II momentcurvature relation. In order to avoid this nonlinearity and allow the superposition of short and longterm curvatures in cracked sections, both Trost & Mainz (1968) and Ghali & Favre (1986) adopt the simplifying assumption of a timeindependent effective concrete area for State II sections. Thereby any concrete not in the compression zone at time t0 is neglected, while any concrete no longer in compression at time t due to shrinkage is considered. With this assumption they derived curvature correction coefficients and sh for determining the additional creep
0 (3.60)
and shrinkage
shsh sh d
(3.61)
curvatures by solving Eqs. (3.58) and (3.59) with Trost's (1967) concrete material behaviour (Eq. (3.17)).
1.0
00
κ
0.2
0.4
0.6
0.8
ϕ
ρ = 0.2 %
1.0
00
κ
0.2
0.4
0.6
0.8
sh
ϕ ϕ
1.2 1.2
1 2 3 1 2 3
State I,
ρ = 1.0 %State II,
ρ = 1.0 %State I,
State II, ρ = 1.0 %
(a) (b)ρ = 1.0 %
ρ = 0.2 %
ρ = 0.2 %
ρ = 0.2 %
Fig. 3.7 Ghali & Favre's (1986) curvature coefficients according to Table 3.2: (a) creep; (b) shrinkage. Note that ' = 0, n = 6, d/h = 0.85 and = 0.8.
Ghali & Favre's (1986) coefficients
c a c a c
a
A x x x x I
I
(3.62)
and
c c ash
a
A d x x
I
(3.63)
are stated here because, due to the convenient location of the axis origin in the centroid of the ageadjusted section, they are more practical. The so called ageadjusted transformed section properties
Basic Principles
28
(xa, Ia) used in Eqs. (3.62) and (3.63) and the curvature coefficients themselves are given in Table 3.2 for rectangular sections. While for uncracked sections the ageadjusted and shortterm transformed section properties are identical except for n = Es/Ec being replaced by na = Es/Ec,a, entirely different equations are required for cracked sections. This is considered the main disadvantage of this method. The ageadjusted elastic modulus is given by Eq. (3.18).
Fig. 3.7 illustrates the curvature coefficients for ' = 0, n = 6 and d/h = 0.85. For = 0.2 % a creep coefficient of = 2 leads to total curvatures and deflections around 3 and 1.2 times as large as the initial values for an uncracked or fully cracked beam, respectively. In contrast, the additional shrinkage curvatures would be negligible in the uncracked beam and approximately –sh/d in the fully cracked beam.
State I ageadjusted transformed section State II ageadjusted transformed section
xa
21 1 2
I,1
0.5 1
1 1
a
aa
nh h f
n
2II 3,
II,II 2,
0.5 aa
a
f bd d f
f b
2, 1a a ab n n and 3, 3 1a a ab n n
Aa 11 1abh n II 2,abd f b
Ia
23I, 1
2 2 31 I, I, 2 I,
10.5 1
12
a a
a a a
bh f n
f f bh g
3 23 3II, II, II II,
2 3II, 3 II,
11
3
1
a a a a
a a a
bd f f f n f
n f bd g
State I net concrete section
with centroid of the ageadjusted section
State II net concrete section
with centroid of the ageadjusted section
xc
211 1 22
11h
II II
3II2 2
f fd
f
Ac 11bh IIbd f
Ic
22 23
I, 1 1 I, I, 2
3I,
1 1
12 2a a a
c a
bh f f f
bh g
3 23 3
II, II, II II, 3
3II,
1
3a a a
c a
bd f f f f
bd g
State I curvature coefficients State II curvature coefficients
2
1 1 2
I, 1 I, I, I1
I,
0.51
1c a a a
a
g f f f
g
II IIII, II 3 II, II, II
II
II,
2 2c a a a
a
f fg f f f f
f
g
sh
21 1 2
1 1 I,1
I,
0.51
1a
a
f
g
II IIII 3 II,
II
II,
2 2a
a
f ff f
f
g
Table 3.2 Ghali & Favre's (1986) State I and II curvature coefficients for rectangular crosssections together with the necessary ageadjusted section properties. Note that na = Es / Ec,a, 1 = d/h, 2 = d’/h, 3 = d’/d and fII according to Table 3.1.
Uncracked and Cracked Elastic State Section Behaviour
29
Effective Modulus Method (EMM)
If shrinkage is neglected and is set equal to 1, Eq. (3.17) is reduced to
, c c c eft E (3.64)
with the effective modulus
0,
01 ,c
c ef
E tE
t t
(3.65)
For N = 0, Eqs. (3.58) and (3.59) with Eq. (3.64) yield
,c ef ef
M
E I (3.66)
with the advantage that both the State I and II effective transformed section properties and deformations can be can be determined with the classic section equations (e.g. Table 3.1) using n = Es/Ec,ef. Eqs. (3.64) and (3.65) are referred to as Effective Modulus Method (EMM). The EMM is the oldest (e.g. McMillan 1916) and simplest method for considering creep deformations of RC members (Bažant and Najjar 1973). For a nonaging material (e.g. very old concrete) with a bounded final creep coefficient the EMM gives the same results as the AAEMM for t ∞. Both EC 2 (European Committee for Standardization 2004) and the simplified method in ACI 209 (ACI Committee 209 1992) refer to the effective modulus for considering the influence of creep in RC members.
With = 1 the statically determinate shrinkage curvature is
c ef c
sh cief
A x x
I
(3.67)
In uncracked sections xI,c and AI,c result with n = 0 from the xI and AI equations in Table 3.1 and the extreme fibre uncracked shrinkage stresses are
,I, ,I ,I
,I
1 csh c ef ci sh ef
ef
AE h x
A
(3.68)
In cracked sections xII,c and AII,c result from the corresponding equations in Table 3.2, where fII is determined with nef according to Table 3.1. For cracked rectangular sections without compression reinforcement with AII,c = b xII,ef and xII,c = 0.5 xII,ef, Eq. (3.67) can be simplified to
,II 1II,3
cish
efd x
(3.69)
and for M = 0 (xII,ef = 0) further to
,,II
c ish d
(3.70)
Example 3
This example illustrates how the State II curvatures and steel stresses in Fig. 3.4 (d) and (e) are calculated according to the EMM. Although
not needed here, the State I section properties are also determined. With nef = 6 (1+3) = 24, = 2% and d/h = 0.85, the equations in Table
3.1 lead to the longterm section parameters
Basic Principles
30
2
I,
2
II,
22
I,
32
II,
0.5 24 1 0.85 2 %0.598
1 0.85 2 % 24 1
24 2 % 2 24 2 % 24 2 % 0.611
1 10.598 0.85 24 1 2 % 0.85 0.598 0.1178
12 2
0.61124 2 % 1 0.611 0.1487
3
ef
ef
ef
ef
f
f
g
g
Therefore, the compression zone heights are
I,
II,
0.5 m 0.598 299 mm
0.85 0.5 m 0.611 260 mm
ef
ef
x
x
and the stiffnesses are
3 3 2, I,
3 3 2, II,
34 GPa1 m 0.5 m 0.1178 25148 kN m
1 3
34 GPa1 m (0.85 0.2) m 0.1487 19496 kN m
1 3
c ef ef
c ef ef
E I
E I
For Fig. 3.4 (a) the section curvature
II 2
150 kNm7.7 mrad/m
19496 kN m
is defined by (Eq. (3.66)), while the steel stress is
,II 2
205 GPa 150 kNm0.425 m 0.260 m 261 MPa
19496 kN ms
The State II shrinkage strains at M = 0 (Fig. 3.4 (e)) are estimated with
,II
0.6 ‰1.4 mrad/m
0.425 msh
1.0
00
0.2
0.4
0.6
0.8
ϕ
1.2
1 2 3
AAEMM, = 0.8
EMM, = 1
1.0
00
0.2
0.4
0.6
0.8
ϕ
1.2
1 2 3
ΧΧκ
ϕ
κ sh
(a) (b)ρ = 0.2 %State I,
ρ = 1.0 %State II,
ρ = 1.0 %State I,
State II, ρ = 1.0 %ρ = 1.0 %
ρ = 0.2 %
ρ = 0.2 %
ρ = 0.2 %
Fig. 3.8 Comparison of AAEMM (same continuous lines as in Fig. 3.7) and EMM (dashed lines) curvature coefficients: (a) creep; (b) shrinkage. Note that ' = 0, n = 6 and d/h = 0.85.
Fig. 3.8 illustrates the small difference between Ghali & Favre's (1986) AAEMM curvature coefficients (Fig. 3.2) and the EMM coefficients
111
ef
I
I
(3.71)
Uncracked and Cracked Elastic State Section Behaviour
31
and = d sh/ci derived from Eqs. (3.66) and (3.67). In comparison to the AAEMM, the EMM yields slightly smaller creep curvature coefficients and slightly larger shrinkage coefficients. The creep curvature coefficient is smaller because the entire creep coefficient is applied to the full stress reduction caused by internal stress redistributions from the concrete to the steel.
3.3.3 Sustained and Variable Loads
If Trost's timedependent material behaviour equation (Eq. (3.17))
,0, , , ,0, , , , ,,1 1c g c t g c g c t g q c t g
c ic c cE E E
(3.72)
is extended by the elastic strains due to variable loads (q) applied at time t (last term in Eq. (3.72)) the concrete compression stresses due to permanent and variable loads at time t are equal to
,0, , , ,0,, , ,
c g c t g c gc t g q c c i
c c
EE E
(3.73)
00
M[k
Nm
]
χ [mrad/m]0
0
100
75
50
25
5 10 15 20 25
(b)
(c)
(d)
(e)
(a)
1000
250
0.35%
1.9
20.6
10.2

500
1.8
16.8
4.5

370
1.5
12.0
5.0 
211
940.60 5.3 65
4.62.510
5 690.60
127 772.8
0.60
1.1
6.1


50
176
78
2.80.60
0.5
13.4
18.0

475
39 39
I II
[MPa][ ]ε σ
(c)
(a)
(e)
(b)
(d)
[MPa][ ]ε σ [MPa][ ]ε σ
[MPa][ ]ε σ
[MPa][ ]ε σ
0.35%
Fig. 3.9 Unloading after sustained loading. Note that fct = 3 MPa before initial cracking and 0 thereafter,Es = 205 GPa, n = 6, sh = 0.6 ‰, = 3, = 0.8, lengths in [mm] and curvatures in [mrad/m].
Basic Principles
32
With a concrete compression behaviour according to Eq. (3.73), the section equilibrium equations (3.58) and (3.59) lead to the State II section deformations due to sustained and variable loads. This is shown in Fig. 3.9 for an example slab section, which is unloaded after sustained loading. As can be seen from the figure, the height and location of the compression zone is variable, indicating a strongly nonlinear deformation behaviour. Even for = 1 and sh = 0, the deformation behaviour remains nonlinear, as the compression zone depth depends on the ratio of the sustained and variable loadportions. For handcalculations involving additive sustained and variable loads it is suggested that the section deformations be determined assuming the effective section properties in the case of dominating sustained loads and elastic section properties in the case of dominating variable loads.
3.4 Tension Chord Model
The Tension Chord Model (TCM) models the interaction between the reinforcement and concrete between the cracks in cracked tension chords. This can be regarded as a refinement to the State II section behaviour, which neglects the effect that is referred to as tension stiffening. The model applies to uniaxial stress states (e.g. tension ties or Bernoulli beams) and was initially derived to analyse the deformation capacity of plastic hinges (Sigrist 1995; Alvarez 1998) in the ultimate limit state, but is also a practical tool for serviceability limit state calculations.
3.4.1 Basic Assumptions
δ s( )σ = syf
(a)
δ
τb
τb0
τb0
δ
τb0
τb1
0
(b)
τb
k 8
Fig. 3.10 Rigidperfectly plastic bond stressslip relations adopted by the Tension Chord Model: (a) Sigrist(1995); (b) Marti, Sigrist, et al. (1997).
The Tension Chord Model is based on Kuuskoski's and Rehm's differential equation of slipping bond and adopts two principal assumptions. The first assumption is the strongly simplifying bond stress – slip relationship (Fig. 3.10 (a)) at the interface between the steel and concrete (Sigrist 1995). Before steel yielding the bond stress transmitted between the reinforcing steel and the concrete is assumed to be constant and equal to b = b0. Based on pull out tests carried out by Engström and Shima and theoretical parameter studies, Sigrist suggested b0 = 2 fct for ordinary ribbed bars (relative rib areas around 0.05 to 0.07), with fct according to Eq. (3.8). Sigrist's suggestion coincides with the findings of test data based parameter studies (250 tests) carried out at TU Darmstadt and reported by König and Fehling (1988). These parameter studies started with a linear bond stressslip relationship with b = 0 + ' and concluded that average crack widths predicted with b = 2 fct (' = 0) and an integration coefficient of 0.6 (belonging to the linear bond stressslip relationship) give the best agreement
Tension Chord Model
33
with measured crack widths. On this basis, Chapter 7 of MC 90 (1993) and MC 2010 (fib 2010b) suggest b = 1.8 fct and an integration coefficient of 0.6 for shortterm loads.
Marti, Sigrist, et al. (1997) suggested the bond stress – slip diagram illustrated in Fig. 3.10 (b). It is assumed that as soon as a positive slip occurs bond stresses equal to b0 are activated. These remain constant unless the slip is released and bond stresses in the opposite direction –b0 are activated. Positive slip and bond stress values apply to a bar being pulled out of the concrete, while negative slip and bond stress values apply to a bar being pushed into the concrete. Later, based on his Bragg grating sensor measurements Kenel (2002) suggested negative bond stress values equal to 0.5 b0.
fct
++
NN
σs, II
l0
Ø τb4
Ø
ρ1 ρ
τb4
c,avg
+ +ε
+ τb
ε s,avgεs, II
2
δ
τ
0
τb
(a) (b)
(d) (e)
σ
ε ε
σl02 l02l02
(c)
Fig. 3.11 Tension tie element between two cracks spaced at twice the transfer length (): (a) tension chordelement; (b) bond stressslip relation; (c) bond stress distribution; (d) concrete tensile stresses andstrains; (e) steel tensile stresses and strains.
The second main assumption behind the Tension Chord Model consists in assuming a constant tensile strength fct for the entire tensile tie or chord.
The two assumptions lead to an upper and lower limit value for the final crack spacing (stabilized cracking) defined by parameter [0.5…1] (Marti et al. 1998). The lower limit () is established if a crack forms a transfer length away from a previous crack, while the upper limit occurs () if a crack forms twice the transfer length
0
1 1
4 8ct
b
fl
(3.74)
away from a previous crack. The transfer length (or alternatively referred to as transmission length) is defined as the length on either side of a crack where the bond is disturbed (see Fig. 3.11). No primary cracks will form within the transfer length because in this region the concrete stresses are smaller than the concrete tensile strength. If a crack forms further away than twice the transfer length, then there is an undisturbed region between the two cracks where a new crack can form. Depending on the crack spacing, the average concrete tensile stresses between two cracks (see Fig. 3.11) are
, 2ct
ct avg
f (3.75)
As a consequence the average steel strains are smaller than they would be without the concrete between the cracks. This effect is referred to as tension stiffening.
Basic Principles
34
3.4.2 Tensile Members
ε0sm ε0
e ε0i
σs, II σs, II σs, II
σs, ,rII
fctEc
1Es
1Es
fctEc
fctEc
1Es
a( ) b( ) c( )
εΔ s,ts
B
εΔ s,ts εΔ s,ts εΔ s,ts εΔ s,ts εΔ s,ts
Fig. 3.12 Tensile tie with a length of 8 l0 and = 1 under (a) an imposed axial load N; (b) an imposed axialdeformation e or restrained cooling strains e = – T; (c) restrained shrinkageinduced strainsi = – sh according to Marti, Alvarez, et al. (1997).
Axial Load
If a constant concrete tensile strength is assumed, upon reaching
(1 )r ctN bhf n (3.76)
all cracks form simultaneously in a force controlled RC tension tie, which immediately changes from State I to State II (Fig. 3.12(a)). For the cracking load the steel stresses in the cracked sections are
,II, 1cts r
fn
(3.77)
With average concrete stresses according Eq. (3.75), the equilibrium equation Es bh s,II = Es bh (s,II – s,ts) + bh (1– )/2 fctFig. 3.11yields the average steel strain reduction due to tension stiffening
,
(1 )
2ct
s tss
f
E
(3.78)
in tensile ties with evenly distributed reinforcement = As/bh. In tensile elements with concentrated reinforcement at the edges refers to the effective reinforcement ratio. The crack widths are
0,II ,II,
2
2s s rs
lw
E
(3.79)
Factor is set equal to 1 and 0.5 to consider the maximum and minimum crack spacing, respecively.
Restrained and Imposed Deformations
Marti et al. (Marti, Sigrist, et al. 1997; Marti, Alvarez, et al. 1997; Marti et al. 1998; Alvarez 1998) use the Tension Chord Model for a restrained tensile tie. They distinguish between internal and external restraint, referring to internal restraint for fully restrained shrinkageinduced strains and referring to external restraint for fully restrained temperature–induced (cooling) strains or imposed defor
Tension Chord Model
35
mations. In addition to the two basic Tension Chord Model assumptions, the shrinkage and temperature induced strains are assumed to be uniformly distributed over the concrete and entire section, respectively.
The crack formation phase starts when the restrained or imposed strains reach fct/Ec. In contrast to the axially loaded tension tie, there is an extensive crack formation phase (see Fig. 3.12(b) and (c)) as each crack causes a global stress relief in the member. The axial force in the member is determined by imposing equilibrium and strain compatibility in the uncracked regions as well as enforcing the boundary conditions (constant member length or the imposed deformation length). The equations given here (Alvarez 1998) apply to a tension tie with cracks spaced further apart than twice the transfer length ( = 1), where j denominates the crack number. For imposed deformations (e = imposed) or restrained coolinginduced strains (e = – T) (see Fig. 3.12(b)) the crack steel stresses
2
0,II 2 2
0
2 1 11 1
1
b c es
b
ln n j E
lnj
(3.80)
fluctuate below s,II,r (Eq. (3.77)), while the corresponding crack widths
2 20
32
2 11 1
21
b
c
l n nw
j E
(3.81)
with
2
20
1c e
b
j E
ln
(3.82)
fluctuate below s,II,r l0 /Es. For shrinkageinduced strains (i = –sh) (see Fig. 3.12(c)), which don't affect the reinforcement, the crack steel stresses
2
0,II 2 2
0
2 1 11 1
1
b c is s i
b
ln n j EE
lnj
(3.83)
fluctuate below s,II,r – Esi. Their maximum value is (point B in Fig. 3.12(c))
2
,II,max 20
111
4ct
s ctb
ff
l
(3.84)
The stabilized cracking phase starts at
, or cte i s ts
c
f
E (3.85)
After this point the steel stresses increase
,II ,s s e s tsE (3.86)
in the case of imposed or restrained coolinginduced strains or remain constant
,II ,s s s tsE (3.87)
for shrinkageinduced strains. In both cases the crack widths increase. Further information on endrestrained and deformationinduced cracking can be found in Chapter 4.2, where the equations for
Basic Principles
36
shrinkage and temperatureinduced cracking are combined and extended to partially endrestrained tension ties.
3.5 Summary
The State I and II deformations of general RC beam sections result from solving the equilibrium Eqs. (3.58) and (3.59). Thereto plane sections according to Eq. (3.57), elastic steel material behaviour according to Eq. (3.56) and Trost's concrete material behaviour according to Eq. (3.17) can be assumed.
The creep coefficient and free shrinkage strains can be estimated e.g. with the MC 90 Eqs. (3.20), (3.21) and (3.36). The aging coefficient is between 0.8 and 1; for ordinary RC sections the influence of is usually negligible and = 1 can be adopted.
In the absence of an axial force (N = 0) the equilibrium equations (3.58) and (3.59) provide the transformed section properties for determining the shortterm momentinduced section deformations. Table 3.1 contains the transformed section properties for rectangular sections.
The transformed section properties can also be used to determine the longterm momentinduced section deformations (N = 0, =1) if the modular ratio n is determined with the effective modulus according to Eq. (3.65).
The crosssection shrinkage curvatures (no external restraint) are provided by Eq. (3.67).
The Tension Chord Model complements the State II section behaviour by providing the transfer length (Eq. (3.74)) for determining the crack spacing as well as the average concrete stresses (Eq. (3.75)) in the tension chord. These concrete tensile stresses reduce the tensile steel strains according to Eq. (3.78).
37
4 Tension Chord Model for Serviceability Problems
The complex and hardly known load history and the highly variable concrete properties (see Chapter 3.1) represent the main difficulties for predicting the deformations of reinforced concrete (RC) structural members. For reasons of simplicity, deformation prediction approaches (see Chapter 2) usually neglect the unknown load history (e.g. precracking due to construction overloads) and the corresponding initial deformations. For these reasons, integral (e.g. midspan deflections) and in particular local deformation predictions (e.g. strains, curvatures, crack widths) will never achieve the same accuracy as ultimate load predictions (Marti 1983). Still, practical applications require reasonably reliable estimates of the magnitude of both integral and local deformations.
The Tension Chord Model (see Chapter 3.4) represents a consistent tool for modelling the inservice deformation behaviour of tensile members with uniaxial stress states, such as tension ties and tension chords in oneway bending members. So far (see Chapter 3.4), the model has been used to describe the shortterm load and restraintinduced cracking behaviour of tensile elements (Marti, Sigrist, et al. 1997; 1998; Alvarez 1998) as well as the loadinduced cracking and deflection behaviour of statically determinate bending elements (Kenel 2002; Kenel et al. 2005).
Based on this previous work, this chapter aims at illustrating the wide range of serviceability prediction equations for designing tensile and oneway bending members that can be derived based on the Tension Chord Model. Thereto, in Section 4.1 the Tension Chord Model is extended in order to account for the effective concrete area in bending elements, the loss of tension stiffening due to bond creep and the influence of unloading. The Tension Chord Model is then combined with the longterm section deformation approaches for bending elements discussed in Chapter 3.3 to obtain handcalculation equations for predicting short and longterm crack widths (Section 4.2) and deflections (Section 4.3). The crack width predictions are focused on moment, restraint, and deformationinduced cracking with different boundary conditions. Further, the influence of the reinforcement detailing on the deflections of statically indeterminate members is discussed and limiting spantodepth ratios are derived. In the whole chapter, the stress in the reinforcement steel is assumed to remain below the yield limit and shear deformations are neglected.
4.1 Tension Stiffening
4.1.1 ShortTerm
The Tension Chord Model considers the contribution of the tensile concrete by assuming a linear distribution of concrete tensile stresses between the cracks (Fig. 4.1 (a)). In bending members the concrete stresses are further assumed to be uniformly distributed over the net concrete area Ac,ef of a tension chord that has the same centroid as the tensile steel (Fig. 4.1 (c)). This leads to average concrete strains in the tension chord equal to
,, 2
c ts ctc ts
c c
f
E E
(4.1)
Tension Chord Model for Serviceability Problems
38
Factor stands for the crack spacing (see Chapter 3.4.1) and varies between 0.5 and 1 and fct is defined by Eq. (3.8). The most general way to consider Eq. (4.1) is by inserting the average concrete tensile force (c,ts Ac,ef) into the section equilibrium equations (Eqs. (3.58) and (3.59)). For tension chords with constant section properties and tension forces (that is V = 0 in bending elements) this yields the average steel strain reduction
,
1
2ct ef
s tsef s
f
E
(4.2)
and the corresponding average curvature reduction
,
II
s tsts d x
(4.3)
for tension chords in bending elements (Fig. 4.1 (d)). The latter equation assumes a constant compression zone height (xII), which allows its superimposition with the State II curvature. The main disadvantage of Eqs. (4.2) and (4.3) is their dependency on the effective reinforcement ratio of the tension chord ef = As / (Ac,ef + As).
Marti (2004) suggested determining the effective reinforcement ratio by equating the State II steel stresses in the actual bending element and the corresponding steel stresses in the tension chord at cracking. In bending members without axial forces (N = 0), the State II steel stresses at M = Mr are equal to s,II,r = (Mr n (d – xII)/III), while the corresponding steel stresses in the fictitious tension chord are equal to s,II,r = fct (1/ef + n – 1). Solving for ef, leads to
1
I II
II I
1( )ef
nI d xn
I h x
(4.4)
and a net concrete area
I II,
II I
1( )c ef s
I d xA nA
I h x
(4.5)
In contrast to Schiessl's effective reinforcement ratio (Eq. (2.8)), Eq. (4.4) is compatible with the Bernoulli bending theory. Inserting Eq. (4.4) into Eq. (4.2) leads to
, ,II,2ct
s ts s rc
f
E
(4.6)
while Eq. (4.4) in Eq. (4.3) produces
II II2ctr
tsc c
fM
E I E d x
(4.7)
The first terms in the brackets of Eqs. (4.6) and (4.7) correspond to the State II steel strain and curvature, respectively at M = Mr. The 2nd term in Eq. (4.6) represents the State I steel strains at M = Mr, while the second term in Eq. (4.7) represents those State I steel strains divided by the State II steel lever arm. Both equations are loadindependent. The fact that they could have been derived directly from Fig. 4.1 (a) for M = Mr proves the consistency of the approach.
Eqs. (4.1) and (4.6) form the basis for crack width predictions, while Eq. (4.7) is a very practical equation for considering tension stiffening in bending elements, as the effective reinforcement ratio is implicitly considered. Eqs. (4.6) and (4.7) are derived for V = 0, but represent good approxi
Tension Stiffening
39
mations also when V ≠ 0, as the tension force gradient due to shear within the cracked elements is usually small (see Seelhofer (2009)).
χ
χΔ
IIIEc
IIEc
1
M(d)
00
/d/d
/h1/h
Mr
My
I IIIII
ts
 
 
/2
d
= 1λ
h xd
l0
σc fct+
+σs
ΔE
II
l0
(b)
χII
εs,II
xII
ε σ
σs,II
xII
xII xII
ε σ
d χII
εs,II εΔ s,ts
χΔ ts

fct
σs,II εΔ s,tsEs
(c)
(a)
εs,tss
crack crack
Fig. 4.1 Tension stiffening in a cracked flexural member (N = 0): (a) Tension chord element between twocracks; (b) strains and stresses in State II section; (c) average strains and stresses considering tension stiffening ( = 1); (d) momentcurvature diagram illustrating ts.
For combined bending and axial force (notation see Fig. 3.5), the procedure described above leads to:
, II, II,s
c ef s r rct
EA A d c n
f
(4.8)
and
1
II, II, 1sef r r
ct
Ed c n
f
(4.9)
as well as
II,
II,II II2
r ctts r
c
d c f
d c E d c
(4.10)
Note that Eq. (4.10) is loaddependent. II,r and cII,r denote the State II curvature and height of the compression zone at cracking.
4.1.2 LongTerm
Under sustained loads, creep relaxes the concrete stresses involved in the mechanical interlock between the steel and the concrete (Fig. 4.2 (a)). As a consequence, the effective bond stresses are reduced and the slip is increased. In order to consider the loss of bond stress due to creep, factor
Tension Chord Model for Serviceability Problems
40
,, 1
1c efb
b c
Ek
E
(4.11)
is introduced. This factor (Fig. 4.2 (b)) is determined according to the Effective Modulus Method (Eq. (3.65)) and used to reduce the concrete strains
, 2ct
c tsc
fk
E
(4.12)
and the steel strain reduction
, ,II,2ct
s ts s rc
fk
E
(4.13)
The crack spacing of existing cracks is not affected by bond creep and remains between 0.5 and 1. Besides bond creep, the average curvature reduction
II
II II, II,2
ctrts
c ef c ef
d x fMk
E I d x E d x
(4.14)
is further affected by the drop in the neutral axis due to compression zone creep. The height of the compression zone xII,ef is determined with the effective elastic modulus (Eq. (3.65)).
CLcrack
l0
(a)
ϕ0
k
1
(b)ϕ
2 3
1.0
0.5
Fig. 4.2 Longterm loss of tension stiffening: (a) Schematic illustration of the internal stress resultants involved in the mechanical interlock between the steel and the concrete in a cracked RC tensionchord; (b) loss of bond stress under sustained loads according to Eq. (4.11).
Neglecting the shrinkage restraint between the steel and the cracked concrete, shrinkage further increases the slip without influencing the bond stresses. The assumption of a constant bond stress, which is reduced in time due to bond creep, impedes the modelling of secondary cracks caused by restrained shrinkage stresses in the tensile concrete between the cracks. If at all, secondary cracks are most likely to form in = 1 crack elements and are therefore included within the range of = 0.5 to 1.
The strongly simplified relationship between k and (Fig. 4.2 (b)) is suggested in view of the highly complex nature of the stresses involved in the mechanical interlock and the large uncertainties involved in determining the longterm concrete parameters. Note that while [0.5...1] takes into account the crack spacing, k[0...1] considers the contribution of the tensile concrete between the cracks, where k = 1 implies b = 2 fct and k = 0 implies b = 0. In this sense, kcan be seen as a general factor for expressing the contribution of tension stiffening for a given crack spacing. kis used in
Tension Stiffening
41
this way in the test data comparisons illustrated in Chapter 5.2.1 to show the limiting cases of full (k = 1) and no (k = 0) tension stiffening.
4.1.3 Unloading
Again based on the loadtransfer model illustrated in Fig. 4.2 (a) the strongly simplified bond stress – slip relationship illustrated in Fig. 4.3 (a) is adopted. The relation implies that the bond stress is lost if the slip is reduced. In other words, pulling the steel bar out of the concrete is resisted by bond stresses, but no bond stresses have to be overcome for it to retrace its way back in again. Before unloading (Fig. 4.3 (b)) the bond stresses are activated along the entire tension chord. Reducing the State II steel stresses in the crack (Fig. 4.3 (c)), reduces the slip along the length x, where the bond stresses disappear. It is assumed that the slip along the remaining sections stays constant (no relative movement).
δ
τ
fct
(a)
2τ
l0
(b)
crack CL
λ
+
+
ε
τ
x
(c)
CL
s
εc +
+
τ
fct x τEc l0
σs,
Es
II
Δσs,
Ec
II
σs,mEsε s
εcfct
Ec
λ
σs,
Es
II
fct x τEc l0
Øτb4
ØEs
σs,mEs
τb4Es
ε s,avg
crack
Fig. 4.3 Half of a tension cord during unloading (a) assumed bond stress – slip relationship; (b) concreteand steel stresses before unloading; (c) concrete and steel stresses during unloading.
During unloading (Fig. 4.3 (c)) the tension stiffening steel strain reduction is
,II , 0,
02s s mu
s tss
l x
l E
(4.15)
with
0,II ,
0
1cts s m
f l x
l
(4.16)
determined by formulating equilibrium for N at the crack and at the symmetry axis leads and
0 ,II
01s
ct
lx l
f n
(4.17)
from formulating equilibrium for N at the crack and at a distance xaway from the crack. Introducing Eqs. (4.16) and (4.17) in (4.15) leads to
Tension Chord Model for Serviceability Problems
42
,II,
10
2 1sctu
s tss ct
f
E f n
(4.18)
which is valid for s,II between zero and
,II ,II, 1cts s r
fn
(4.19)
where x = l0 is reached. Replacing s,II with Es (s,avg,max + s,ts – s,avg – us,ts) leads to
2 2, , ,,
2 2, , ,
2 1 2 1
11 1
us avg s ts s avgs ts
us ts s ts s ts
n n n nk
(4.20)
ku is between 1 and 0 and s,avg = s,avg,max – s,avg.
4.2 Crack Width
The Tension Chord Model is based on the slippingbond approach (Chapter 2.1.1) to crack width prediction, which assumes that the crack spacing and concrete strains remain constant over the depth of the tension chord. In this case, the crack width
0 , ,2 s avg c avgw l (4.21)
is constant over the entire depth of the member and is defined as the integral of the difference between the steel and concrete strains within the crack influence region, which according to the Tension Chord Model is equal to 2l0 (l0 and are defined in Chapter 3.4.1). Inserting the average steel strains
, ,II ,II,2ct
s avg s s rc
k f
E
(4.22)
determined with Eq. (4.13) and the average concrete strains
, 2ct
c avg cic
k f
E (4.23)
determined with Eq. (4.12) into Eq. (4.21) results in
0 ,II ,II,22s s r ciw l k
(4.24)
Eq. (4.24) forms the basis for determining the widths of moment, restraint and deformationinduced cracks in tension ties and chords. The decisive components of this equation are the crack influence length 2l0 and the loadcase dependent State II steel strains s,II at the time when the crack width is predicted. The concrete tensile strains ks,II,r due to tension stiffening reduce the crack width, while shrinkage or temperatureinduced concrete contraction strains (c,i) increase the crack width. The State II steel strains at cracking s,II,r are a function of the stress resultant at cracking, determined at the time of loading.
At the beginning of the crack formation phase, the crack influence region 2l0 extends over twice the transfer length l0 (Eq. (3.74)) and = 1. At the end of the crack formation phase the extent of the crack influence region corresponds to the stabilized crack spacing
Crack Width
43
02rs l (4.25)
which according to the Tension Chord Model (Chapter 3.4.1) is assumed to be between once ( = 0.5) and twice ( = 1) the transfer length. In many practical cases the crack spacing corresponds to the stirrup spacing; in this case is defined. In all cases, = 1 is decisive for predicting maximum crack widths.
Both the crack widths at the concrete surface and the bar surface are relevant for crack width control. The former are of interest for aesthetical considerations, while the latter may be of interest for durability and, in the absence of a compression zone, liquid tightness. The secondary Goto cracks (Goto 1971), which form at the bar ribs, considerably reduce the crack width at the bar surface, as the integral strain difference between the steel and concrete is absorbed by a larger amount of cracks. With increasing distance from the bar surface, the Goto cracks disappear until at the concrete surface only the primary cracks are visible. If the shear lag effect is neglected, the theoretical crack widths determined with the Tension Chord Model correspond to theoretical surface crack widths, as they are based on the surface crack spacing.
4.2.1 Bending
For bending members with N = 0, the State II steel strains at M = Mr correspond to
II I II,II,
II II I
r cts r
c c
M d x f I d x
E I E I h x
(4.26)
They are a function of the concrete material parameters (fct and Ec) and the section properties (, ', d/h, d'/h). Neglecting the influence of V on tension stiffening, Eq. (4.26) and Eq. (4.24) lead to
I II0 ,II
II I
22
cts ci
c
f I d xw l k
E I h x
(4.27)
The transfer length
I II I II0
II I II I
1 14 8
ct
b
I d x I d xnf nl
I h x I h x
(4.28)
results from inserting Eq. (4.4) into Eq. (3.74).
The first term in the brackets of Eq. (4.27) corresponds to the State II steel strains. In bending members they are usually determined at the centroid of the tensile reinforcement. However, in deep beams with multiple layers of tensile reinforcement, the stress gradient between the different steel layers causes an increasing crack opening with increasing distance from the neutral axis. This can be considered by determining the State II steel strains at the height of the specific reinforcement layer. For shortterm loads the State II steel strains correspond to
II,II
IIs
c
M d x
E I
(4.29)
For sustained loads the steel strains can either be determined with the section equilibrium equations (Eqs. (3.58) and (3.59)) and Trost's concrete material behaviour (Eq. (3.17)) or estimated with the effective concrete properties (EMM, neglecting shrinkage). In many cases they can also be assumed timeindependent, as the influence of longterm effects on the steel strains is often negligi
Tension Chord Model for Serviceability Problems
44
ble because the increase in curvature is compensated by the increase in compression zone height (see e.g. Marí et al. 2010).
The second term represents the average contribution of the tension concrete, assumed to be constant within the whole effective concrete area (Fig. 5.10 (c)). For maximum crack widths = 1. For shortterm predictions k = 1, while for sustained loads k can be reduced according to Fig. 4.2 (c). If the tensile concrete is neglected k = 0 and
0 ,II2 s ciw l (4.30)
The third term reflects any shrinkage or temperatureinduced concrete strains. The assumption of a constant bond stress between the steel and concrete implies that imposed concrete contraction strains are not restrained in cracked sections.
For shortterm crack width predictions with ci = and k Eq. (4.27) can be simplified to
II0
II
2 12
r
c
M d x Mw l
E I M
(4.31)
At cracking Eq. (4.27) with s,II = s,II,r leads to
I II I II
II I II I
1 14 2
ctr
c
I d x f I d xnw
I h x E I h x
(4.32)
Example 4
This example illustrates the maximal crack width caused by a moment M = 70.5 kNm in a slab strip with sections and material properties
according to Fig. 3.9. It is assumed that the slab strip is reinforced with 12 mm bars (spaced at 150 mm). Table 3.1 provides the section
parameters: fI = 0.505, fII = 0.185, gI = 0.0851 and gII = 0.0161.
A transfer length (Eq. (4.28)) of
0 2
0.0851 1 0.18561 8.3
8 0.0161 0.85 1 0.505l
leads to a maximal ( = 1) crack spacing of 16.6 · 12 mm = 200 mm. With fct = 3 MPa, the State II steel strains at cracking (Eq. (4.26))
equal
,II, 2
0.0851 1 0.1856 3 MPa1.06 ‰
205 Ga 0.0161 0.85 1 0.505s r
while the State II steel strains at M = 70.5 kNm equal s,II = 475 MPa / 205 GPa = 2.32 ‰ (Stage A in Fig. 3.9). On this basis Eq. (4.27)
provides a crack with
1.06 ‰2 8.3 12 mm 2.32 ‰ 0.36 mm
2w
Shrinkage strains of sh = – 0.6 ‰ and a reduced k value of 2/3 increase the crack width to
2 1.06 ‰2 8.3 12 mm 2.32 ‰ 0.6 ‰ 0.51 mm
3 2w
if the steel strain increment due to longterm effects is neglected or
2 1.06 ‰2 8.3 12 mm 2.44 ‰ 0.6 ‰ 0.54 mm
3 2w
fors,II = 500 MPa / 205 GPa = 2.44 ‰ (Stage B in Fig. 3.9).
Crack Width
45
4.2.2 Restrained Deformations
Restraintinduced cracking is caused by shrinkage or temperatureinduced concrete strains c,i (contractive strains), which are restrained by neighbouring section parts (internal restraint) or boundary conditions (external restraint). The resulting tensile stresses can cause surface cracks, if they are concentrated at the surface (e.g. mass concrete), or separation cracks, if they extend over the entire section (e.g. flat plates in lowmoment regions). In the second case the whole section requires a minimum reinforcement and in absence of a compression zone the cracks can cause leakage.
This paragraph discusses the two principal external restraint cases illustrated in Fig. 4.4, neglecting loadinduced stress resultants. It is assumed that the shrinkage and temperatureinduced concrete strains ci = sh + T are uniformly distributed over the section. In the case of temperature, the concrete strains are accompanied by steel strains si = T = – T. Shrinkageinduced concrete strains range between 0 and –1 ‰. Assuming a thermal expansion coefficient 0.01‰/K, a temperature drop of 100 °C causes a strain increase of –1 ‰.
l
(a) (b)
h
l
τcx
k
Fig. 4.4 Basic external restraint cases: (a) Endrestraint; (b) continuous edgerestraint. Note that x = 0 to l/2and k in [N/mm3].
Prior to cracking, the concrete tensile stresses
c c ciRE (4.33)
increase until at
,ct
ci rc
f
E R (4.34)
the crack formation process starts. The degree of restraint R ranges between 0 and 1. Creep releases a part of the restraint tensile stresses and can be considered for example by replacing Ec with Ec,ef (Eq. (3.65)) in Eqs. (4.33) and (4.34). Eq. (4.24) with
,II,
1cts r
s
f n
E
(4.35)
defines the crack widths
0 ,II
12
2ct
s cis
k f nw l
E
(4.36)
where
,II,II
ss si
sE
(4.37)
Unless stated otherwise the transfer length l0 is defined by Eq. (3.74) and k = 1 is assumed.
Tension Chord Model for Serviceability Problems
46
The two basic concepts of crack control consist in either trying to prevent cracks from forming (Eq. (4.33)) or reducing their widths (Eq. (4.36)). If restraintinduced axial forces are combined with loadinduced bending moments, the MN interaction has to be considered for determining the State II steel stresses (see Specimen RG8 in Chapter 5.2.1).
EndRestraint
The member deformations l = – N/(kbh) (Fig. 4.4 (a)) are defined by the axial stiffness of the support k [N/mm3] and the axial restraint force N, which is assumed to be constant within the member. Two dimensionless coefficients are defined as
s
lk
E (4.38)
and
II 1
Aa n
bh (4.39)
Before cracking
With s,I = Es (I – si) and c,I = Ec (I – ci), l = lI leads to
I
1si cinl
l n a
(4.40)
the concrete stresses
,I
I
si cic cnE
n a
(4.41)
the degree of restraint
I
1 si
ci
n n
Rn a
(4.42)
and the axial force
I I ,Ic s ci siN bh a E (4.43)
Crack Formation Phase
The crack formation phase starts at
I, ,1
ct c sici r
c
f a n E
E
(4.44)
when c,I first reaches the concrete tensile strength. If k > 0 each new crack causes a global stress relief in the member. This leads to an extensive crack formation phase, during which the axial restraint force N decreases and increases between the development of the cracks.
The steel stresses in the cracks peak just before a new crack forms, when the concrete stresses in the uncracked sections reach the concrete tensile strength (Fig. 4.5 (b)). For c,I = fct, equilibrium ( s,II = s,I + c,I) and strain compatibility (s,I = n c,I + Es (ci si)) lead to
Crack Width
47
I,II,
cts r s si ci
f aE
(4.45)
with the corresponding axial force Nr = bh s,II,r, deformations l = Nr/(kbh) and crack widths
0 I2 ctr
s
l f aw
E
(4.46)
This crack width wr corresponds to the crack width obtained if the member is loaded with its cracking load. Both s,II,r and wr are independent of the support stiffness k. They are illustrated with dashed lines in Fig. 4.6 for a lightly reinforced example member.
fct
+
l02
+ + fct
fctEc
+
ε
fct
Es
(1 )ρρ
++
ε
εEs

2
εEs
fct (1 )ρρ
ε
σc
ε c
εs
σs si
ci
si
ci
fctEs
(1 )ρρ
fct (1 )ρρ
fct
lb2
+
ε
+

εEs
ε
(a)
si
ci
fctEs
(1 )ρρ 
lbl0
lbl0
2
 
σs,II
σs,I
σc
ε c
εs
σs
σc
ε c
εs
σs
(b) (c)
l02
crack crack crack
Fig. 4.5 Endrestraint with = 1 and = ∞: Stresses and strains due to shrinkage and temperatureinducedcompressive strains: (a) just after crack j; (b) just before crack j+1; (c) stabilized cracking.
According to the Tension Chord Model (see also 3.4.2), the member deformations inbetween two cracks j and j + 1 (Fig. 4.5 (a)) correspond to
,I ,II ,IIcrackcrack crack
0
1
4s s sct
sis s s
l fl l jl l jl
E E l E k
(4.47)
Cracks spaced no closer than twice the transfer length ( = 1) have an influence region lcrack equal to twice the reduced transfer length (Fig. 4.5 (a))
,II ,I 0
1s s
bct
ll
f
(4.48)
where
,II,I
I
1s s si cis
n E
a
(4.49)
Tension Chord Model for Serviceability Problems
48
is the steel stress in the uncracked sections. Assuming that no cracks are closer twice the transfer length, inserting Eqs. (4.48) and (4.49) into (4.47) leads to
I I,II 2
I
21 1
s ci si cicts s si ci
ct
E nn a a fE
n f n a
(4.50)
where
02 1
n l
l j
(4.51)
N = s,II bh and l = N/(kbh). Equating Eqs. (4.45) and (4.50) and setting j = 1 leads to the induced concrete strains at point B
22
I, ,
I
1 12
ct sici r B
s
f n a n
nE n a
(4.52)
where the steel stresses (Eq. (4.45) with ci ≠ si) are maximal (see Fig. 4.6 (b)).
00
400
300
200
100
σ[M
Pa]
s,II
00
ε [ ]0
00.2 0.4 0.6 0.8 1
ci
w[m
m]
0
ε [ ]0 0.2 0.4 0.6 0.8 1
ci
0
0.1
0.2
0.3
0.4
0.5
000
σs, ,rII
Bσs, ,rII
wr wr
(a) (b)
(c) (d)
Fig. 4.6 Endrestrained tension chord with l = 40 l0 ≈ 10 m and k = ∞: (a) State II steel stresses for si = ci;(b) State II steel stresses for si = (c) crack widths for si = ci; (d) crack widths for si = Notethat = 0.6 %, = 12 mm, fct = 2 MPa, n = 6, Es = 205 GPa, b = 2 fct and = 1.
Crack Width
49
With Eq. (4.50), a crack influence region equal to 2 lb and a concrete contribution reduced by the factor lb / l0, the crack width Eq. (4.36) yields
222
0 I I2 2
I
21 1
s ci si cict
s ct
E nl f n a aw
n E f n a
(4.53)
Cracks that form closer than twice the transfer length away from an existing crack cause a smaller global stress relief than according to Eq. (4.50). For the limiting case of all cracks following the first crack forming a transfer length away from the previous crack ( = 0.5), lcrack in Eq. (4.47) equals l0.
For k = ∞ (Fig. 4.6), Eqs. (4.50) and (4.53) can be simplified to
I,II
21 1ct s ci
s s si cict
a f EE
nf
(4.54)
and
22
0 I 21 1ct s ci
s ct
l f a Ew
E nf
(4.55)
Stabilized Cracking
After the crack formation phase is concluded (Fig. 4.5 (c)), jlcrack = l and lcrack = 2l0 so that Eq. (4.47) can be simplified to
,II ,II1
2s sct
sis s
fl l
E E k
(4.56)
Inserting s,II,r according to Eq. (4.45) into Eq. (4.56) yields the induced concrete strains
, , I
12
2ct si
ci r jns
fa
E
(4.57)
necessary to finalize the crack formation phase with
02n
lj
l
(4.58)
cracks. Further, solving Eq. (4.56) leads to the stabilized cracking steel stresses
,II
1
2ct
s s si
fE
(4.59)
with the corresponding crack widths
I02
2ct
si cis
f n aw l
E
(4.60)
as well as axial force N = s,II bh and deformations l = N/(kbh).
Tension Chord Model for Serviceability Problems
50
For k = ∞ (Fig. 4.6), Eqs. (4.57), (4.59) and (4.60) can be simplified to
, , I1 22
ctci r jn
s
fa
E
(4.61)
and
,II 12
cts s si
fE
(4.62)
as well as
022
ctci
s
nfw l
E
(4.63)
For k = 0 both ci,r,1 (Eq. (4.44)) andci,r,jn (Eq. (4.57)) can be simplified to
I,
ctci r si
s
f a
E
(4.64)
as there is no global stress relief in the member due to cracking and all cracks form simultaneously if a constant concrete tensile strength is assumed. Eq. (4.59) yields s,II = 0, while Eq. (4.60) yields
0
12
2ct
ci sis
f nw l
E
(4.65)
Example 5
In this example the State II steel stresses and crack widths of the approximately 10 m long (40 l0) endrestrained tension chord illustrated in
Fig. 4.6 are determined. The tension chord has a reinforcement ratio of = 0.6 % established by = 12 mm bars. The material properties
are fct = 2 MPa, n = 6 and Es = 205 GPa. The tension chord is submitted to a) uniform cooling induced strains (e.g. due to loss of hydration
heat) with si = ci and b) uniform shrinkage strains with si = 0. A restraint stiffness of k = ∞ is assumed.
The length of the tension chord is chosen to be 20 times the double transfer length (Eq. (3.74))
0
12 mm 1 0.6 %249 mm
8 0.6 %l
so that 20 cracks lead to the maximal final crack spacing ( = 1). Further aI (Eq. (4.39)) = 6 · 0.6% – 0.6% + 1 = 1.03 and
6 0.6 % 40 249 mm 0.724
2 249 mm 1 0.6 % j j
With R = 1, cracking starts when the imposed concrete strains reach (Eq. ((4.44)))
, ,1
6 2 MPa0.06 ‰
205 Gaci r
Uniform cooling  induced strains
During the crack formation phase the cracks j = 1 to 20 occur. Assuming that the cracks are not spaced closer than twice the transfer length
is set equal to 1. After a crack j has formed, the steel stresses increase according to (Eq. (4.54))
,II
2 205 GPa1.03 0.724 2 MPa1 1
0.6 % 0.724 6 2 MPaci
s
j
j
until (Eq. (4.45)
,II,
1.03 2 MPa343 MPa
0.6 %s r
is reached (dashed horizontal line in Fig. 4.6 (a))) and the crack j + 1 forms. Accordingly, the crack widths of cracks spaced further apart
than twice the transfer length increase with (Eq. (4.55))
Crack Width
51
22
2
2 205 GPa249 mm 2 MPa 1.03 0.7241 1
205 GPa 0.6 % 0.724 6 2 MPaci j
wj
and remain below (Eq. (4.46) and dashed horizontal line in Fig. 4.6 (c))
249 mm 2 MPa 1.030.4 mm
0.6 % 205 GParw
Note that for a concrete tensile strength of 3 MPa instead of 2 MPa the maximal steel stresses would be 515 MPa instead of 343 MPa and
the maximal crack width 0.6 mm instead of 0.4 mm. The crack formation phase is concluded with 20 cracks when (Eq. (4.61))
, ,
2 MPa 1 0.6 % 2 6 0.6 %0.87 ‰
2 0.6 % 205 Gaci r jn
is reached. With 0.01‰/K this requires a temperature drop of 87 °C.
Uniform shrinkageinduced strains
In this case (Eq. (4.54))
,II
2 205 GPa1.03 0.724 2 MPa1 1 205 GPa
0.6 % 0.724 6 2 MPaci
s ci
j
j
and (Eq. (4.45))
,II,
1.03 2 MPa205 GPa 343 MPa + 205 GPa
0.6 %s r ci ci
include the terms Esci, while the crack width equations remain the same. Free shrinkage strains equal to –0.87 ‰ are necessary to conclude
the crack formation phase. For = 2 % instead of 0.6 % free shrinkage strains of –0.30 ‰ are sufficient to conclude the crack formation
phase.
Continuous EdgeRestraint
The edgerestrained cracking behaviour is influenced by the section thickness h and the bond stresses c along the continuous edge Fig. 4.4 (b). For small thicknesses it makes sense to assume plain sections, while for large c values loadintroduction lengths are negligible. Therefore, three cases are regarded here: Case (a) c ≈ fct and h small (e.g. concrete overlays); Case (b) c ≈ fct/100 and h small (e.g. flat ground slabs); and Case 3(c) c ≈ fct and h large (e.g. base restrained walls). In line with the Tension Chord Model, a rigidperfectly plastic bondslip behaviour is assumed at the restrained edge, leading to constant bond stresses c.
Case (a):
Before cracking R = 1. The stressrelief per crack is purely local and there is no crack formation phase if a constant tensile strength is assumed. The buildup of the concrete stresses on either side of a crack
0
14
ct
c b
fl
h
(4.66)
is established by the bond stresses b between the cracked concrete and the reinforcement as well as by the bond stresses c between the cracked concrete and the baseWith = 0, Eq. (4.66) is also valid for nonreinforced sections where sr = 2 h fct / c. Assuming average steel strains equal to zero, results in crack widths equal to Eq. (4.63). Values for c between different layers of concrete can be found for example in Randl & Wicke (2000).
Example 6
This example discusses the influence of shrinkage on a 10 cm thick, 1 m wide strip of unreinforced overlay concrete. Both the tensile
strength of the overlay concrete and the bond stress c between the overlay and base concrete are assumed to be 2 MPa. Further n = 6 is
adopted. According to Eq. (4.34) with R = 1 all cracks are formed at
Tension Chord Model for Serviceability Problems
52
,
6 2 MPa0.06 ‰
205 Gaci r
with a crack spacing (Eq. (4.66))
2 ctr
c
fs h
between once ( = 0.5) and twice ( = 1) the overlay thickness, corresponding to 100 to 200 mm. Free shrinkage strains equal to
ci = 0.6 ‰ lead to a maximal crack width Eq. (4.63)) of
6 2 MPa200 mm 200 mm 0.6 ‰ 0.03 ‰ 0.1 mm
2 205 GPaciw
Note that the dominant factor in the above equations is the crack spacing. If the overlay thickness is doubled to 20 cm or the bond stress is
halved to 1 MPa, crack widths up to 0.2 mm have to be expected.
Case (b):
Before cracking, the axial force in the member
I cN bx (4.67)
is built up from the free end (x = 0) towards the centre of the member (x = l/2) (Fig. 4.4 (b)). If the length of the member is larger than twice the load introduction length
1ca ci si
c
hEl n
(4.68)
its central sections are fully restrained with NI = –Ecbh [(1– ) ci + nsi]. If la = l/2 is reached before cracking starts, then the bond stresses c are activated over the whole member. In this case the degree of restraint
11
c ci si c
c ci
E n x hR
n E
(4.69)
increases with x and the crack formation process occurs gradually from the middle outwards. The axial force N and the corresponding State II steel strains decrease with increasing distance from the member centre. Assuming s,II = xc/h, Eq. (4.36) leads to
0
12
2ctc
si cis s
f nxw l
h E E
(4.70)
The influence of c on the transfer length is negligible. For ground slabs under selfweight the bond stresses are equal to c = h and Eqs. (4.68) and (4.70) are independent of the slab thickness.
Case (c)
The degree of restraint in uncracked base restrained walls varies over the height and width of the wall. The sections at the bottom of the wall are fully restrained by the base and the cracks only provide local stress relief, so that at the base the cracking behaviour corresponds to Case (a). Not all of the base cracks extend up to the top of the element; the ones that do are denominated primary cracks. The regions around the top wall corners are hardly influenced by the base restraint and they do not crack unless the horizontal reinforcement ratio is very large (see endrestraint for = 0). The wall regions outside the edge and base regions are restrained by the neighbouring wall sections and according to Marti, Sigrist et al. (1997) their cracking behaviour can be modelled with endrestrained tension chords.
Crack Width
53
h
l
lTCh
lTC
(a)
l 8
low restraintcorners
low restraintcorners
(b)
Fig. 4.7 Schematic illustration of tension chord lengths in base restrained walls: (a) long wall (l ∞); (b)short wall (or wall element between joints).
The restraint in the assumed tension chords is reduced by the formation of each crack, meaning that the tension chord length corresponds to the influence region of a crack. In long (l ∞) walls (Fig. 4.7 (a)) the horizontal extent of the stress relieved region belonging to a crack (= tension chord length) is zero at the wall base and increases with increasing distance from the base. In shorter walls (Fig. 4.7 (b)) the tension chords are also limited by the low restraint regions. For long walls (l ∞), Marti, Sigrist et al. (1997) suggest tension chord lengths equal to 2 z, with z being the distance from the base. This assumption is in agreement with the observed primary crack spacing ranging between h and 2h (ACI Committee 207 1990) in unreinforced walls.
4.2.3 Imposed Deformations
Deformationinduced cracking is caused by tension strains e = l/l, which are imposed for example through lateral support movements or shrinkage of stiffer neighbouring members. Once
, ,1ct
e rc
f
E (4.71)
is reached the crack formation phase starts. The cracking process caused by imposed deformations closely resembles the cracking process initiated by restrained deformations for k ∞ and ci = si. During the crack formation phase each crack causes a global stiffness relief defined by
,I ,II ,Is s ss b e
s s s
l l jl lE E E
(4.72)
Eq. (4.48) defines the reduced transfer length, with
,I ,II1s s
n
n
(4.73)
leading to
,II
1 21 1ct c e
sct
f n E
f
(4.74)
and
22
0 1 21 1ct s e
s ct
l f n Ew
E nf
(4.75)
Tension Chord Model for Serviceability Problems
54
Eqs. (4.74) and (4.75) are valid for = 1 and correspond to Eqs. (4.54) and (4.55) for ci = si= e. Accordingly, during crack formation the steel stresses and crack widths remain below
,II, 1cts r
fn
(4.76)
and
02 1ctr
s
l f nw
E
(4.77)
and start to increase with
,II 12
cts s e
fE
(4.78)
and
022
cte
s
nfw l
E
(4.79)
for stabilized cracking once
, , I2 12
cte r jn
s
fa
E
(4.80)
4.3 Deflections
00
load
deformation
cracking
yieldinguncracked elastic (I)
cracked elastic (II)
Fig. 4.8 Basic loaddeformation behaviour of a flexural member.
Together with the cracking load and the yield load, the deflections
2aa kl (4.81)
determined with a constant uncracked (State I) or cracked (State II) elastic stiffness provide a good basis for deflection estimates (Fig. 4.8). However, in many cases, the actual deflections have to be located somewhere between these two limiting cases, as most members have both uncracked and cracked regions. Further, depending on the load case, tension stiffening, longterm effects and variable section properties, as well as statically indeterminate moment redistributions due to nonuniform stiffness distributions (e.g. due to cracking or curtailed reinforcement) may need considering. With
Deflections
55
Eqs. (4.7) and (4.14), the Tension Chord Model provides the section equations for considering tension stiffening.
For general section properties, the integral member deformations (e.g. deflection or rotation) of oneway bending members
M l d (4.82)
result from integrating the section curvatures, for example with an equivalent statical system featuring a unit load/moment located at the section and in the direction of the required deformation. If the moment distribution is stiffnessdependent Eq. (4.82) can also be used to determine the moment redistribution coefficient
,
1 a
a el
M
M (4.83)
by enforcing a kinematic boundary condition (e.g. zero rotation at a clamped end or zero deflections at a supported end). Table 4.1 summarizes the section moments and integration parameters for the basic structural systems illustrated in Fig. 4.9.
Static system M ,a elM 1k 2k 0
Q
ξ , 2a elM
4
Ql
1
12
1
8
Q QξQl
ξ , a el Q
Q
M
QQl 23 4
24Q
1
8
q
ξ 2
, 4 4a elM 2
8
ql
5
48
1
8
Q
ξ , 1a elM Ql
1
3
1
2
q
ξ 2
, 1 2a elM 2
2
ql
1
4
1
2
Q
ξ , 1 4a elM
8
Ql
1 3
24
2
0
1
8
1
4
q
ξ 2
, 1 6 6a elM 2
12
ql
1 4
32
2
0
1
8 1 1
2 12 6
Q
ξ 11
, 31a elM 3
16
Ql
7 15
144
2
0 0
1
8
3 1
11 3
q
ξ 2
, 1 5 4a elM 2
8
ql
1 2.5
24
2
0 0
1
8
1
4
Table 4.1 Moment distribution, elastic moment at critical section, midspan (free end) deflection integration factors k1 for a constant member stiffness and k2 for a constant curvature distribution ( and in negative and positive moment regions, respectively) and location where moment is zero. Notethat = x/l according to Fig. 4.9.
Tension Chord Model for Serviceability Problems
56
4.3.1 Interpolation Equations
Interpolation equations are a wellknown tool for determining the momentinduced deflections
1 I 1 II1a a a (4.84)
of partially cracked flexural members with constant State I and State II stiffnesses. Effectively the State II stiffness is only strictly constant in symmetrically reinforced members, or, if the transition zones are neglected, in members with equally reinforced span (M > 0) and support (M < 0) sections (i.e. sup = span and 'sup = 'span). In contrast to most interpolation coefficients (see Chapter 2.2.2), the interpolation coefficients suggested in Table 4.2 are systemdependent (see Fig. 4.10). They were directly derived from Eq. (4.82) and are expressed as a function of
,
r
a el
M
M (4.85)
Eq. (4.81) with k1 (Table 4.1) and a equal to the absolute value of the critical section curvature (Fig. 4.8) provides the State I and State II deflections. If creep needs to be considereda can be determined with the effective stiffness according to Eq. (3.65).
h
(a)
ξ a
ξrM
χ
Ma
hξ a
ξr,1
ξr,2M
χ
ξ0
Δχts
Ma
ρ
+
+
ρ’
Δχts
ξ a
M
χ
Ma 
Δχts
hξ a
M
χ
Ma
+ξr,1
ξr,2 ξr,3
Δχts
ξ0
q
q
q
q
l
Ma+
Ma 
Ma
χa
χa
χa
χa
(b)
(c) (d)
h
Fig. 4.9 Moment and curvature distributions for the four structural systems regarded in this chapter. Theregions where M > Mr are marked in gray. The tensile and compression reinforcement is illustrated with continuous and dashed lines, respectively. = x/l = 0…0.5 in Figs. (a) and = x/l= 0…1 in Figs. (b) to (d).
It is also possible to use interpolation equations for determining the tension stiffening deflection reduction
2 ,II1ts tsa a (4.86)
and the shrinkage deflections
Deflections
57
2 ,I 2 ,II1sh sh sha a a (4.87)
for partially cracked members with constant State I and State II stiffnesses. Table 4.2 provides the interpolation coefficient . The absolute curvatures  are constant and Eq. (4.81) with k2 (Table 4.1) yields ats,II, ash,II and ash,I. Thereto, the Tension Chord Model provides ts (Eq. (4.7) or (4.14)), while Eqs. (3.67), (3.69) and (3.70) provide the shrinkage curvatures. Independent of the method chosen for determining the State II shrinkage curvature the superposition of Eqs. (4.84) and (4.87) represents an estimation, as the interaction of creep and shrinkage on the height of the compression zone is not considered.
By reducing the cracking moment
I,
I,
ct sh efr
ef
f IM
h x
(4.88)
with sh according to Eq. (3.68) shrinkageinduced cracking can be accounted for in factor .
Static system r
Q
2
3 2
Q Q
ξQl Q
3 2
2
8
3 4Q
Q
2 24 Q
q
11 1
2 316 4 3
5r r
24 r
Q
1 3 2
q
1 2
Q
1
4 4
3 2
q
< 0.5+
1 1
2 12 6 6
,2 ,1
,1 ,2
81 2
3 1 4
3 1 2 1 2
r r
r r
0 ,1 ,2
0
12 2
4 7 24r r
Q
< 5/6+
31
11 3
33
2
864
7 15 3 11
22
2
72
71 9 126
q
< 0.5(1+
29 6 165
8 8
2
,2 ,1
,1 ,2
(1 )3
8 2 5
5 8 5 8
r r
r r
,1 ,2
2
1 2 2 1
2 1r r
Table 4.2 Midspan (or free end for the cantilever) deflection interpolation coefficients for cracked flexuralmembers with constant State I and State II stiffnesses (1) or constant absolute curvatures (2). = MrMa,el ranges between 1 and 0 unless stated otherwise. For the clampedended beam and the propped cantilever, cracked span sections are assumed.
Provided that a constant cracked stiffness can be assumed, the interpolation Eqs. (4.84) to (4.87) consider cracking, tension stiffening and longterm effects. This makes them particularly suitable for thin lightly reinforced flexural members with similar, noncurtailed support and span reinforcement, as in this case the contribution of the uncracked sections and tension stiffening are important factors
Tension Chord Model for Serviceability Problems
58
(see e.g. Fig. 6.14). Even in members with constant tension and compression reinforcement ratios there are still statically indeterminate moment redistributions (≠ 0due to cracking and shrinkage. These moment redistributions can either be estimated numerically with Eq. (4.82) or neglected (= 0, taking into account that compatibility is not fulfilled.
100
0.8 0.6 0.4 0.2 0
ζ 1
0
0.2
0.4
0.6
0.8
1.0
000
& EC 2
bilinear
Mr
Ma,el
Fig. 4.10 Contribution of the uncracked member regions 1 (Table 4.2) for partially cracked members withconstant section properties. For the clampedended beam and the propped cantilever it is assumedthat the support and span sections are cracked and = 0.
Example 7
This example illustrates how the interpolation coefficients given in Table 4.2 are used to determine the longterm deflections of a 4 m (l/h =
8) cantilever with a sustained uniform load (inclusive selfweight) of 30 kN/m corresponding to 75 % of the yield load. The cantilever
sections correspond to the section illustrated in Fig. 3.4 (upside down) with the section properties determined in Example 2 and Example 3.
According to Table 4.2 the shortterm elastic cantilever deflections at the free end are
4 4
I 2
30 kN/m 4 m12 mm
8 79378 kN ma
and
4 4
II 2
30 kN/m 4 m28 mm
8 33787 kN ma
With fct = 3 MPa, Mr = 29.5 kNm and = 1, Eq. (4.7) leads to
2
1 29.5 kN m 6 3 MPa mrad0.27
2 33787 kN m 205 GPa 0.85 0.5 m 0.163 m mts
and the tension stiffening deflections
2 2
,II
4 m mrad0.27 2.2 mm
2 mtsa
Interpolating with
2 2
29.5 kNm0.123
0.5 30 kN/m 4 m
and the coefficients (Table 4.2)
21
2
0.123 0.015
0.123
leads to
0.015 12 mm 1 0.015 28 mm 1 0.123 2.2 mm 25 mma
Deflections
59
As shrinkage strains equal to 0.6 ‰ cause tensile stresses sh, = 3.3 MPa (Eq. (3.68)) in the extreme concrete fibres, the whole
cantilever is assumed to be cracked for the longterm deflection predictions. The cracked elastic deflections
4 4
II 2
30 kN/m 4 m49 mm
8 19496 kN ma
and with Eq. (4.14) and k = 1/4
2
29.5 kN m 0.85 0.5 m 0.163 m1 1 6 3 MPa mrad0.11
2 4 33787 kN m 0.85 0.5 m 0.260 m 205 GPa 0.85 0.5 m 0.260 m mts
the tension stiffening deflection reduction
2 2
,II
4 m mrad0.14 0.9 mm
2 mtsa
and finally with sh = 1.77 mrad/m (Eq. (3.69) the State II shrinkage deflections
2 2
,II
4 m mrad1.77 14 mm
2 msha
lead to deflections
49 mm 0.9 mm 14 mm 62 mma
EC 2 and MC 2010 (European Committee for Standardization 2004; Fédération Internationale du Béton 2010b) both recommend a
limit of span/250 for the sag of a beam under the quasipermanent combination of loads (for the cantilever 2 · 4 m / 250 = 32 mm). The sag
is assessed relative to the supports and span refers to the distance between the supports. A limit of span/500 (= 16 mm) is suggested for the
deflections, which occur after any deformationsensitive adjacent members (e.g. claddings) have been fitted. Further, precamber can be
provided to compensate maximal span/250 = 32 mm. For the example cantilever this means that with a camber of 30 mm the first limit can
be fulfilled. However, the second limit cannot be fulfilled, unless half of the longterm deflections are awaited before any deformation
sensitive adjunct members are fitted.
4.3.2 Influence of Reinforcement Detailing
In most practical cases the flexural reinforcement is curtailed and the cracked stiffness is not constant. Fig. 4.11 illustrates the influence of the reinforcement detailing on the moment redistribution coefficient (Eq. (4.83)) and related deflections
II
II,avg
a
a (4.89)
for a fully cracked clampedended beam and a propped cantilever as a function of the stiffness ratio. Positive values indicate larger span moments, while negative values indicate larger support moments relative to the elastic moment distribution. The stiffness ratio
II,sup
II,span
c
c
E I
E I (4.90)
is defined by the stiffnesses in the critical support and span sections. For both structural systems the figure illustrates two limiting situations: A perfectly curtailed reinforcement with a cracked stiffness affine to the moment distribution (crosses) and a noncurtailed reinforcement distribution with EcIII,sup and EcIII,span in the positive and negative moment sections (continuous lines). The average stiffness deflections aII,avg were determined with Eq. (4.81) and the average cracked stiffness 0.5 (EcIII,sup + EcIII,span), while aII and were determined with Eq. (4.82). The affine stiffness distribution leads to support moments that are 12.5% and 17.2% larger than according to the elastic moment distribution. Tension stiffening and shrinkage are neglected, while creep is implicitly considered within . As can be seen from Fig. 4.11, the stiffness ratio strongly influences the moment redistribution coefficient
Tension Chord Model for Serviceability Problems
60
Fig. 4.11 (a), while the extent of the reinforcement curtailing has a considerable influence on the size of the State II deflections (Fig. 4.11 (b)).
1
1
0
2
1
01
1
2 4 6 00
2 4 6
2
1
1M
a
Ma,
el1
Ma
Ma,
el 0
0
aII
aav
gII
,
aII
aav
gII
,
III,supEIII,spanEc
c III,supEIII,spanEc
c
(a)
(c)
(b)
(d)
Fig. 4.11 State II moment redistributions and their influence on the deflections: (a) & (b): clampedendedbeam with a uniform load; (c) & (d) propped cantilever with a uniform load. The affine stiffnessdistribution is marked with crosses, while the constant stiffness distribution is marked with lines.
Based on Fig. 4.11 it is therefore suggested that for flexural elements with strongly curtailed reinforcement the influence of the uncracked sections is neglected and a constant cracked curvature a = Ma,el/EcIII,a is assumed in the cracked sections, so that the controlling deflections can be estimated with
2 II1a a (4.91)
The State II deflections aII result from Eq. (4.81) with k2. In this case the tension stiffening curvature reduction is variable and the corresponding deflection reduction has to be determined by integrating the individual curvatures. However, in beams with large reinforcement ratios, where curtailing is most likely necessary, the loadlevels are usually high and thus tension stiffening is less important (see e.g. Fig. 6.14). Note that in statically indeterminate systems 2 is dependent on . For initially restraint free (ci = si = 0) cracked (fct = 0) members with affine reinforcement distributions is equal to 0.125 if both ends are clamped (0 = 0.5) or 0.172 if one end is clamped and one end supported (0 = 120.5/2). Other values for have to be estimated or determined with Eq. (4.82).
Deflections
61
4.3.3 SpantoDepth Ratios
000000
10
20
30
40
50
00
ρ
0
l
00001 2 3
10
20
30
40
50
0 1 2 3
= 6nconstant EI
= 6nχ= 18n
= 18nconstant
(a) (b)
(c) (d)
[%] ρ [%]
dl d = 6nconstant EI
= 18n
= 6nχ= 18n
constant
= 6nconstant EI= 18n
= 6nχ= 18n
constant
= 6nconstant EI= 18n
= 6nχ= 18n
constant
l l
l l
Fig. 4.12 Spantodepth ratios (Eq. (4.94)) for maintaining a/l ≤ 1/240 (1/320) at midspan (or cantilever end)up until reaching 80% (60%) of the characteristic yield moment in the critical section: (a) cantilever; (b) simple beam; (c) propped cantilever; (d) clampedended beam. Note: Es = 205 GPa, fsy
= 500 MPa, fct = 2 MPa, d/h = 0.85, d'/h = 0.15, ' = 0.25 and mr = fct/6.
Combining Eqs. (4.81) and (4.84) and neglecting the contribution of the curvatures in the uncracked member regions as well as shrinkage, leads to the midspan (or cantilever end) deflection equation
2,
II,
1 a el
a
k l Ma
EI
(4.92)
where the subscript a denotes the section with the largest moment Ma,el. This equation can be used with k = k1 or k2 and 1 or 2 (Table 4.1 and Table 4.2) in order to capture the two limiting detailing options of a constant cracked stiffness (constant EI) and an affine cracked stiffness (constant ). With Ma,el = My, My = my bd2, Mr = mr bh2 and III,a = bd3 gII,a (Table 3.1), Eq. (4.92) is rearranged to form the limiting span to depth ratios
IIlimlim 1
s
y
a l g El d
m nk
(4.93)
Tension Chord Model for Serviceability Problems
62
where the interpolation coefficient is a function of the moment ratio (Eq. (4.85))
2r
y
m
m d h
(4.94)
If creep needs to be considered, gII and n in Eq. (4.93) are determined with the effective modulus (Eq. (3.65)).
Fig. 4.12 illustrates the limiting spantodepth ratios for rectangular sections for (a/l)lim = 1/240 at = 0.8. This limit is equivalent to (a/l)lim = 1/320 at = 0.6 or (a/l)lim = 1/192 at = 1. ACI 318 (ACI Committee 318 2008) recommends (a/l)lim = 1/240 for the deflections occurring after the attachment of nonstructural elements (sum of the longterm deflection due to all sustained loads and the immediate deflection due to any additional live load) for floor constructions supporting or attached to nonstructural elements not likely to be damaged by large deflections.
4.4 Summary
Crack widths in members with uniaxial stress states are defined by Eq. (4.24). For maximal crack widths is set equal to 1, while k can be chosen between 1 (full tension stiffening according to the Tension Chord Model) and zero (no tension stiffening). The State II steel strains are determined as described in Chapter 3. For specific cases simplified equations can be provided:
For bending members with axial force, Eq. (3.74) with an effective reinforcement ratio according to Eq. (4.9) defines the transfer length. The required section properties and deformations at cracking have to be determined with the section equilibrium equations according to Chapter 3.
For bending members without axial force Eq. (4.27) provides the crack width, while Eq. (4.28) provides the transfer length.
For axially loaded tensile members Eq. (4.36) provides the crack width, while Eq. (3.74) provides the transfer length.
For elastically endrestrained tensile members Eqs. (4.45) and (4.46) (with Eq. (3.74)) provide an upper limit for the steel stresses and crack widths during the crack formation phase. The crack formation phase is delimited by Eqs. (4.44) and (4.57).
For continuous edgerestrained concrete overlays Eq. (4.66) provides the transfer length, while Eq. (4.63) provides the crack width.
For continuous edgerestrained walls the lengths of the fictitious tension chords are estimated according to Fig. 4.7. The fictitious tension chords can then be approximately treated as endrestrained tensile members.
For tensile ties under imposed deformations Eqs. (4.76) and (4.77) (with Eq. (3.74)) provide an upper limit for the steel stresses and crack widths during the crack formation phase. The crack formation phase is delimited by Eqs. (4.71) and (4.80).
Beam deformations are defined by Eq. (4.82), which can also be used to determine the moment distribution in statically indeterminate members. The State I and II section curvatures are determined according to Chapter 3. Tension stiffening is accounted for by including the additional force provided by the average concrete tensile stresses (see Eq. (4.1)) and the effective concrete area (Eq. (4.8)). For specific cases simplified equations can be provided:
Summary
63
For beams (N = 0) with uniform stiffnesses (State I or State II), Eq. (4.81) with Table 4.1 provides the midspan (or free end) loadinduced deflections, as well as additional shrinkage deflections (with Eq. (3.67)) and deflection reductions due to tension stiffening (with Eq. (4.7)).
For partially cracked beams (N = 0) with uniform State I and II stiffnesses, the State I and II deflections can be interpolated according to Eqs. (4.84), (4.86) and (4.87). Thereto Table 4.2 provides the system dependent interpolation coefficients. For statically indeterminate systems the moment redistributions due to cracking have to be neglected or determined with Eq. (4.82).
For extensively cracked beams (with N = 0) with strongly curtailed tensile reinforcements, the loadinduced deflections can be estimated with Eq. (4.91). For statically indeterminate systems the moment redistributions due to cracking have to be determined with Eq. (4.82).
65
5 Verification
So far, in terms of serviceability behaviour, mainly shortterm test data validations at section and member level have been carried out for the Tension Chord Model. Sigrist (1995) found a good agreement between the deflection measurements from his test specimens (Sigrist and Marti 1993) and the corresponding calculated deflection curves. With Bragg grating sensor measurements Kenel and Marti (2002) showed that a linear steel strain distribution between the cracks is a reasonable assumption. Kenel also carried out test data comparisons for load deformation curves with a selection of shortterm test series (Polak and Killen 1998; Pfyl and Marti 2001; Kenel and Marti 2002) with lightly reinforced specimens.
This chapter is focused on longterm serviceability behaviour and aims at validating the prediction approaches discussed in Chapter 4. Thereto a selection of test series from various research institutions is used. Appendix A contains an overview of the test data. An example calculation is provided for most test series. Some of the test data comparisons also include predictions carried out with the code equations discussed in Chapter 2.
5.1 Tensile Members
5.1.1 Loss of Tension Stiffening
1200
70
10
D15 & D8
N
( )a
885
100
ST1ST3( )b
N
N
1200
120
T16B1B3( )c
N
N
T20B1B3
Ø 12Ø 16/20Ø
N
Fig. 5.1 Longterm tensile tests: (a) Günther and Mehlhorn (1989); (b) Scott & Gill (1990); (c) Beeby andScott (2006). The dimensions are in [mm].
As longterm effects influence the deformation behaviour of both the compression and tension chord, it is not convenient to experimentally determine the longterm loss of tension stiffening from bending tests. Therefore, the longterm tensile tests illustrated in Fig. 5.1 (see also Table A. 1 in Appendix A) are used to experimentally determine the quotient of the longterm and immediate bond stress k (Eq.
Verification
66
(4.11)). kts,/ts= (s,II – s,avg,)/(s,II – s,avg) is determined from the calculated State II strains and the average strain measurements after immediate and sustained loading. The bond stress quotient is plotted versus time (Fig. 5.2 (a)) and versus the MC 90 creep coefficient (Eq. (3.36)) (Fig. 5.2 (b)), assuming RH = 0.4. Fig. 5.2 (b) also illustrates the bond stress quotient according to Eq. (4.11) as well as according to Model Code and Eurocode 2 (k = 0.4/0.6 = 0.67, see Eq. (2.6)).
0
0.2
0.4
0.6
0.8
1.0
τϕ
001800
060 120
ST2ST3
ST1
T16B1
T16B3T16B2
T20B3
T20B1
T20B2
D1
D4
D8
[d]tt0
D2 D5D3
b, τ b
0ϕ
1 2 3 4
D1
D4
D2D5D3
D8
ST1
ST2ST3
T16B1
T16B2T16B3
T20B1
T20B2
T20B3
MC, EC 2
(a) (b)
kϕ
Fig. 5.2 Loss of tension stiffening in the tensile tests illustrated in Fig. 5.1: (a) vs. time; (b) vs. , where is estimated according to Eq. (3.36) assuming RH = 0.4 and 13 = 1.
The short specimen lengths and the large reinforcement ratios do not facilitate the delicate task of estimating the tension stiffening steel strain reductions from the measured average steel strains and the calculated State II steel strains. Further, the calculated State II steel strains are slightly underestimated as the shrinkageinduced compression steel strains, which are released at cracking (see specimen RL1 in Chapter 5.1.2) are neglected. This means that if the restrained shrinkage strains released at cracking are larger than the steel strain reduction, then the tension stiffening values obtained will appear negative (see Heinzmann 2006). This is the case for Specimens D6 and D7 (not plotted in Fig. 5.2).
5.1.2 Restrained Deformations
EndRestrained Shrinkage Specimens Tested at the University of New South Wales
Nejadi and Gilbert (2003) tested eight (S1a/b to S4a/b), very lightly reinforced endrestrained specimens with 2 m long test lengths and variable reinforcement ratios (Fig. 5.3 and Table A. 2 in Appendix A). A section reduction at midlength defined the location of the first crack. Fig. 5.4 compares the predicted and experimental State II steel stresses and crack widths. The experimental State II steel stresses are determined from the average of nine strain gauge measurements taken within 50 mm of the first crack. The experimental crack widths represent the maximum crack opening observed at t = 122 d or t = 150 d (S2b). The free shrinkage strains (see Fig. 5.5) were measured on companion specimens (600/600/100 mm) with the same section dimensions as the test specimens.
All predictions are carried out according to Chapter 4.2.2 (see example below for specimen S1) with the 28day concrete properties of batch I unless mentioned otherwise. Any strains caused by the loss of hydration heat are neglected (i.e. ci = sh and si = 0), the axial restraint stiffness k is as
Verification
67
sumed to be ∞ and creep is neglected, leading to R = 1. The numbered vertical lines in Fig. 5.4 indicate that a new crack has formed.
2000
1000
4660
(a)
600100
(b)
100
600
185
S1
100
185
S2
10010Ø
300
S3
100
120
S410Ø
10Ø
12Ø
(c)
12Ø
10Ø
10Ø
10Ø
Fig. 5.3 Overview of Nejadi and Gilbert's (2003) shrinkage tests: (a) plan view; (b) elevation; (c) sectionsof specimens S1 to S4. The specimens were made in pairs, e.g. S1a and S1b. The dimensions arein [mm].
Predictions test specimen S1
With R = 1 and the 7day concrete properties (N.B. also with the 28day properties), the crack formation phase starts at (Eq. (4.44))
1.55 MPa 120.09 ‰
205 GPash
The transfer length (Eq. (3.74))
0
12 mm 1 0.565 %264 mm
8 0.565 %l
leads to initial crack influence regions equal to 528 mm ( = 1) and a final crack spacing between 264 and 528 mm ( = 0.5 to 1). = 1 is
used for the following calculations. The end of the crack formation phase at (Eq. (4.61) with aI = 1.045)
1.97 MPa2 1.045 1 0.565 % 0.93 ‰
2 0.565 % 205 GPash
with at total of (Eq. (4.58))
2 m1 5
528 mmnj
cracks is not reached. The additional crack is added to account for the first edge crack at the beginning of the instrumented length.
During the crack formation phase the ascending steel stress curves (Eqs. (4.54) and (4.45) with aI = 1.045) are defined by
,II
2 205 GPa1.045 1.97 MPa 1.045 1.97 MPa1 1 205 GPa 205 GPa
0.565 % 9 1.97 MPa 0.565 %sh
s sh sh
where (Eq. (4.51))
9 0.565 % 5
1 0.565 %j
The crack number is defined by j (1 to jn). The corresponding crack widths (Eqs. (4.55), (4.46))
22 2 205 GPa264 mm 1.97 MPa 1.045 264 mm 1.97 MPa 1.045
1 1 0.47 mm0.565 % 205 GPa 9 1.97 MPa 0.565 % 205 GPa
shw
are expected to remain below 0.47 mm. In Fig. 5.4 the upper limits on the right hand side of the above equations for s,II and w are illus
trated with dashed lines.
Verification
68
0
500
250
0
w[m
m]
0.39 %
000
0.2
0.4
0.6
0.8
1
000
test S2btest S2a
0
500
250
0
w[m
m]
0.26 %
000
0.2
0.4
0.6
0.8
1
000
test S3atest S3b
0
500
250
0
w[m
m]
0
0.52 %
000
0.2
0.4
0.6
0.8
1
0000.125 0.25 0.375 0.5
εsh [ ]0
εsh [ ]
σ s,
[MPa
]II
σ s,
[MPa
]II
σ s,
[MPa
]II
test S4a
test S4b
1
2
1
2
1
1
1
23
1
3
0 0000000
0
500
250
σ s,
0
w
[MPa
]
[mm
]
test S1a
test S1b
0.57 %
000
0.2
0.4
0.6
0.8
1
000
II
1
23
1
2
3
 
test S2b
0.125 0.25 0.375 0.5
2
test S2a
test S3b
test S3a
2 m
predicted
predicted
predicted
test S4atest S4b
predicted
predicted
predicted
test S1b
test S1a
predicted
predicted
(a) (b)
(c) (d)
(e) (f)
(g) (h)
Fig. 5.4 Nejadi and Gilbert's (2003) endrestrained shrinkage specimens. The predicted curves use the 28day concrete properties of batch I and = 1.
Verification
69
00
ε sh
[
]
0
0.6
0.3

15050 100[d]t
I
II
0.09
8
Fig. 5.5 Shrinkage strains measured on Nejadi and Gilbert's (2003) 600/600/100 mm shrinkage specimensfor Batch I and Batch II concrete. The predicted start of the crack formation phase 0.09 ‰ isreached at 8 days (dashed line).
According to Fig. 5.5 the predicted start of the crack formation phase sh = 0.09 ‰ is reached at 8 days. By this time all specimens except S1b have cracked (see experimental steel stresses in Fig. 5.4). Even though earlyage creep is neglected, the predictions do not underestimate the cracking age.
The end of the crack formation phase is not reached by any of the specimens. At 122 days (0.46 ‰ free shrinkage strains) Specimen S3a has one large crack, while Specimen S3b has two cracks (one crack is predicted). The short specimen length (2 m), which is responsible for the large stiffness loss at first cracking, is the only reason the experimental steel stresses in S3a/b remain below the yield limit. In a longer member, such a low reinforcement ratio would lead to steel yielding (see Fig. 5.6). Specimens S2a/b and S4a/b end up with three cracks (2 are predicted for S2 and three are predicted for S4), while four cracks can be observed on the S1 specimens. All of the observed cracks penetrate through the full depth of the specimen crosssections.
0
1000
500
l = 2 m
0 0.25 0.50 0.75 100.25 0.50 0.75 10εsh [ ] εsh [ ] 
σ s,
[MPa
]II
(a) (b)
l = 10 m
Fig. 5.6 Influence of the member length on the steel stress development of an endrestrained tension chord:(a) specimen S3 with its original length of 2 m; (b) Specimen S3 with an assumed alternativelength of 10 m.
Verification
70
Continuous edgerestrained walls
Al Rawi and Kheder tested 14 (Al Rawi and Kheder 1990) and 8 (Kheder 1997) small scale baserestrained mortar walls and observed 37 (Kheder 1997) full size walls under shrinkage. Unfortunately, the material properties given in the papers are insufficient for recalculations; however the qualitative results are summarized here.
Kheder's (1997) mortar walls have l/h ratios of 2 (4 walls) and 3 (4 walls) and horizontal reinforcement ratios of 0.2 % and 0.8 %. All eight walls have crack free top corner regions as illustrated in Fig. 4.7 (b). This observation illustrates the influence region of an unrestrained edge or crack and agrees with the model assumption of a crack influence region (fictitious tension chord length), which increases from zero at the base to 2 h at the wall top (see continuous edgerestraint Case (c) Chapter 4.2.2).
Further, the walls feature closely spaced base cracks that are slightly further apart and wider in the walls with lower horizontal reinforcement ratios at the base. The largest crack widths observed on Kheder's mortar walls occur in the bottom quarter of the walls. This coincides with Al Rawi and Kheder's (1990) findings. They observed maximal crack widths somewhere at midheight of short walls as opposed to at the top of long walls. These findings support the model assumption of endrestrained tension chords with crack widths that fluctuate between a maximum and minimum value (see Fig. 4.6 (b)). While the former is primarily defined by the horizontal reinforcement ratio, the latter increases with increasing tension chord length (see Fig. 5.6). As the longest fictitious tension chords are located at the top of long walls and somewhere in the middle of short walls (see Fig. 4.7), the chances of finding the largest crack widths at these locations are high. All tests support the notion that it is practically impossible to prevent base cracks, which even for joints spaced at 2 h were observed (Kheder 1997) until part way up the wall.
5.1.3 Imposed Deformations
Deformation Controlled Tensile Tests carried out at EPF Lausanne
2500
450
(a)
1000
instrumented
160
8Ø
B11
(b)
120
8Ø
190
10Ø
120
10Ø
450 450 450 450
B12 B13 B14
150
lengthinstrumentedlength
6 8 6 88Ø6 8Ø8 10Ø6 10Ø6 10Ø8
Fig. 5.7 Overview of four deformation controlled tensile tests carried out by Jaccoud et al. (1984): (a) planview; (b) sections of specimens B11 to B14. The imposed deformations were controlled withinductive displacement transmitters over a length of 1 m. The dimensions are in [mm].
Verification
71
0
800
400
0
w[m
m]
0.45 %
000
0.2
0.4
0.6
0.8
1
000
0. 45 %
σ s,
[MPa
]II
test B11
0
800
400
0
w[m
m]
0.70 %
000
0.2
0.4
0.6
0.8
1
000
0.70 %
σ s,
[MPa
]II
crack 36, test B11
crack formation stabilized cracking
0
800
400
0
w[m
m]
0. 93%
000
0.2
0.4
0.6
0.8
1
000
0. 93%
σ s,
[MPa
]II
0εe[ ]
01.50.5 1.0εe[ ]
1.50.5 1.0
0
800
400
0
w[m
m]
0.60 %
000
0.2
0.4
0.6
0.8
1
000
0.60 %
σ s,
[MPa
]II
crack 12 test B12
test B12
predicted
predicted
predicted
predicted
predictedtest B13 predicted
crack 36 test B13
test B14predicted
crack 13 test B14
predicted
predicted upper limit(a) (b)
(c) (d)
(e) (f)
(g) (h)
Fig. 5.8 Jaccoud et al.'s (1984) deformation controlled tensile members. The vertical dashed lines illustratethe predicted ( = 1) transition between the crack formation phase and stabilized cracking phase.
Verification
72
Jaccoud et al. (1984) performed 12 deformationcontrolled tests on lightly reinforced concrete tensile elements (see Table A. 3 in Appendix A). Four of them (all from the B1Series) are illustrated in Fig. 5.7 and used for the test data comparisons in Fig. 5.8. The imposed deformations were controlled with inductive displacement transmitters over a length of 1 m. The corresponding average strains are illustrated together with the experimental State II steel stresses and the opening of the largest crack in Fig. 5.8. The figure also illustrates the corresponding predictions based on Chapter 4.2.3 (see example B14). The predicted curves are based on a tension chord length equal to 1 m, corresponding to the length of the inductive displacement transmitters used to control the deformations. While the length of the tension chord has no influence on the strains necessary to start and end the crack formation phase, it does define the final amount of cracks and therefore the strain difference between two consecutive cracks. The tension chord length also has no influence on the maximal steel stresses and crack widths during or after the crack formation phase.
The positive influence of the reinforcement ratio on the State II steel stresses and crack widths during the crack formation phase is clearly visible in Fig. 5.8. However, the specimens with higher reinforcement ratios have a shorter crack formation phase, so that in the case of large imposed deformations, the positive influence of the additional reinforcement is at least partially lost once the crack formation phase is concluded (i.e. compare Fig. 5.8 (f) and (h)).
Predictions test specimen B14
The crack formation phase starts at
2.43 MPa 6.40.08 ‰
205 GPae
and ends at (Eq. (4.80) with Eq. (4.39))
2.43 MPa1 2 6.4 0.93 % 0.93 % 0.71 ‰
2 0.93 % 205 GPae
With a transfer length (Eq. (3.74))
0
10 mm 1 0.93 %133 mm
8 0.93 %l
and a maximal crack spacing of 266 mm ( = 1), a total of (Eq. (4.58))
1 m4
266 mmnj
cracks is necessary to conclude the crack formation phase. With j equal to the crack number, factor
6.4 0.93 %
1 0.93 %nj
j
During the crack formation phase the steel stresses (Eqs. (4.74) and (4.76) with aI = 1.050)
,II
2 205 GPa1.050 2.43 MPa 2.43 MPa 1.0501 1 274 MPa
0.93 % 6.4 2.43 MPa 0.93 %e
s
remain below 274 MPa, while the crack widths (Eqs. (4.75) and (4.77))
22 2 205 GPa133 mm 2.43 MPa 1.050 133 mm 2.43 MPa 1.050
1 1 0.18 mm0.93 % 205 GPa 6.4 2.43 MPa 0.93 % 205 GPa
ew
remain below 0.18 mm. In Fig. 5.8 the two upper limits on the right hand side of the equations for s,II and w are illustrated with dashed
lines. Once the crack formation phase is concluded the steel strains (Eq. (4.78))
,II
2.43 MPa 1 0.93 %205 GPa 129 MPa 205 GPa
2 0.93 %s e e
and crack widths (Eq. (4.79))
6.4 2.43 MPa266 mm
2 205 GPaew
start to increase.
Verification
73
5.2 Beams
5.2.1 Statically Determinate Beams
Espion et al. (Espion 1988; Espion and Halleux 1990) provided a detailed summary of longterm oneway bending tests carried out between 1907 and 1988. A selection of recent test series with complete sets of measured concrete properties is used for the test data comparisons carried out in this chapter. Further, the predictions of two large beam specimens, belonging to the French benchmark program ConCrack (NECS 2010) are included.
Unless mentioned otherwise, the Tension Chord Model (TCM) deflection predictions are determined with the interpolation equations given in Chapter 4.3.1, using the interpolation coefficient corresponding to the predominant load. The TCM crack widths are determined with the equations given in Chapter 4.2.1 and unless mentioned otherwise represent the crack openings at the height of the centroid of the tensile reinforcement. The deflections are assumed to be zero at the beginning of loading. Most of the predictions assume = 1 (maximum crack spacing). Factor k = 0....1 is used according to Chapter 4.1.2 to indicate the contribution of the tensile concrete between the cracks.
For comparison, code crack width (see Chapter 2.1) and deflection (see Chapter 2.2) predictions are included in some of the figures. The deformation predictions referred to as ACI use Branson's effective moment of inertia according to Eq. (2.16) with m = 3 or 4. The deformation predictions referred to as EC use Rao's interpolation coefficient according to Eq. (2.17) or (2.24). The Frosch crack widths refer to Eq. (2.12) with either the bottom (Eq. (2.13)) or side (Eq. (2.14)) transfer length, where there is no distinction between the short/longterm predictions. The crack widths denominated MC refer to Eq. (2.6) with Eq. (2.8) with parameters 1 = 0, 2 = 0.5 as well as 3 = 0.6/0.4 and 4 = 0/1 for short/longterm predictions.
ShortTerm 4PointBending Tests carried out at ETH Zurich
200
125
1000
1200 1200 1200
Q Q
200
250
1000
200
B1 & B3
10Ø
B4 & B5
10Ø14Ø
118
28
57.5
28 or
(a)
(b)
8 44
10Ø8 10Ø14Ø
or44
Fig. 5.9 Overview of Kenel and Marti's (2002) bending tests: (a) structural system; (b) sections. The dimensions are in [mm].
Kenel and Marti (2002) tested five thin, lightly reinforced slab strips (B1 to B5) with two different reinforcement ratios and concrete types under shortterm fourpointbending. Fig. 5.10 illustrates the section and midspan member deformations of specimens B1, B3 and B4 (the prestressed specimen B2 is not considered). The experimental section curvatures (marked by crosses) are taken from Fig. 4.16 in Kenel (2002), while the measured midspan deflections (labelled test) are obtained from Figs. 5.2 (b), 5.14 (b) and 5.21 (b) in Kenel and Marti (2002). The measured crack widths (marked by crosses) in Fig. 5.11 are maximal crack widths observed on the specimen side face in the constant
Verification
74
moment zone (see Figs. 5.4, 5.19, 5.25 and 5.32 in Kenel and Marti (2002)), while the corresponding crack steel stresses are determined from the average support moment maintained during the load step (average vertical load Q) considering the slab selfweight and the test equipment (Ma = 1.2 m (Q + 1.1 kN) + 0.5 · 1.42 m2 4.72 kN/m).
0
0
M[k
Nm
]
60
40
20
1000200 0.38%B1
0
M[k
Nm
]
60
40
20
χ [mrad/m]0 5 10 15 20 25
12
3
4
5
12 3
4
5
9
12 3
4 5 6
78
0
[mm]a10 20
00
M[k
Nm
]
60
40
20
30
Q[k
N]
10
20
30
40
50
0
Q[k
N]
10
20
30
40
50
Q[k
N]
10
20
30
40
50
ACI
EC β = 1
EC β = 1
ECβ = 1
= 1..0TCM
Q
1200
Qa
EC β = 1
EC β = 1ECβ = 1
TCM TCM
m = 4
ACIm = 4
ACIm = 4
ACI m = 3
ACI m = 3
ACIm = 3
0.38%B3
0.19%B4
kϕ
= 1..0TCM kϕ
= 1kϕ = 0kϕ
= 1..0TCM kϕ
= 1..0TCM kϕ
= 1..0TCM kϕ
(a)
0
0
(b)
(c) (d)
(e) (f)
0.38%B1
0.38%B3
0.19%B4
1000200
1000200
1200 1200
test
test
test
Fig. 5.10 Deformations of Kenel and Marti's (2002) 4point bending tests. The crosses and lines labelled testmark the measured curvatures and deflections, respectively. Illustrated are predictions according tothe Tension Chord Model (TCM with = 1), ACI 318 and EC 2. The dimensions are in [mm].
Verification
75
Deflection and crack width predictions test specimen B1
For a rectangular section without compression reinforcement (Table 3.1)
2
I
0.5 6.1 1 0.84 0.38 %0.505
1 0.84 0.38 % 6.1 1f
and
2
2
I
1 10.505 0.84 6.1 1 0.38 % 0.84 0.505 0.0852
12 2g
as well as
2
II 6.1 0.38 % 2 6.1 0.38 % 6.1 0.38 % 0.193f
and
3
2
II
0.1936.1 0.38 % 1 0.193 0.0175
3g
lead to compression zone heights
I
II
0.2 m 0.505 101 mm
0.84 0.2 m 0.193 32 mm
x
x
the stiffnesses
3 3 2I
3 3 2II
34 GPa 1 m 0.2 m 0.0852 23237 kN m
34 GPa 1 m (0.84 0.2) m 0.0175 2828 kN m
c
c
E I
E I
and the cracking moment
3 33.2 MPa 1 m 0.2 m 0.08522.0 kN m
0.2 m 0.101 mrM
which together with (Eq.(4.14))
2
22.0 kN m 3.2 MPa mrad3.55
2 2828 kN m 34 GPa 0.84 0.2 m 0.032 m mts
kk
define the section deformation behaviour illustrated in Fig. 5.10 (a, c & e).
The plotted midspan deflections in Fig. 5.10 (b, d & f) represent the distance measured between the slab at midspan and under the
point loads (equivalent to the midspan deflections in the classic 4pointbending setup). The selfweight of the jacks is 1.1 kN. The slab
selfweight (4.72 kN/m) is neglected for the deflection calculations but considered for . With (see Table 4.2) Q = 1.2m / 3.6 m = 1/3 the
State I deflections
2 2
I 2
1.2 m 1.1 kN 3.6 m23 mm0.07 0.1 mm
9 24 23237 kN m kN
Qa Q
and the State II deflections
2 2
II 2
1.2 m 1.1 kN 3.6 m23 mm0.59 0.7 mm
9 24 2828 kN m kN
Qa Q
can be determined. The tension stiffening deflections = 1) are
2 2
,II
3.6 m mrad3.55 5.8 mm
8 mtsa k k
The deflections of the partially cracked beam
1 I 1 II 2 ,II1 1 tsa a a a
are interpolated with (Eq.(4.85))
2 2
22.0 kN m
1.2 m 1.1 kN 0.5 4.72 kN/m 1.4 mQ
and (Table 4.2)
3 21 2
8 4 and
23 9
The maximal crack widths in the constant moment zone are determined with (Eq. (4.28))
Verification
76
02
0.0852 1 0.1936.11 7.8
8 0.0175 0.84 1 0.505
l
and (Eq.(4.26))
,II, 2
0.0852 1 0.1936.1 3.2 MPa1.056 ‰
208 Ga 0.0175 0.84 1 0.505s r
leading to Eq. (4.27) with = 1)
,II 1.056 ‰2 7.8
2s
s
wk
E
illustrated in Fig. 5.11. Factor k is set equal to 0 for neglecting the tensile stresses in the concrete and equal to 1 for considering average
concrete stresses equal to half the concrete tensile strength (for = 1).
00000000
0.08
0.06
0.04
0.02
200 300 400 500 600
[MPa]σs,II
000
wm
ax
Ø
00000
0.08
0.06
0.04
0.02
200 300 400 500 600
[MPa]σs,II
TCM= 0..1kϕ
Frosch
Frosch
TCM
TCM
Frosch
TCM
Frosch
TCM
= 0kϕ
= 1kϕ
= 0..1kϕ
= 0..1kϕ
= 0.4%ρ = 0.4%ρ
= 0.4%ρ = 0.2%ρ
1000 mm
200 mm
MC α = 0.63 α = 04
MC α = 0.63 α = 04
MC α = 0.63 α = 04
MC α = 0.63 α = 04
wm
ax
Ø
(a) (b)
(c) (d)
Fig. 5.11 Maximal side face crack widths in the constant moment zone of Kenel and Marti's (2002) 4pointbending tests (marked as crosses): (a) specimen B1; (b) specimen B3; (c) specimen B5; (d) specimen B4. Illustrated are predictions according to the Tension Chord Model ( = 1), MC 2010 andFrosch (slab face).
Both the section and member deformations (Fig. 5.10) are underestimated to a greater or lesser extent by all approaches if tension stiffening is considered. The direct tensile strength leads to reasonable cracking loads if the selfweight of the slab is considered. In these slab strips without stirrups, most of the observed maximal crack widths are located between the Tension Chord Model predictions with and without (k = 0...1) considering the contribution of the concrete between the cracks. The crack spacing on either side of the relevant crack in B1 is larger than predicted with = 1.
Verification
77
LongTerm 4PointBending Tests carried out at EPF Lausanne
160
(a)
150750
1000 1100
Q Q
16012Ø1000
6Ø
23
(b)
528@200Ø
12Ø6Ø
528@200Ø
Fig. 5.12 Overview of Jaccoud and Favre's (1982) bending tests Series C: (a) structural system; (b) section.The dimensions are in [mm].
Jaccoud and Favre (1982) tested seven identical slab strips (Series C) at different sustained load levels (see Fig. 5.13). The experimental section deformations, midspan deflections and maximal crack widths are taken from Tables 14 to 18 in Jaccoud and Favre (1982). The State II steel stresses illustrated vs. the measured crack widths are calculated shortterm State II steel stresses.
0
20
15
10
5
750 mm
160 0.06%
0.6%
M[k
Nm
]
t = 28 d0
0
χ [mrad/m]5 10 15 20 25
t = 388 d
0
20
15
10
5
0
20
15
10
5
1000
a
1100 1000 mm
Q Q
[kN
]Q
0
[mm]a
5 10 15 20 25
t = 28 d0
t = 388 d
0
20
15
10
5
M[k
Nm
]
[kN
]Q
ECβ = 1 EC β = 1
EC β = 0.5 EC β = 0.5
ACIm = 4
ACI m = 3
= 1..0TCM kϕ
= 1..0TCM kϕ
= 0.3..0TCM kϕ
= 0.3..0TCM kϕ
(a)
(c)
(b)
(d)
ACI ξ = 1.4
Fig. 5.13 Measured (crosses) and predicted 28day and 388day section deformations and midspan deflections for Jaccoud and Favre's (1982) 4point bending tests. Illustrated are predictions according tothe Tension Chord Model (TCM, = 1), ACI 318 and EC 2.
The 28day deformation predictions are carried out as described above for the Kenel and Marti (2002) tests. The 388day predictions are illustrated in the example below. The measured free shrink
Verification
78
age strains at 388 days are reduced based on Eq. (3.21) from 0.35 ‰ to 0.25 ‰ in order to account for the size difference between the shrinkage specimens and the test specimens. As stated in the report, the crack spacing is defined by the stirrup spacing (200 mm). This can be seen in Fig. 5.14 (c) and (d).
388day deformation predictions for the C specimens
With n = 6.9, fI = 0.508, fII = 0.245, gI = 0.0865 and gII = 0.0277 (Table 3.1), the 28day section properties are xI = 81 mm, xII = 32 mm, EcII
= 7892 kNm2 and EcIII = 1395 kNm2, while Mr = 9.4 kNm and ts = 2.91 mrad/m ( = 1). Accordingly with n = 6.1 (1 + 2.31) = 22.8 the
effective 388day section properties are xI,ef = 84 mm, xII,ef = 52 mm, Ec,efII,ef = 2602 kNm2 and EcIII,ef = 1057 kNm2. With k = 0.3 (Eq.
(4.11) with = 2.31) and = 1 the 388day tension stiffening curvature reduction is (Eq. (4.14))
2
9.4 kN m 0.131 m 0.032 m1 2.8 MPa mrad3.6
2 1395 kN m 0.131 m 0.052 m 30 GPa 0.131 m 0.052 m mts k k
The 388day free shrinkage strains are reduced based on Eq. (3.21) from sh = –0.35 ‰ measured on the shrinkage specimen (h0 = 60 mm)
to –0.25 ‰ for the test specimen (h0 = 132 mm) in order to account for the size difference. With II,ef = 0.290 103 m4 and the net uncracked
concrete properties Ac = 0.119 m2 and xc = 80 mm, this leads to shrinkage curvatures (Eq. (3.67))
2
,I 3 4
0.119 m 0.080 m 0.084 m mrad0.25 ‰ 0.5
0.290 10 m msh
and (Eq. (3.69))
,II
3 mrad0.25 ‰ 2.2
3 0.131 m 0.052 m msh
The concrete tensile stresses in the extreme fibres (Eq. (3.68))
2
,I 2
205 GPa 0.119 m mrad0.25 ‰ 1 0.16 m 0.084 m 0.5 0.6 MPa
22.8 0.134 m msh
reduce the cracking moment (Eq. (4.88)) to
3 42.8 MPa 0.6 MPa 0.290 10 m8.6 kN m
160 mm 84 mmrM
With g = 2.9 kN/m and Q = 1 m / 3.1 m = 0.323, the midspan deflections in Fig. 5.13 (d) are determined according to Chapter
4.3.1. The State I deflections
2 2 2 4 4
I 2 2
3 4 0.323 1 m 3.1 m 5 2.9 kN/m 3.1 m mm0.40 1.4 mm
24 2602 kN m 384 2602 kN m kN
Qa Q
the State II deflections
2 2 2 4 4
II 2 2
3 4 0.323 1 m 3.1 m 5 2.9 kN/m 3.1 m mm0.98 3.3 mm
24 1057 kN m 384 1057 kN m kN
Qa Q
the tension stiffening deflections = 1)
2 2
,II
3.6mrad3.1 m4.3 mm
8 mts
ka k
and the shrinkage deflections
2 2
,I
2 2
,II
3.1 m mrad0.5 0.6 mm
8 m
3.1 m mrad2.2 2.6 mm
8 m
sh
sh
a
a
are interpolated (Eqs. (4.84), (4.86) and (4.87))
1 I 1 II 2 ,II 2 ,I 2 ,II1 1 1ts sh sha a a a a a
with the 4point bending interpolation coefficients (Table 4.2)
3 23
1 2
2 2 22
8 0.3230.32
3 4 0.323
4 0.323 0.42
and
Verification
79
2 2
8.6 kNm
1.1 m 0.125 2.9 kN/m 3.1 mQ
corresponding to the predominant load.
000
max
Ø
00000
0.08
0.06
0.04
0.02
w
100 200 300 400 500
[MPa]σs,II
00000000
0.08
0.06
0.04
0.02
[MPa]σs,II
MC α = 0.43 α = 14
Frosch
100 200 300 400 500
= 0.6%28 d,
TCM = 0..1kϕ
Frosch
TCM = 0..0.3kϕ
rs = 200 mmrs = 200 mm
750 mm
160
ρ
= 0.6%28 d, ρ
= 0.6%388 d, ρ
= 0.6%388 d, ρ
MC α = 0.63 α = 04
max
Øw
(a) (b)
(c) (d)
Fig. 5.14 Maximum crack widths in the constant moment zone of Jaccoud and Favre's test Series C (1982)with stirrups spaced at 200 mm: (a) at 28 days; (b) at 388 days; (c) at 28 days assuming max crackspacing = stirrup spacing; (d) at 388 days assuming max crack spacing = stirrup spacing. Illustratedare predictions according to the Tension Chord Model ( = 1), MC 2010 and Frosch (bottom side).
The related transfer length (Eq. (4.28)) equals
02
0.0865 1 0.2456.91 5.3
8 0.0277 0.82 1 0.508
l
and the State II steel strains at cracking (Eq. (4.26)) equal
,II, 2
0.0865 1 0.2456.9 2.8 MPa0.67 ‰
205 Ga 0.0277 0.82 1 0.508s r
The related maximal crack widths in the constant moment zone Eq. (4.27)with = 1) are determined for both a 127 mm crack spacing
equal to twice the transfer length
,II 0.67 ‰2 5.3 0.25 ‰
2s
s
wk
E
and a 200 mm crack spacing equal to the stirrup spacing. Factor k is set equal to 0.3 (Eq. (4.11) with = 2.31) and 0.
Verification
80
LongTerm Bending Tests Carried out at the University of New South Wales
var
1170 1170
Q Q
1170
150
40
42
250
348
B1
180
25
27
250
333
B2
90
25
27
250
B3
400
12Ø
3082540
161S1
400
15425
40
161S2
400
10325
40
161S3
161
3500
333
B1  B3
S1  S3
q
(a) (b)
(c) (d)
16Ø
B1
2
B2
16Ø2
B3
16Ø3
2 12Ø3
12Ø4
12ØS1
2S2
12Ø3
S312Ø4
Fig. 5.15 Overview of Gilbert and Nejadi (2004) beams and slabs: (a) structural system beams; (b) beamsections; (c) structural system slabs; (d) slab sections. The dimensions are in [mm].
Gilbert and Nejadi (2004) tested 6 beams (B1a/b to B3a/b) and 6 slabs (S1a/b to S3a/b) with reinforcement ratios between 0.4 and 0.8 % under loads sustained for 400 days. The free shrinkage strains sh = –0.825 ‰ measured on 600/160/600 mm shrinkage specimens are corrected with Eq. (3.21) to account for the specimen size (see example calculation), leading to sh = –0.76 ‰ for the beams and sh = –0.87 ‰ for the slabs.
Fig. 5.16 compares the measured and predicted midspan deflections, while Fig. 5.17 and Fig. 5.18 illustrate the maximum crack widths observed at the bottom of the specimen side faces. The steel stresses plotted vs. the measured crack widths correspond to the calculated shortterm State II steel stresses given in the test report.
Verification
81
0 205 10 15
0
[mm]a
04010 20 30
0
Q Q
0
q
3500 mm
a
a
10
7.5
5
2.5
[kN
/m]
g+q
0
30
20
10
Q[k
N]
3 1170 mm
10
7.5
5
2.5
ρ = 0.8 %
ρ = 0.4 %
[kN
/m]
g+q
0 205 10 15
0
[mm]a4010 20 300 4010 20 30
ρ = 0.5 %
14 d 400 d
14 d 400 d
14 d 400 d
14 d400 d
14 d
400 d
14 d400 d
14 d
14 d
400 d
400 d
14 d
14 d
400 d
400 d
14 d
14 d400 d
400 d
400 d
ρ = 0.8 %B3a/b
14 d:= 1TCM kϕ
EC β = 1ACI ξ = 0
= 0TCM kϕ
= 0.4TCM kϕEC β = 0.5400 d:
ACI ξ = 1.4= 0TCM kϕ
(a) (b)
B1,2a/b
14 d 400 d
(c) (d)
(e)
S1a/b ρ = 0.6 %S2a/b
ρ = 0.8 %S3a/b
14 d
[mm]a
[mm]a [mm]a
Fig. 5.16 Measured (crosses) and predicted 14 and 400day midspan deflections for Gilbert and Nejadi's(2004) flexural members: (a) beams B1/2a/b; (b) beams B3a/b; (c) slabs S1a/b; (d) slabs S2a/b;(e) slabs S3a/b. Illustrated are predictions according to the Tension Chord Model ( = 1), ACI 318and EC 2 (line types and parameters according to figure (a)).
Verification
82
00000000
0.08
0.06
0.04
0.02
max
Øw
0
0.08
0.06
0.04
0.02
100 200 300 400 500
[MPa]σs,II
100 200 300 400 500
[MPa]σs,II
= 0..1kϕ
MC α = 0.63
MC α = 0.43α = 14
α = 04
Frosch
00000000
0.08
0.06
0.04
0.02
TCM
= 0..0.4kϕTCM
0.5%400 d,0.5%14 d,
0.5%400 d,0.5%14 d,
0.8%400 d,0.8%14 d,
Frosch
(a) (b)
(c) (d)
(e) (f)
max
Øwm
ax
Øw
Fig. 5.17 Maximum side face crack widths for Gilbert and Nejadi's (2004) test beams: (a) B1a & b at loading; (b) B1a & b 386 days later; (c) B2a & b at loading; (d) B2a & b 386 days later; (e) B3a & bat loading; (f) B3a & b 386 days later. Illustrated are predictions according to the Tension ChordModel ( = 1), MC 2010 and Frosch (side face).
Verification
83
400day predictions Specimens S1
With n = 9, fI = 0.508, fII = 0.240, gI = 0.0859 and gII = 0.0265 (Table 3.1), the 14day section properties are xI = 82 mm, xII = 31 mm,
EcII = 3266 kNm2 and EcIII = 536 kNm2, while Mr = 3.3 kNm and ts = 2.64 mrad/m (Eq. (4.7) with = 1). Accordingly with
n = 9 (1 + 1.71) = 24.4, the effective 400day section properties are xI,ef = 84 mm, xII,ef = 47 mm, Ec,efII,ef = 1269 kNm2 and
EcIII,ef = 430 kNm2, while Mr,ef = 0.6 kNm and ts = 1.2 mrad/m (Eq. (4.14) with = 1 and k = 0.4). Free shrinkage strains equal to
sh = 0.87 ‰ lead to sh,I = 1.43 mrad/m (Eq. (3.67)) and sh,II ≈ 7.60 mrad/m (Eq. (3.69)).
The 400day State I and State II deflections
4 4
I 2 1
4 4
II 2 1
5 3.5 m mm1.54
384 1269 kN m kNm
5 3.5 m mm4.54
384 430 kN m kNm
qa
qa
are interpolated with (Table 4.2)
3
1
16 4 3
5r r
while the 400day tension stiffening deflections
2 2
,II
3.5 m mrad1.2 1.8 mm
8 mtsa
and the shrinkage deflections
2 2
,I
2 2
,II
3.5 m mrad1.43 2.2 mm
8 m
3.5 m mrad7.6 11.6 mm
8 m
sh
sh
a
a
are interpolated with (Table 4.2)
22 4 r
where
2 2
1 0.6 kNm1 1
2 0.125 3.5 mr q
The maximal crack widths (in the middle third of the beam) are determined with (Eq. (4.28))
02
0.0859 1 0.24091 7.45
8 0.0265 0.81 1 0.508
l
and (Eq. (4.26))
,II, 2
0.0859 1 0.2409 1.8 MPa0.60 ‰
205 Ga 0.0265 0.81 1 0.508s r
leading to maximal crack widths Eq. (4.27) with = 1)
,II 0.60 ‰2 7.45 0.87 ‰
2s
s
wk
E
With a crack spacing of 2 · 7.45 · 12 mm = 180 mm, shrinkage alone causes a crack opening of 0.16 mm.
As there are no stirrups, the reinforcement ratio primarily defines the related crack spacing, which together with the State II steel stresses and the free shrinkage strains defines the size of the crack widths (Fig. 5.17 and Fig. 5.18). According to the slab crack width predictions, slab S1 with the lowest reinforcement ratio (sr,max = 180 mm) should have the largest cracks followed by slabs S2 (sr,max = 116 mm) and S3 (sr,max = 84 mm). In reality, the order is the other way round (see Fig. 5.18). It must, however, be taken into account that at the low steel stress levels found in the slabs, the predicted crack widths are close and generally reflect the observed values. A look at the crack patterns shows that the largest crack influence region is just over 250 mm in S1, around 200 mm in S2 and S3a, but over 250 mm in S3b, where the observed crack spacings are considerably larger than predicted.
Verification
84
00000000
0.08
0.06
0.04
0.02
00000000
0.08
0.06
0.04
0.02
00000000
0.08
0.06
0.04
0.02
100 200 300 400 500
[MPa]σs,II
100 200 300 400 500
[MPa]σs,II
0.4%14 d,
Frosch bottom
0.4%400 d,
TCM= 0..1kϕ
TCM = 0..0.4kϕ
MC α = 0.43 α = 14
MC α = 0.63
0.6%14 d, 0.6%400 d,
TCM= 0..0.4kϕ
TCM= 0..1kϕ
0.8%14 d, 0.8%400 d,
TCM= 0..1kϕ
TCM= 0..0.4kϕ
Frosch side
Frosch side
bottom, side
Frosch bottom
Frosch
bottom, sideFrosch
bottom, sideFrosch
bottom, sideFrosch
MC α = 0.63
MC α = 0.63
MC α = 0.43 α = 14
MC α = 0.43 α = 14
max
Øwm
ax
Øwm
ax
Øw
(a) (b)
(c) (d)
(e) (f)
Fig. 5.18 Maximum side face crack widths (bottom fibre) for Gilbert and Nejadi's (2004) test slabs: (a) S1a& b at loading; (b) S1a & b 386 days later; (c) S2a & b at loading; (d) S2a & b 386 days later;(e) S3a & b at loading; (f) S3a & b 386 days later. Illustrated are predictions according to theTension Chord Model ( = 1), MC 2010 and Frosch.
Verification
85
ConCrack Benchmark Specimens RL1 and RG8
The ConCrack Specimens RL1 and RG8 (NECS 2010; BuffoLacarriere et al. 2011) belong to the Benchmark tests carried out within the national French project CEOS (Comportement et Evaluation des Ouvrages Speciaux visàvis de la fissuration et du retrait). The Beam Specimens RL1 and RG8 were submitted to 4point bending tests after either 2 months of free shrinkage and cooling (RL1) or 1 month of restrained shrinkage and cooling (RG8). The axial deformations of RG8 were restrained by two tube struts.
Apart from some minor changes, the predictions illustrated here represent a part of the author's results (BuffoLacarriere et al. 2011) submitted for the blind stage of the prediction contest carried out for the Benchmark tests.
t fctm1) fcm Ecm sh total2) sh autog. 2) creep
3) concrete T
[d] [MPa] [MPa] [GPa] [m/m] [m/m] [m/m] [°C]
0 22/174)
1 3.15 33.8 32.6 50 20
2 3.60 42.2 34.8 83 30 0 76.15)
5 163 57 133
7 4.45 54.0 36.9 183 60 204
14 283 80 301
21 370 100 341
28 4.65 60.0 39.1 433 113 389 10
56 490 120 
Table 5.1 Measured concrete properties C50/60 for RL1 and RG8: 1) splitting tensile strength from three 160 x 320 mm prisms (NF EN 123906); 2) refractometer with 70 x 70 x 280 mm specimens (h0 = 17.5 mm, ts = 1 d); 3) prismatic 110 x 220 mm specimens loaded at 40% of their compressive strength(12.2MPa); 4) 22°C for RL1 and 17°C for RG8; 5) measured under adiabatic conditions in a thermally isolated 300 mm cubic container.
Test Specimen RL1
Specimen RL1 was cast on the 12th of October 2009 (t = t0). After the formwork was removed on the 14th of October (t = 2 d) the specimen remained supported on wooden log elements (Fig. 5.19, left) under outdoor environmental conditions (≈ 10 °C) until it was moved to the testing bench (Fig. 5.19, right and Fig. 5.20 (a)) on the 27th of November (t = 46 d). The four point bending test took place on 14th of December (t = 63 d). The specimen was loaded up to Q = 2250 kN and unloaded back to Q = 0. The predictions are carried out with the structural system illustrated in Fig. 5.20 (c) and the 28day concrete properties (Table 5.1). The specimen is b = 1.6 m wide, h = 0.8 m thick (with exception of the end regions) and 6.1 m long. 16 32 mm bars provide the tensile reinforcement with As/bd = 1.11 %, while 8 25 mm bars provide the compression reinforcement with '= 0.34 % (Fig. 5.20 (b)). The distribution reinforcement (0.14 % from 8 16 mm bars) is not taken into account for the predictions. There are stirrups ( = 16 mm) spaced at 350 mm in the constant moment zone and at 310 mm in the rest of the beam.
Verification
86
Fig. 5.19 Specimen RL1 (NECS 2010): (a) during 63 days of free shrinkage and cooling; (b) on testingbench.
x
1750 800
CL
Q
(P7)
500
P9P10(P8)
P14 (P16)
P17 P2(P4)
722
800
xz
2550
P11
Q
2 Ø 32
25Ø
16Ø
800
99 255 192 158 96
800
16Ø
CL
170 1075 320 815 170100
4 macalloy bars 50,Ø approx. l = 3300 mm
(a)
(c)
(b)
2 Ø 32
25Ø
16Ø
16Ø
l2
lΔ(= )a
(= )(= )
Fig. 5.20 Specimen RL1: (a) schematic illustration of the specimen on the testing bench; (b) section; (c)static system used for predictions. The dimensions are in [mm]. The measurement locations inbrackets are located on the other half of the symmetrical beam.
CEOS.fr french national programme CEOS.fr french national programme
Verification
87
0
t [d]
03010 20
T[
C]
SU
CSL
SUCSL
1600 mm
800
mm
80
60
40
20
o
SUCSL
Fig. 5.21 Specimen RL1: Concrete temperature measured at points SU, C and SL during 30 days after casting.
Predictions 4point bending test RL1
The static bending test takes place at t = 56 d. Cooling after hydration is assumed to cause evenly distributed strains equal to 0.012 ‰/°C ·
30°C = 0.36 ‰, which due to the lack of external restraint cause an even shortening and do not affect the bending behaviour. Uniformly
distributed autogenous and drying shrinkage strains equal to 0.12 ‰ (measured) and 0.16 · 0.37 ‰ = 0.08 ‰ (reduced according to Eq.
(3.21) to account for h0 = 267 mm and ts = 2 d) are adopted. The internal restraint due to 0.2 ‰ shrinkage is not large enough to cause
separation cracks, so that RL1 is modelled as uncracked at the beginning of the static bending test.
The RL1 deformation predictions are carried out with the structural system illustrated in Fig. 5.20 (c) and the moment distribution
2
2 2
2 2
if  x 02
if 0 x2
if x2 2
gl x l
gM Qx lx l x a
g lQa lx l x a
where g = 32 kN/m,l = 0.5 m, a = 1.75 m and l = 5.1 m (for x and z see Fig. 5.20). The average section deformations avg = 0,avg + z avg
are defined by the equilibrium equations
0.5
, , ,0.5
0.5
, , ,0.5
0 dz
dz
h
c s c s c s ss avg s s s avg u s ts sh
h
c s s c s s c s s ss avg s s s s avg u s ts sh
b A A A E A k E
M b z z A z A z A E z A k E
The 28day concrete properties with n = 5.1 and therefore EcII = 2954 103 kNm2, EcIII = 881 103 kNm2, xI = 409 mm, xII = 200 mm as well
as Es = 200 GPa are used. The concrete stresses c = (avg – ci) Ec are determined with ci = 0.2 ‰ and assumed zero in the tension zone of
cracked sections.
Tension stiffening is considered with the effective reinforcement ratio (Eq. (4.4))
13 2
3 2
2954 10 kNm 0.722 m 0.200 m5.1 5.1 1 5.33%
881 10 kNm 0.8 m 0.409 mef
Factor is set equal to 1 because the transfer length (Eq. (4.28) with d = 0.722 m and 32)
3 2
0 3 2
2954 10 kNm 0.722 m 0.200 m5.1 32mm1 71 mm
8 881 10 kNm 0.8 m 0.409 ml
implies a maximum crack spacing equal to 142 mm, which is less than half the stirrup spacing. With fct = 4.65 MPa this leads to (Eq. (4.2))
,
4.65 MPa 1 5.33%0.21‰
2 5.33% 200 GPas ts k k
The vertical displacements (relative to supports)
Verification
88
/2 /2
1 2dx dxl l
z avg avg
l l
u M M
at x = xa are determined with
1
1 if 0
if 2
aa
aa a
xx x x
lM
x lx x x x
l
and
2ax
M xl
For comparison, the elastic midspan deflections at Q = 2250 kN are estimated with the elastic deflection equation
2
2
3 2
1.75m3 4
1.75m 2250 kN 5.1m5.1m12.2 mm
24 881 10 kNma
for 4point bending according to Table 4.1.
The maximum crack widths (Eq. (4.21))
max
4.65 MPa142 mm 0.2 ‰ 142 mm 0.2 ‰ 0.06 ‰
2 39.1 GPaavg u avg uw k k
result from the average section strains (= average steel strains) and average concrete strains. For reasons of simplicity tension stiffening is
neglected for all predictions during unloading (ku = 0).
Q[M
N]
ε [ ]
2.4
1.8
1.2
0.6
01 0 1 2
P17 P14
ε [ ]1 0 1 2
P4, P2 P16
= 1..0, ciε = 0.2
= 1..0, ciε = 0
= 1, ciε = 0.2
= 1..0, ciε = 0.2
= 1..0, ciε = 0
test
testtest
test
kϕ
kϕ
kϕ
= 1, ciε = 0.2kϕ
kϕ
kϕ
Fig. 5.22 Specimen RL1: Predicted average strains during the 4point bending test with = 1: P14, P16 andP17 are steel strains; while P2 and P4 are concrete strains (see Fig. 5.20).
Judging from Fig. 5.21 the assumption of a uniform concrete (and steel) temperature distribution is not unreasonable, but the assumed 30 °C temperature drop after hydration is too small. The predicted and measured steel strains at points (see Fig. 5.20 (a)) P14 (z = –0.34 m; x = 1.63 m), P16 (z = –0.34 m; x = 1.880 m) and P17 (z = 0.35 m; x = 1.610 m) as well as the concrete compressive strains at P2 (z = 0.383 m; x = 2.360 m) and P4 (z = 0.393 m; x = 1.775 m) are compared in Fig. 5.22. The predicted and measured strains are set equal to zero at the beginning of static loading ( = 0 at Q = 0). The unloading strains are not illustrated because the difference between loading and unloading is small on the compression side, while the steel strain measurements on the tension side are only available up to Q = 1 MN. The dashed lines on the tension side illustrate predictions neglecting shrinkage (no difference is visible on the compression side). It can be seen that, the predicted steel strain reduction due to tension stiffening is about the same size as the shrinkage strains released at cracking.
Verification
89
Judging from the cracking load and the tensile steel strains, it seems that the predictions either overestimate shrinkage or underestimate the concrete tensile strength.
Q[M
N]
2.4
1.8
1.2
0.6
0u [mm]
Q[M
N]
2.4
1.8
1.2
0.6
5 10 0 5 10
= 1..0, ciε = 0.2
elastic midspan eq.
= 1..0, ciε = 0.2
P10
= 1..0, ciε = 0.2
= 1..0, ciε = 0.2
0
0
kϕkϕ
corr. test data
kϕ
corr. test data
corr. test data
kϕ
corr. test data
z u [mm]z
(a) (b)
(c) (d)
P9 P7
P8
Fig. 5.23 Specimen RL1: Predicted and measured vertical displacements during the 4point bending test atlocations (see Fig. 5.20 (a)) P9, P7, P10 and P8.
Fig. 5.23 compares the vertical displacements at points P9 (x = 2.38 m), P7 (x = 1.565 m), P10 (x = 1.245 m) and P8 (x = 0.17 m) (see Fig. 5.20) relative to the supports (x = 0). Thereto, the potentiometric displacement sensor measurements are corrected with the displacements measured at P8 and P11 according to
P11 ,P8 P8 ,P11z,corr
P8 P11
z zz
x u x uu u
x x
(5.1)
in order to eliminate the displacements attributed to the elongation of the macalloy bars. Fig. 5.24 illustrates the predicted maximum crack widths at the concrete surface (z = – 0.400 m) as well as the maximum crack widths observed on the specimen.
Verification
90
0
w [mm]
Q[M
N]
2.4
1.8
1.2
0.6
max
0.1 0.2 0.3 0.4
z =  0.400 m
test
predicted
Fig. 5.24 RL1 predicted and observed maximal crack widths. It is assumed that the observed values refer tothe maximum crack opening found on the entire specimen.
Test Specimen RG8
Test specimen RG8 is illustrated in Fig. 5.25 and Fig. 5.26. The central part of the specimen is b = 0.5 m wide, h = 0.8 m thick, 5.1 m long and symmetrically reinforced with 10 32 mm bars (see Fig. 5.26 (b)) providing TC(As + As')/(bh) = 2.01 % or ' = As/(bd) = As'/(bd) = 1.10 %. The distribution reinforcement (4 12 mm) is not taken into account for the predictions. 16 mm diameter stirrups are spaced at 220 mm in the middle of the beam (over a length 1100 mm) and at 200 mm elsewhere. Two steel tubes (Atube = 35563 mm2) on either side of the specimen (Fig. 5.26 (c)) restrain its axial deformations. The tubes are braced against the eccentrically prestressed heads of the specimen.
Fig. 5.25 Specimen RG8 (NECS 2010).
RG8 was cast on the 7th of April 2010 in isolating formwork (on all four sides), which was removed 2 days later (t = 2 d). The THM (ThermoHydroMechanic) test (t = 2d to 30 d) consisted in letting the axially restrained member shrink and cool down under environmental conditions (≈ 15 °C). During this time the specimen was supported on wooden log elements. At t = 30 d the 4point bending test
CEOS.fr french national programme
Verification
91
took place. The specimen was placed on the testing bench (Fig. 5.26 (a)) and loaded in 50 kN (20 minutes) steps up to 800 kN (per point load).
age1) Ec fct sh
2) / 3) sh T4) temp5) ci si
[d] [GPa] [MPa] [‰] [‰] [°C] [‰] [‰] [‰]
2 34.8 3.6 0.030/0 0.03 75 0 0.03 0
3 35.2 3.8 0.04 70 0.06 0.10 0.06
4 35.6 3.9 0.06 65 0.12 0.18 0.12
5 36.1 4.1 0.057/0.012 0.07 60 0.18 0.25 0.18
6 36.5 4.3 0.07 55 0.24 0.31 0.24
7 36.9 4.5 0.060/0.016 0.08 50 0.30 0.38 0.30
8 37.0 4.5 0.08 45 0.36 0.44 0.36
9 37.1 4.5 0.09 40 0.42 0.59 0.42
10 37.2 4.5 0.09 35 0.48 0.57 0.48
11 37.3 4.5 0.10 30 0.54 0.637 0.54
12 37.4 4.5 0.10 25 0.60 0.70 0.60
13 37.5 4.5 0.11 20 0.66 0.77 0.66
14 37.6 4.5 0.080/0.033 0.11 15 0.72 0.83 0.72
21 38.4 4.6 0.100/0.050 0.15 15 0.72 0.87 0.72
28 39.1 4.7 0.113/0.066 0.18 15 0.72 0.90 0.72
30 39.1 4.7 0.18 15 0.72 0.90 0.72
Table 5.2 Assumed concrete properties for the RG8 blind stage predictions with 1) linear interpolation of values inbetween measurements (coloured in grey); 2) autogenous shrinkage as measured (Table5.1); 3) drying shrinkage reduced according to Eq. (3.21); 4) the cooling rate of 5 °C per day is assumed based on Lohmeyer & Ebeling (2009) pg. 117; 5) with the measured concrete dilatation coefficient of 12 m/m/°C.
Predictions THMtest RG8
During the THMtest the central part of RG8 (l = 5.1 m and TC = 2.01 %) is modelled according to 4.2.2 as an endrestrained beam
with a restraint stiffness
232 2 35563 mm 200 GPa
7.0 N/mm5.1 m 0.5 m 0.8 m
tube sA Ek
lbh
and (Eq. (4.38))
35.1 m 7.0 N/mm0.178
200 GPas
lk
E
For comparison the case of no external ( = 0) restraint is also regarded.
Before cracking the compression force in the steel struts (Eq. (4.43))
,I(1 )2 c s ci si
bhR n E
is determined with (Eq. (4.41))
,I
I
si cic sE
n a
During the crack formation phase an upper limit for
(1 )2 ct s sh
bhR n f E
Verification
92
is estimated with c,I = fct. The force fluctuations between the cracks are not considered.
x
1750 800
CL
Q
1300
800
xz
(a)
2550
Q
steel strut outer 323 mmØ
800
500
725
C, (D)
500
16Ø
C, (D)
800
1250
900
1250
360
750
C, (D)
40 mm wall thickness
900
2200 16
0
(b)
(c)
(d)
32Ø5
32Ø5
12Ø4
steel strut outer 323 mmØ40 mm wall thickness
16Ø
l2
(= )
Fig. 5.26 Specimen RG8: (a) schematic illustration of specimen on testing bench; (b) regular section; (c)schematic plan view illustrating steel struts (d) static system used for predictions. The dimensionsare in [mm]. Point D in brackets is on the other half of the symmetrical specimen.
The relative displacement between points C and D
2CD CDCD
s tube
l l RRl
l kbh E A
results from R for ≥ 0 or is equal to
1
1ci si
CD CD sil ln
for = 0. The cracking behaviour during the crack formation phase is modelled assuming a transfer length equal to
0
1 32 mm 1 2.01 %195 mm
8 8 2.01 %l
Verification
93
With between 1 and 0.5 this leads to a final amount of cracks between (Eq. (4.58))
5.1 m13 ... 26
2 195 mmnj
and with = 1 a maximum crack width (Eq. (4.46) equal to
195 mm 4.65 MPa 1 2.01 % 5.1 –10.25 mm
2.01 % 200 GPaw
The cooling and shrinkage induced steel si and concrete ci strains adopted for the blind stage predictions are given in Table 5.2 and Fig.
5.27 (a). As there are 26 stirrups = 0.5 is assumed. According to c,I (Fig. 5.27 (b)) the crack formation phase starts at t = 5 d with
ci,1 = 0.25 ‰ (Table 5.2) and ends (Eq. (4.57) with si = 0.72 ‰ and aI = 1.083) at
,26
0.5 1 2.01% 0.178 0.72‰ 2.01%4.65 MPa2 1.083 1.068 ‰
2 2.01% 200 GPa 0.178 2.01% 0.178 2.01%ci
This implies an average concrete strain increase of
1.068 ‰ 0.25‰0.032 ‰
26 1ci
per crack, resulting in 20 cracks at t = 30 d.
With the simplified temperature evolution adopted based on the measured concrete temperatures (T2 in Fig. 5.27 (a)) and = 0.5,
the crack formation phase starts at (Fig. 5.27 (b)) t = 3 d with ci,1 = 0.10 ‰ (Table 5.2) and ends (Eq. (4.57) with si = 0.42 ‰ and aI =
1.083) at
,13
0.5 1 2.01% 0.178 0.42‰ 2.01%4.65 MPa2 1.083 1.041 ‰
2 2.01% 200 GPa 0.178 2.01% 0.178 2.01%ci
This implies an average concrete strain increase of
1.041 ‰ 0.10‰0.038 ‰
25ci
per crack, resulting in (0.60 ‰ + 0.10 ‰)/0.038 = 13 cracks at t = 30 d.
Fig. 5.27 illustrates the predicted and measured behaviour of Specimen RG8 during the THM test. The concrete temperature evolutions denominated T1 and T2 correspond to the temperature evolution predicted for the blind stage and an evolution approximating the measured concrete temperatures, respectively. The concrete temperatures measured in RL1 (Fig. 5.20) and RG8 (Fig. 5.27 (a)) are similar. They indicate concrete hardening at a temperature of around 50 °C before the maximum temperature of 55 °C is reached after 24 hours. After this point the concrete starts to cool down to ambient temperature, reaching its hardening temperature (l ≈ 0) at around 2 days and ambient temperature at 4 days. It is cooling below the hardening temperature, which leads to tensile stresses in an axially restrained member. The present predictions assume si = 0 and ci = 0.03 ‰ at t = 2 days.
As concrete shrinkage strain and tensile strength measurements were available for the blind stage predictions and the concrete temperature evolutions were provided afterwards (Fig. 5.27 (a)), the main assumption behind the refined THM predictions is the restraint stiffness. This is why the predictions in Fig. 5.27 were carried out with a restraint stiffness corresponding to no restraint ( = 0) and the stiffness of the two 5.1 m long steel struts ( = 0.178). The latter stiffness represents an upper limit, as neither the coupling elements at the end of the steel struts nor the flexibility of the end beams is taken into account. For = 0 there should not be any cracking, while for = 0.178 cracking is predicted to start at 5 or 3 days (Fig. 5.27 (b)), depending on the rate of cooling. For > 0, the maximal tensile force (= –2 R) in the member during the crack formation phase (Fig. 5.27 (c)), which is reached each time before a crack forms, is independent of the cooling strains and restraint stiffness.
The restraint stiffness, however, defines the relative axial displacement between C and D shown in Fig. 5.27 (d). The figure illustrates the good agreement between the displacements calculated with = 0.178 and the displacements measured with the 2.5 m long optic fibre sensor located between the points C and D. In this context it remains unclear why the predicted amount of 20 (for T1) or 13 (for T2) cracks strongly overestimates the 3 cracks (at 3, 7 and 10 days) observed during the
Verification
94
THM test. Unfortunately experimental strut forces (R), which could disclose the axial force in the member, are not available.
1
2
3
4
5
σ c,[M
Pa]
I
fct
0
t [d]
00
t [d]
l [m
m]
Δ
3010 203010 20
1
R[M
N]
0.2
0.4
0.6
0.8
500 mm
800
mm
4
80
60
40
20
0
PT1009
PT1004
PT100119
0 3010 20 2 4 60 8
rem
oval
of
form
wor
k
1st c
rack
test
0.5
0.0
0.5
1.0
1.2
1.5
2.0
2.5κ = 0,
measured
for blind
predictions
κ = 0.18,
predictions
2nd
crac
k te
st
T1
for refinedT2
T2
κ = 0.18, T1
κ = 0.18, T1
κ = 0.18, T2
T1
κ = 0, T2
κ = 0.18, T2κ = 0.18, T1
(a) (b)
(c) (d)
T[
C]
o
Fig. 5.27 THM test Specimen RG8: (a) concrete temperature during cooling; (b) development of concretestresses before cracking (neglecting creep); (c) axial force per steel strut; (d) relative displacementbetween points C and D.
Predictions static bending test RG8
Based on the THM predictions and for reasons of simplicity RG8 is assumed to be fully cracked at the start of the 4point bending test.
With = 0.178, = 0.5 and Eq. (4.59)
2 0.5 4.65 MPa 1 2.01%0.1782 2.01 % 500 800 mm 200 GPa
0.178 2.01% 2 2.01% siN R
equals 1451 kN for si = 0.72 ‰ (T1, see Fig. 5.27 (a)) and 1071 kN for si = 0.42 ‰ (T2). The corresponding average member strains are
0.11 ‰ in the first case and 0.07 ‰ (Fig. 5.28 (b)) in the second case.
Within an iterative procedure, a midspan moment Ma is assumed, leading to a moment distribution (selfweight neglected)
if 0 x 1.75 m
if 1.75 m 0.5
a
a
M x
lM
M l
On this basis, the equilibrium equations
, ,c
c s s avg si u s ts s s avg si u s tsAN dA A E k A E k
and
Verification
95
, ,c
c s s s avg si u s ts s s s avg si u s tsAM zdA z A E k z A E k
are used to provide the average section strains
0, avg avg avgz z
as a function of the assumed midspan moment Ma and the unknown axial force N, which then results from
/2
0,
0
2 dxl
avgN kbh
The bottom steel layer is defined by ' = 1.1% and d' = 75 mm, while the top steel layer is defined by = 1.1% and d = 725 mm.
Tension stiffening top and bottom reinforcement) is implicitly accounted for within the steel term according with
,
,
1 if 0.07 ‰
if 0.07 ‰ 0.35 ‰
0 if 0.35 ‰
avg
u u s avg
s avg
k k
assuming the tension force carried by the concrete to have the same centroid as the steel. The first line in the equation applies to most of
the top reinforcement (Fig. 5.28 (c)) where the average steel strains increase under bending. The other two lines apply to most of the bot
tom reinforcement (Fig. 5.28 (d, e)) where the steel strains decrease under bending. Eq. (4.2) with = 0.5, n = 5.1 and = 2.01% pro
videss,ts = 0.29 ‰, while Eq. (4.20) with aI = 1.083 provides
, ,0.07 ‰ 0.07 ‰1.231 2.210 0.011
0.29 ‰ 0.29 ‰s avg s avg
uk
δ
τ
fct
(a)
[ ]
2
+
ε
0.21
0.35
0.28
τ
sr0.5
τ
sr0.5
0.28[ ]
+
ε0.28
0.28
[ ]+
ε
< 0.21
τ
sr0.5
[ ]
ε
sr0.5
crack CL CL
CLCL
> 0.35
(b) (c)
(d) (e)crack
crack
crackcrack
> 0.21
Fig. 5.28 Assumed steel strains during the 4point bending test for = 0.178 and si = 0.42 ‰: (a) assumedbond stressslip relation; (b) at the start of the 4point bending test; (c) in most of the top reinforcement during the bending test; (d) & (e) in most of the bottom reinforcement during the staticbending test (tensile force changes into compression force). When reaches zero the cracks close.
The compression concrete becomes loadbearing once avg reaches ci (and cracks close) and
2
1 2c c
kf
k
according to Sargin (1971). In this case fc = 60 MPa, cu = 2.3 ‰, Ec = 39.1 GPa, = (– + ci)/cu and k = cu Ec/fc.
Once N belonging to Ma is determined, the reaction force in each steel strut R = –N/2, the relative displacement between C and D
Verification
96
/2
0,
1.3m
2 dxl
avgl
the vertical displacement at x = xa (for 1M and 2M see RL1)
/2 /2
1 2
0 0
dx dxl l
z avg avgu M M
as well as the average crack widths in the constant moment zone
,220 mm2
ctavg s avg ci
c
fw
E
can be determined as a function of
1.75 ma mM Na
Q
where am is the absolute value to the midspan deflections relative to the supports.
0, =Ma 1017 kN=Nx
0.07
=1.75 m 0.8 m
0 ,avg
0.11ε0

MMa
500 kNm, =Ma 738 kN=N
CL
Q
1.75 m 0.8 m
χavg2.1
C / D


0 ,avgε0
a
1000 kNm, =Ma 294 kN=N
+
0.26
 3.5χavg
0 ,avgε00.02
(a) (b)
(c) (d)
Fig. 5.29 Average section strains [‰] and curvatures [mrad/m] during the 4point bending test for = 0.178,ci = 0.60 ‰, si = 0.42 ‰, = 0.5 and k = 1.
The average section deformations at three different load levels are shown in Fig. 5.29. Fig. 5.30 illustrates the tensile steel strains at x = 1.9 m and 2.35 m, the vertical displacements at x = 2.1 m and 1.45 m, the force per steel strut and the relative displacement between points C and D. All four figures show predictions carried out with the full stiffness of the steel struts ( = 0.178) and the two temperature evolutions T1 and T2 (see Fig. 5.27 (a)). Independent of the temperature evolution chosen, the predicted steel strains (Fig. 5.30 (a)) reflect the measured values up until the vertical loadrange where the compression concrete is activated. This could mean that the compression concrete is activated later than predicted (e.g. because the shrinkage strains are underestimated) or that there is steel yielding. In view of the THM predictions and the fact that si = 0.42 ‰ does not reduce the yield strains below 2.1 ‰ even for fsy = 500 MPa, both explanations seem unlikely. As the measured deflections and axial displacements start increasingly exceeding the predicted values above Q = 400 kN, it is likely that (as found for RL1) there are additional effects (e.g. rigid body translations) influencing the global deformation behaviour during the 4point bending test.
Verification
97
1 0.5 0 0.5 1
0 5 10 15 200.50
R [MN]
800
600
400
200
800
600
400
200
Δ CDl [mm]
0.5 0 0.5 1.0 1.5 2.0
Q[k
N]
predicted
0
ε[ ]0.5 1.5 2.50 1.0 2.0
measured= 2.35 mx= 1.90 m
measured= 1.45 mx= 2.10 m
> 1.75 m,x = 1.45 mx= 2.10 m
T1T2
predicted T1T2
predicted T2T1
predicted T1
= 1.45 mx= 2.10 m
predicted T2
Q[k
N]
u [mm]z
(a) (b)
(c) (d)
Fig. 5.30 Fourpoint bending test RG8: (a) tensile steel strains; (b) vertical displacements; (c) force per steelstrut; (d) displacement between C and D. The predictions are carried out assuming = 0.178 andeither ci = 0.90 ‰ & si = 0.72 ‰ (T1) orci = 0.60 ‰ & si = 0.42 ‰ (T2).
5.2.2 Statically Indeterminate Beams
In this section three test series of twospan beams are used to discuss the influence of the reinforcement detailing and the corresponding moment redistributions on the deflections of statically indeterminate beams.
Twospan beams tested at Gent State University
Taerwe (1981) tested four twospan beams (C1 to C4) with 5 m spans and approximately the same ultimate loads but different reinforcement detailings. The experimentally determined moment distribution coefficients (determined from support moments given in Figs 17 and 18 of Taerwe (1981)) and the measured deflection curves are compared to the predictions carried out according to Chapter 4.3.
Verification
98
400
35
35
198
Q
20003000
= var= 0.31 %= 0.31 % = var
CL
cρ aρbρcρ
x
(a) (b)
Fig. 5.31 Overview of Taerwe's (1981) beams: (a) structural system; (b) beam sections. The dimensions arein [mm].
Predictions Specimen CB 3
With n = 6.8 the section properties in the negative moment regions are EcII,sup = 33937 kNm2, EcIII,sup = 4674 kNm2, Mr,sup = 13.5 kNm and
ts,sup= 1.31 mrad/m ( = 1). Accordingly the section properties in the positive moment regions are EcII,span = 36037 kNm2, EcIII,span =
11904 kNm2, Mr,span = 14.7 kNm and ts,span = 0.46 mrad/m ( = 1). The average cracked stiffness is EcIII,avg = 8289 kNm2 and the ratio of
the cracked stiffnesses = EcIII,sup / EcIII,span = 0.4.
With a middle support moment (x = 0) equal to
1 2 2
, 2 2
3 m 2 m 2 kNm 5 m5 m 2 m
2 5 m 8a el
QM
the moment distribution is
21
,
21
,
2 m 5 m1 1 2 kNm if 0 3 m
5 m 5 m 2 2
2 m 5 m1 1 2 kNm 3 m if 3 m 5 m
5 m 5 m 2 2
a el
a el
x xM Q x x x
M xx x
M Q x x Q x x
This leads to the curvature distribution
22
2
2
2
1.31mrad m if 13.5 kNm4674 kNm
if 13.5 kNm 033937 kNm
if 0 14.7 kNm36037 kNm
0.46 mrad m if 14.7 kNm11904 kNm
Mk M
MM
MM
Mk M
The compatibility equation
5 m
1
0
0 M dx
with M1 = x – 5 m defines the moment distribution with factor . With Fig. 4.11 the State II distribution factor for = 0.4 is estimated (as
Q in CB3 is not at midspan) to be 0.7. The deflections under the load are determined with
3 m
2
0
a M dx
and M2 = x – 3 m. The average State II deflections are determined with 0 and
3 m
220 8289 kNm
Ma M dx
Fig. 5.32 compares the predicted and experimentally determined moment redistribution coefficients (Eq. (4.83)) and deflections of specimens 1 to 3. Also illustrated are the State II redistribution coefficients (dashed horizontal lines) estimated with Fig. 4.11 (a) and the State II average stiffness deflec
Verification
99
tions (dashed lines). The deflections are set equal to zero at Q = 0. Due to the nature of the static system, the support and span cracking loads are similar.
0
100
50
75
25
[kN
]Q
0
100
50
75
25
[kN
]Q
0
100
50
75
25
[kN
]Q
IIavg
IIavg
0
[kN]Q
20 40 60 80 100
0.5
0.5
0
0.5
0.5
0
0.5
0.5
0
0 5 10 15
a [mm]
test CB 1
test CB 2
IIavg
test CB 3
a
0.8%ρ =sup0.8%ρ =span
0.3%ρ =sup1.0%ρ =span
1.4%ρ =sup0.5%ρ =span
predicted
predicted
test CB 1
predicted = 10
test CB 2
predicted
predicted
predicted
test CB 3
predicted
State II
State II
with1.0κ =
2.1κ =
0.4κ =
kϕ
= 10
kϕ
= 10
kϕ
= 10
kϕ
= 10
kϕ
= 10
kϕ
1M
a
Ma,
el1
Ma
Ma,
el1
Ma
Ma,
el
(a) (b)
(c) (d)
(e) (f)
Fig. 5.32 Moment redistribution coefficients (Eq. (4.83)) and deflections for Taerwe's (1981) specimensCB1 to CB3, with = EcIII,sup / EcIII,span and = 1.
For all three specimens illustrated in Fig. 5.32, the measured midspan support moments are smaller than predicted and the measured deflection curves are initially steeper and then flatter than the predicted curves. The measured deflections are larger for > 1 and smaller for < 1 than the average stiffness deflections, confirming the influence of the stiffness ratio illustrated in Fig. 4.11 (b). Fig. 5.33 compares the measured deflection curves of all four specimens, which are very similar despite
Verification
100
the different stiffness ratios and average cracked stiffnesses. Elastically reinforced CB1 ( = 1, EcIII,avg,CB1) has the smallest deflections, followed by CB4 ( = 0.9, 0.92 EcIII,avg,CB1) and CB2 ( = 2.1, 1.13 EcIII,avg,CB1) and finally CB3 ( = 0.4, 0.81 EcIII,avg,CB1). It can be seen that both the average stiffness and the stiffness distribution influence the deflections. Further, Fig. 5.33 shows the influence of the reinforcement detailing on the yield load and therefore the service load range of the members.
0
100
50
75
25
[kN
]Q
CB1...CB4
14
2
3
0 5 10 15
a [mm]
Fig. 5.33 Comparison of the measured deflection curves for Taerwe's (1981) specimens CB1 to CB4
Twospan slab strips tested at ETH Zurich
Q
CL
b
1020
ρ = var
24002580
Qaρ = var
16@200Ø
100
240
1000
30
30= varØ
Ø
b
a = var
x
(a)
(b)
16@200Ø= varØb
Fig. 5.34 Overview of Alvarez and Marti's (1996) slab strips: (a) structural system; (b) slab section. Thedimensions are in [mm].
Alvarez and Marti (1996) tested 3 slab strips (ZP1 to ZP3), two with the same support reinforcement and two with the same span reinforcement. Fig. 5.35 illustrates the predicted and experimentally determined moment distribution coefficients and deflections. In all cases the moment redistributions between support and span cracking are overestimated. This is also reflected by the measured deflection curves between the support and span cracking loads; they are less stiff than predicted. The predicted State II (fully cracked) supporttospan moment redistributions are experimentally reached by ZP2 and ZP3, while the predicted State II spantosupport moment redistributions are not reached by
Verification
101
ZP1. Nevertheless, after span cracking, the measured deflections are between the curves predicted with = 1 and = 0.
Fig. 5.36 compares the measured deflection curves for specimens ZP1 (1.38,EIII,avg,ZP1), ZP2 (0.79,EIII,avg,ZP1) and ZP3 (0.66,EIII,avg,ZP1). It can be seen that the deformation behaviour of these three specimens is dominated by the average cracked stiffness.
[kN
]Q
0
80
40
60
20
[kN
]Q
0
80
40
60
20
[kN
]Q
0
80
40
60
20
IIavg
IIavg
IIavg
0
[kN]Q
20 40 60 80
0.5
0.5
0
0.5
0.5
0
0.5
0.5
0
0 4010 20 30
a [mm]
= 0
= 10
Q QQQ
aab
= 10
= 10
= 10
1
= 10
= 01
= 10
= 01
test ZP1
predicted
test ZP 1
predictedState II
predicted
test ZP 2
test ZP2predicted
State II
State II
test ZP 3
predicted predicted
test ZP 3
cracking span
cracking 1.38κ =kϕ
kϕ
kϕ
kϕ
kϕkϕ
kϕ
kϕ
kϕ
1M
a
Ma,
el1
Ma
Ma,
el1
Ma
Ma,
el
support
0.79κ =
0.66κ =
(a) (b)
(c) (d)
(e) (f)
Fig. 5.35 Moment distribution coefficients and deflection curves for Alvarez and Marti's (1996) specimensZP1 to ZP3 with = EcIII,sup / EcIII,span and = 1. The curves end at nominal steel yielding.
Verification
102
Predictions Specimen ZP1
With n = 6.7 the section properties in the negative moment regions are EcII,sup = 40055 kNm2, EcIII,sup = 7679 kNm2, Mr,sup = 40.5 kNm and
ts,sup = 2.26 mrad/m ( = 1). Accordingly the section properties in the positive moment regions are EcII,span = 38452 kNm2, EcIII,span =
5559 kNm2, Mr,span = 39.1 kNm and ts,span = 3.16 mrad/m ( = 1). The average cracked stiffness is EcIII,avg = 6619 kNm2 and the ratio of
the cracked stiffnesses is 1.4. With a middle support moment equal to
1 2 2
,
6 kNm 6 m1.65 m
8a elM Q
and a midspan support reaction (x = 0) equal to
1,14.44 m 6 kNm 6 m
6 m 6 m 2a elM
A Q
the moment distribution is
2 1
,
2 1
,
2 1
,
6 kNm1 if 0 2.58 m
2
6 kNm1 2.58 m if 2.58 m 4.98 m
2
6 kNm1 2 7.56 m if 4.98 m 6 m
2
a el
a el
a el
xM A x x
xM x M A x Q x x
xM A x Q x x
With M1 = x – 6 m and M2 = x – 3.6 m the rest of the calculation occurs as illustrated for CB 3.
0
80
40
60
20
3
1
2
ZP1...ZP3
0 4010 20 30
a [mm]
[kN
]Q
Fig. 5.36 Comparison of the measured deflection curves for Alvarez and Marti's (1996) specimens ZP1 toZP3.
Twospan beams tested during 400 days at the University of New South Wales
(a)
Q
1750 1750
150
100
CL
20
20
2 12Ø 2 12Ø
(b)
Fig. 5.37 Overview of Bakoss et al.'s (1982b; 1982a) beams: (a) structural system; (b) slab section. Thedimensions are in [mm].
Verification
103
Bakoss et al. (1982b; 1982a) tested two 2span beams (2B1 and 2B2) with midspan point loads sustained for 400 days. The two identical beams have an elastic, not curtailed reinforcement detailing with the same support and span reinforcement ratios (span = sup = 1.7 %). The support and span cracking loads are similar. The beams were tested horizontally in order to avoid the influence of selfweight. Therefore, the predictions are carried out with the interpolation equations given in Table 4.2, neglecting any moment redistributions ( = 0).
0
[kN
]Q
0
20
10
15
5
2B1 and 2B2
I
5 10 15 20 25
a [mm]
II
= 10
aa
a
= 0.30
II
23d 23d
423d
23d423d
kϕ
kϕ
Fig. 5.38 23day and 423day deflection curves of the Bakoss et al. (1982b; 1982a) beams 2B1 and 2B2( = 1). The average measured deflections (from three readings taken at the midpoints of threeidentical spans) are illustrated with crosses.
423day deflection predictions
With n = 7.5 the 23day stiffnesses are EcII = 880 kNm2 and EcIII = 408 kNm2 and the compression zone heights are xI = 80 mm and
xII = 51 mm. Accordingly, with n = 24.8 the effective 423day stiffnesses are Ec,efII,ef = 332 kNm2 and Ec,ef III,ef = 256 kNm2 and the com
pression zone heights are xI,ef = 89 mm and xII,ef = 77 mm. The State I net concrete section properties (n = 0) are Ac = 0.0148 m2 and xc = 74
mm. As the support and span stiffnesses are equal, if the splice sections are neglected, is 1. The free shrinkage strains were measured on
specimens with the same sections as the beams, so no conversions are necessary. The measured flexural tensile strength is transformed to
0.7
0.7
153 mm1.5
100 mm4.9 MPa 3.3 MPa
153 mm1 1.5
100 mm
ctf
according to Eq. (3.6). The 23day cracking moment equals 1.5 kNm.
The 423day tension stiffening curvature reduction (Eq. (4.14) with = 1 and k = 0.3) is
2
1.5 kN m 0.131 m 0.051 m1 3.3 MPa mrad0.5
2 408 kN m 0.131 m 0.077 m 27.3 GPa 0.131 m 0.077 m mts k
while the shrinkage curvatures are (Eq. (3.67))
2
,I 3 4
0.0148 m 0.074 m 0.089 m mrad0.64 ‰ 3.6
0.0401 10 m msh
and (Eq. (3.69))
,II
3 mrad0.64 ‰ 6.1
3 0.131 m 0.077 m msh
The maximum concrete shrinkage tensile stresses at 423 days (Eq. (3.68))
2
,I 2
0.01478 m mrad8.28 GPa 0.64 ‰ 1 0.15 m 0.089 m 3.6 3.2 MPa
0.02027 m msh
Verification
104
indicate that the entire beam is cracked by the end of the test, so that there is no need for interpolations. The total deflections of the fully
cracked beam are estimated by adding the State II deflections
3 21
II 2
7 3 3.5 m1.5 mm kN
144 16 256 kN m
Qa
the tension stiffening deflections = 1, k = 2/3,0 = 3/11)
2 2,II
3 1 9 mrad3.5 m 0.5 0.4 mm
11 8 121 mtsa
and the State II shrinkage deflections
2 2,II
3 1 9 mrad3.5 m 6.1 5.5 mm
11 8 121 msha
5.3 Slabs
Tabulated elastic solutions and linear finite element programs provide the deflections of uncracked flat plates. However, once cracking starts, the stiffness matrix becomes dependent on the stressresultants and, on principle, nonlinear finite element calculations are required in order to consider the influence of cracking on the bending and twisting stiffnesses. This means that flatslab deflection predictions must rely on either nonlinear finite element calculations or approximate methods.
This Chapter aims at illustrating the influence of cracking, creep and moment redistributions on flat plate deflections with three test series of largescale flat plates under sustained uniform loads. As a reference, the observed deflections are compared with the corresponding deflections a = ka ql4/D estimated with the uncracked elastic stiffness
3
I
212 1cE h
D
(5.2)
as well as a reduced stiffness
II,II I avg
g
ID D
I (5.3)
in an attempt to account for cracking. The latter is a gross simplification neglecting both the anisotropic nature of a cracked slab and the fact that the twisting stiffness is more affected by cracking than the bending stiffness. Creep is considered with the effective elastic modulus (Eq. (3.65)). The cracking loads qr = mr / (kM l2) are estimated with
2,I
6ct sh
r
f hm
(5.4)
neglecting any moment redistributions due to cracking.
Simply supported rectangular slabs tested at EPF Lausanne
Jaccoud and Favre (1982) (Fig. 5.39 (a)) tested three 4 m by 4 m, 120 mm thick slabs (B1 to B3), which are simply supported at the edges and have clamped corners. Tellenbach (1984) tested three 2.7 m by 2.7 m, 110 mm thick slabs. D1 and D2 (Fig. 5.39 (b)) have simply supported edges and clamped corners, while D3 (Fig. 5.39 (c)) is only supported by edge columns. In contrast to the other two slabs, D2 is skewly reinforced. All slabs were loaded with sustained uniform loads and the measured deflections are illustrated in Fig. 5.40.
Verification
105
(a)
2000
2100
120
CL
B1  B3
q 1350
1500
CL
D1, D2
q
1500
CL
D3
110
1350
q110
A A
AA
A A A A
AA AA
C L
C L C L
B1  B3 D1, D2 D3
(b) (c)
Fig. 5.39 Overview of the slabs tested at EPF Lausanne: (a) simply supported slabs B1 to B3 tested by Jaccoud and Favre (1982); (b) simply supported slabs D1 and D2 tested by Tellenbach (1984); (c)corner supported slab D3 tested by Tellenbach (1984). The dimensions are in [mm].
In Fig. 5.40 the measured deflections are marked with crosses. According to the test reports, all slabs except B1 featured advanced crack patterns on the bottom surface after initial loading. B1 was uncracked at initial loading, but partially cracked by the end of the test. The deflection estimates determined with DI (Eq. (5.2)) and DII (Eq. (5.3)) do not include shrinkage, which in the absence of span compression reinforcement, is considered responsible for the difference between the observed and estimated DII deflections.
373day deflection predictions for B1
The 373day stiffnesses DI = 1139 kNm and DII = 492 kNm are estimated with = 0, n = 25.9, avg = 0.55 % and davg = 95mm. With a
midspan deflection factor ka = 0.00406 according to e.g. Bareš (1971) the deflections are
4 4
I 2
4 m mm0.00406 0.91
1139 kNm kNm
qa
and
4 4
II 2
4 m mm0.00406 2.11
492 kNm kNm
qa
For a simply supported unit width slab strip with Ac = 0.119 m2, xc = 58.9 mm, II,ef = 0.1584 103 m4, xI,ef = 63.4 mm and
xII,ef = 39.0 mm (average stiffness) the reduced free shrinkages strains sh = 0.33 ‰ lead to sh,I = 0.9 mrad/m, sh,II = 4 mrad/m and
sh,I = 0.7 MPa. As a consequence
2 2,I
2 2,II
1 mrad4 m 0.9 1.8 mm
8 m
1 mrad4 m 4.0 7.9 mm
8 m
sh
sh
a
a
as well as
2 23.05 MPa 0.7 MPa 1 m 0.12 m5.7 kNm
6rM
The cracking load qr is determined assuming a maximum span moment equal to 0.0368 ql2 (e.g. Bareš (1971) for = 0). The shrinkage
deflections of 7.9 mm (not illustrated in Fig. 5.40) correspond to the difference between the observed and predicted DII deflections at t =
373 days.
Verification
106
q[k
N/m
]q
00
40
30
20
10
2
qr
qr
D1
D1
D2
D2
q[k
N/m
]q
00
40
30
20
10
2
qrB1
B3 B2
B1
B3 B2
qr
0
q[k
N/m
]q
000
40
30
20
10
2
00a
1/501/1001/200 1/67 1/501/1001/200 1/67
qr
D3
qrD3
13 days 373 days
21 days 386 days
21 days 386 days
ID IID
ID IID ID IID
ID IID ID
IID
ID IID
lal
Fig. 5.40 Midpanel slab deflections for slabs B1 to B3 (Jaccoud and Favre 1982) and D1 to D3 (Tellenbach1984). Slabs B1, B2, B3, D1 and D2 are simply supported at their edges (with clamped corners),while slab D3 is only supported at its corners.
Verification
107
Flatslab corner panels under sustained loads tested at the University of New South Wales
Guo and Gilbert (2002) tested seven 7.2 m by 6.2 m flat slabs supported on columns, which were pinned (S6) or fixed (S2, S4, S5 and S7) at the base. Each slab has four 3 m by 3 m corner panels of the type illustrated in Fig. 5.41 (a). Slabs S2, S4, S6 and S7 were uniformly loaded at 14 days and then maintained loaded for 1 to 2 years depending on the specimen. Slab S5 was loaded with 6.23 kN/m2 at 14 days unloaded again at 15 days and then left for 732 days under selfweight (2.16 kN/m2).
C L
CL
3000
100
3000600
(a)
220
S2140
all bars 10Ø
300
S6, S7
all bars 10Ø
220
220
S4, S5 140
all bars 10Ø
B
BB
BB
BB
100
90
90
8
8
8
8
8
8
(b)
B
Fig. 5.41 Overview of Guo and Gilbert's (2002) uniformly loaded flat plates. They are supported by 9 columns and consist of four identical corner panels: (a) one corner panel; (b) reinforcement in sectionBB. The dimensions are in [mm]. The two bottom and the two top layers have the same bar spacing. The upper two layers are limited to an area of 1.8 m by 1.8 m over the columns.
Fig. 5.42 shows the measured deflections (crosses) of the slabs (average of four panels). The figure also contains elastic deflection estimates determined with DI (Eq. (5.2)) and DII (Eq. (5.3)) (continuous lines) as well as estimated support and span cracking loads (dashed lines). They were determined with the elastic factors ka = 0.01326, kM = 0.256 (support, = 0) and kM = 0.0533 (span, = 0) given in the CEB Bulletin No. 158 (Comité EuroInternational du Béton 1985) for the corner panel of a twelvepanel example slab. Note that the supporttospan moment ratio of Guo and Gilbert's slabs is 5. The stiffnesses DI and DII (avg and davg of the bottom reinforcement) are determined with the 14day and corresponding longterm effective elastic modulus (for see Table A. 6 in Appendix A) assuming = 0. The additional shrinkage stresses are determined as shown above for B1.
As can be seen in Fig. 5.42, the applied load levels are between the 14day support and span cracking loads. Accordingly, after loading all slabs feature cracks on the top surface above the columns. Despite the presence of these support cracks, the observed 14day deflections correspond to the values estimated with the uncracked stiffness DI. Supporttospan moment redistributions due to cracking are considered responsible for maintaining the uncracked stiffness. After sustained loading (for 1 to 2 years depending on the specimen) all specimens feature cracks on the bottom surface. Nevertheless, even the deflections of slab S4 with the most advanced crack pattern still correspond to the uncracked DI deflections (determined with the effective modulus ratio).
Verification
108
q[k
N/m
]q
00
20
15
10
5
2
field cracking
S2 S2
0
q[k
N/m
]q
000
20
15
10
5
2
001/501/1001/200 1/67 1/501/1001/200 1/67
S7S6
S7S6
q[k
N/m
]q
00
20
15
10
5
2
S5S4
S5
S4
S5
support cracking
field cracking
support cracking
support cracking
field cracking
field cracking
support cracking
14 days= 100 mmh
2 years= 100 mmh
14 days= 90 mmh
1.25 years= 90 mmh
support cracking
field cracking
support cracking
field cracking
14 days= 100 mmh
1.5 years= 100 mmh
ID IID ID IID
ID
IID ID
IID
ID
IID
ID
IID
al
al
Fig. 5.42 Midpanel deflections of Guo and Gilbert's (2002) uniformly loaded panels. The predicted deflections (continuous lines) are determined with DI (Eq. (5.2)) and DII (Eq. (5.3)).
Verification
109
Cardington insitu concrete frame building
C L
7500
7500
400/400400/250
internalpanel
edgepanel
edgepanel
C L
400/400400/250
internalpanel
edgepanel
edgepanel
7500 7500
7500
Fig. 5.43 Plan view of the Cardington insitu building. The flat plates are 250 mm thick and consist oftwelve 7.5 m by 7.5 m columnsupported panels. The dimensions are in [mm].
At Cardington a sevenstory insitu concrete frame (Vollum et al. (2002)) was built and tested under service loads. Each floor slab has twelve 7.5m by 7.5m floor panels (Fig. 5.43), which were tested under sustained loads. The flat plates are 250 mm thick and column supported. The columns are fixed at both ends.
floor design bending
reinforcement backprops striking concrete type
concrete 28day strength
[t/floor] [levels] [d] [MPa]1 equivalent
frame 1 bar
16.91 27 skip
no admixtures 63
2 equivalent frame 1
bar17.1
1 1 skip no admixtures
58
3 equivalent frame 2 a)
bar 15.3
1 2 pump water red. admix.
57
4n b) yield line blanket cover bars14.5
2 2 pump selflevelling
water red. admix. superplast.
72
4s b) equivalent frame 1
blanket cover bars23.2
5 equivalent frame 1
oneway mats19.9
1 2 pump no admixtures
49
6 FE blanket cover twoway mats 25.5
1 3 pump 40 % GGBS c)
56
Table 5.3 Cardington flat plates. Notes a) No additional reinforcement for serviceability; b) north and southpanels; c) Ground Granulated Blastfurnace Slag.
The floors have different reinforcement detailings, backprop conditions and concrete properties (see Table 5.3). The concrete properties are given in Table A.6 of Appendix A. The flat plates were stripped of their formwork 1 to 7 days after loading (see Table 5.3), left for approximately one year under selfweight and then loaded with 3 kN/m2 for another year.
The midpanel deflections of floors 1 to 6 are illustrated in Fig. 5.44 (average of two internal panels) and Fig. 5.45 (average of four edge panels). The Cardington floor plan corresponds to the example flat plate given in the CEB report 158 (Comité EuroInternational du Béton 1985). The elastic deflection and moment coefficients provided by the report are used to estimate the deflections and cracking loads. The cracking moment (Eq. (5.4)) is estimated assuming shrinkage strains of 0.3 ‰ (reduced from 0.5 ‰ to account for the specimen size).
Verification
110
q
[kN
/m ]
q
00
20
15
10
5
2
0
q[k
N/m
]q
000
20
15
10
5
2
1/2001/4001/800 1/267 00 1/2001/4001/800 1/267
one yearat striking
800 daysone year
support cracking
cracking betw. columns
1 231 4n4s5 6
1 234n4s 56
support cracking
cracking betw. columns
1 2 34n4s 56 1 2 34n4s 56
overload during construction
ID
ID
ID ID
IID IID
IID
support cracking
cracking betw. columns
overload during construction
IID
support cracking
cracking betw. columns
overload during construction
al
al
Fig. 5.44 Midpanel deflections internal panels: = 0, Ec = 27 GPa, = 2.2, sh = 300 106, ka = 0.00307,kM = 0.256 (top face over internal columns), kM = 0.0536 (bottom face between internal columns)and kM = 0.0184 (bottom face span).
The deflections after striking correspond to the elastic shortterm deflections even though selfweight alone leads to cracking at the supports. According to the assumed moment distribution (neglecting moment redistributions), the construction overloads cause cracking on the bottom surface of the edge slabs and between the internal columns. This agrees with the visual inspection, where the slabs were found to be extensively cracked. Despite the extensive cracking, particularly the midpanel deflections of the edge panels remain close to the corresponding elastic deflections determined with the 600day creep coefficient. While all floors have similar deflections after striking, there is a considerable scatter after 800 days. In both cases the floors 1 and 4 with the highest 28day concrete strength show the smallest deflections.
Verification
111
q[k
N/m
]q
00
20
15
10
5
2
0
q[k
N/m
]q
000
20
15
10
5
2
1/2001/4001/800 1/267 00 1/2001/4001/800 1/267
cracking midpanel
support cracking
one yearat striking
800 daysone year
cracking betw. col.
cracking midpanel
support cracking
cracking betw. col.
623514n4s 1 63524n4s
63521 4n4s 63521 4n4s
overload during construction
cracking midpanel
support cracking
cracking betw. col.cracking midpanel
support cracking
cracking betw. col.
ID
ID
IIDIID
IID IID
IDID
al
al
Fig. 5.45 Midpanel deflections edge panels: = 0, Ec = 27 GPa, = 2.2, sh = 300 106, ka = 0.00917,kM = 0.256 (top face over internal columns), kM = 0.0536 (bottom face between internal columns)and kM = 0.0576 (bottom face span).
5.4 Summary
This chapter verifies the approaches discussed in Chapter 4 with a selection of test series from various research institutions. These test data comparisons show that:
A good upper limit can be provided for the steel stresses, crack widths and integral deformations of endrestrained tensile ties during the crack formation phase (see Fig. 5.4 and Fig. 5.27 (d)). However, the theoretical saw teethlike steel stress, crack width and deformation fluctuations (see Fig. 4.6) caused by the discrete cracks must be regarded as guidelines.
The shortterm State I and II section and corresponding member behaviour of beams is well understood (see e.g. Fig. 5.10, Fig. 5.13, Fig. 5.16, Fig. 5.22, Fig. 5.23 and Fig. 5.38) as long as there are no moment redistributions. The stiffnessdependent moment distributions of statically indeterminate beams are a challenge to predict (see Fig. 5.32 and Fig. 5.35). For the twospan beams illustrated in this chapter the predicted support moments altogether overestimate the experimentally determined support moments.
Verification
112
In combination with the shrinkage Eqs. (3.67) and (4.87), the Effective Modulus Method (EMM) enables straight forward predictions for the State I and II section and corresponding member deformations of beams under sustained loads (see e.g. Fig. 5.13, Fig. 5.16 and Fig. 5.38).
With the effective reinforcement ratio according to Eq. (4.4) the Tension Chord Model mostly provides good estimates for the maximum crack spacings ( = 1) in bending members. Together with the State II steel and concrete shrinkage strains they lead to reasonable upper (k= 0) crack width limits (see e.g. Fig. 5.11, Fig. 5.17, Fig. 5.18). Especially for low reinforcement ratios Schiessl's effective reinforcement ratio (Eq. (2.8)) leads to less consistent crack width predictions because, as pointed out in Chapter 4.1.1, it is incompatible with the Bernoulli bending theory (see MC 2010 curve in Fig. 5.11). The prediction quality of Frosch's crack width equation is highly variable and there can be an unrealistically large difference between the predicted side face and bottom crack widths (see e.g. Fig. 5.18).
The Tension Chord Model provides good lower limits for the average steel strains, average section curvatures, crack widths and integral deformations, which are determined assuming the maximum influence of tension stiffening ( = 1 and kaccording to Eq. (4.11)). However, it is not possible to locate the effective influence of tension stiffening between the upper (k= 0) and lower deformation limits (see Fig. 5.2, Fig. 5.10, Fig. 5.11, Fig. 5.13, Fig. 5.14, Fig. 5.16, Fig. 5.17, Fig. 5.18, Fig. 5.22, Fig. 5.23 and Fig. 5.38). For the statically determinate beams regarded here, the EC 2 (2004) load – deformation curves are mostly located between the two limits provided with the Tension Chord Model.
The predicted initial cracking loads determined with the average tensile strength both over and underestimate the observed cracking loads (see Fig. 5.4, Fig. 5.10, Fig. 5.22 and Fig. 5.23). Further, the span cracking loads in statically indeterminate beams are strongly influenced by the moment redistributions (see Fig. 5.32 and Fig. 5.35).
The uncracked elastic (effective modulus) slab panel deformations (corner, edge and centre panels) represent reasonable estimates even for extensively cracked slabs (see Fig. 5.42, Fig. 5.44 and Fig. 5.45). Possibly moment redistributions and membrane action are responsible for preserving the stiffness.
113
6 Discussion
6.1 Crack Width
Crack control can imply preventing cracks or limiting their widths. The concrete tensile stresses that lead to cracking are defined by the nature of the imposed or restrained deformations and the boundary conditions, while the crack widths are defined by the State II steel stresses, the crack spacing and the strains in the concrete between the cracks. This chapter discusses the influence of these parameters.
6.1.1 Tensile Members
Fig. 6.1 to Fig. 6.4 illustrate the cracking behaviour of a tensile tie according to Chapters 4.2.2 and 4.2.3 for reinforcement ratios above = As/(bh) = 0.5 %. The discussion includes axial loads as well as imposed and restrained deformations. The restrained deformations consist of uniform concrete shrinkage strains as well as uniform coolinginduced steel and concrete strains. Restraint stiffnesses (Eq. (4.38)) between the limiting cases of = ∞ and 0 are considered. The discussion also applies to the fictitious tension chords used to model base restrained walls (see Case (c) in Section Continuous EdgeRestraint of Chapter 4.2.2). The dashed vertical lines apply to the example member discussed below.
In order to prevent cracks from forming, the load, deformation or restrained concrete strains must not reach the values that start the crack formation phase (see Fig. 6.1). These limiting concrete strains increase with increasing concrete tensile strength, but unfortunately so do the corresponding steel stresses (Fig. 6.2) and crack widths (Fig. 6.4) during the crack formation phase. The start of restraintinduced cracking (Fig. 6.1 (c, d)) can further be delayed by reducing the shrinkage or coolinginduced strains or the degree of restraint. The influence of the reinforcement ratio is small, except for very low restraint stiffnesses.
For limiting crack widths it is convenient to distinguish between the crack formation phase and stabilized cracking. Fig. 6.1 illustrates the concrete strains delimiting the crack formation phase. In contrast to the strains at the start of the crack formation phase, the strains at the end of the crack formation phase are strongly dependent on the reinforcement ratio. For deformation or restraint induced cracking, increasing the reinforcement ratio reduces the length of the crack formation phase and therefore increases the rate at which the cracks form. As a constant tensile strength is assumed, axially loaded tensile ties (Fig. 6.1 (a)) and members with internally restrained shrinkage strains ( = 0) (Fig. 6.1 (d)) do not feature a theoretical crack formation phase, because cracking does not globally relieve the stress level. Under axial load all cracks form simultaneously upon reaching N = Nr, causing the strain increase illustrated in Fig. 6.1 (a).
Discussion
114
start & end
εsi = 0εci = εsh
κ
κ = 0
end
1.25
00000000
ε
start
e
0 0.5 1.0 1.5 2.0
[%]ρ
κ = 0.025
8
0.05
κ
εci = εsi = εΔTendκ = 0.025
8
0.050.18
> 0
,
start
κ = 0.025
8
0.05
0.18
start
κ = 0.0258
0.05
start
εe
end
N
0 0.5 1.0 1.5 2.0
[%]ρ
Es
1.00
0.75
0.50
0.25
[
]
1.25
1.00
0.75
0.50
0.25
end
ε ciE
s f ct[
]

(a) (b)
(c) (d)
f ct10
510
5
Fig. 6.1 Boundaries of the crack formation phase for n = 6 and = 1: (a) axial load; (b) imposed deformation (Eqs. (4.71) and (4.80); (c) restrained cooling strains (no internal restraint) (Eqs. (4.44) and(4.57)); (d) restrained shrinkage strains (Eqs. (4.44) and (4.57)). Note that for fct = 2 MPa andEs = 200 GPa the quotient 105 fct /Es equals 1.
The most important measure for crack width limitation is to ensure that the reinforcing steel does not yield under service loads. Fig. 6.2 illustrates the maximum steel stresses during the crack formation phase. They correspond to the steel stresses reached at N = Nr for axial loading and each time before a new crack forms during the entire crack formation phase for deformation or cooling induced cracking (Fig. 6.2 (a)). For shrinkageinduced cracking (Fig. 6.2 (b)), the illustrated steel stresses correspond to the steel stresses reached in the first crack just before a second crack occurs (point B in Fig. 4.6 (b)). In both cases the steel stress is primarily dependent on the concrete tensile strength and the reinforcement ratio. For serviceability concerns, yielding must also be prevented during stabilized cracking. Chapters 4.2.2 and 4.2.3 contain equations for determining the steel stresses during stabilized cracking.
The second most important parameter is the transfer length (Fig. 6.3 (a)), which is directly proportional to the crack width. According to the slippingbond approach, increasing the reinforcement ratio or reducing the bar diameter decreases the transfer length.
Discussion
115
50
100
150
200
250σ s
, ,r
II f ct
0
N
0 0.5 1.0 1.5 2.0
[%]ρ
5 m
0.05κ = 8
κ
0.0250
> 0
εci = εshεsi = 0
εe
κ
εci = εsi = εΔT
0 0.5 1.0 1.5 2.0
[%]ρ
(a) (b)
Fig. 6.2 Maximum State II steel stresses during the crack formation phase (Eq. (4.45)): (a) load, deformation or restraintinduced cracking with si – ci = 0 (e.g. due to cooling); (b) restraintinduced cracking with si – ci ≠ 0 (e.g. due to shrinkage) and ci,r,B acc. to Eq. (4.52)). Note that n = 6.
0 0.5 1.0 1.5 2.0
[%]ρ
l 0 Ø
5
10
15
20
25
00000000 00000000 0.5 1.0 1.5 2.0
[%]ρ
00
0.2
0.4
0.6
0.8
1
Es
f ctΔε
ts[
]
(a) (b)
105
Fig. 6.3 Tensile tie: (a) transfer length (Eq. (3.74)) related to bar diameter; (b) immediate contribution ofthe tensile concrete (Eq. (6.1) with = k = 1). Note that for fct = 2 MPa and Es = 200 GPa thequotient 105 fct /Es equals 1.
Fig. 6.3 (b) illustrates the average reduction of the steel and concrete strain difference (third term in Eq. (4.36))
1
2ct
tss
k f n
E
(6.1)
due to tension stiffening upon initial (k = 1) loading. For = 0.5 %, fct = 2 MPa and Es = 200 GPa the strain difference responsible for the crack opening is reduced by 1 ‰ if k = 1. However, both bond creep (Fig. 5.2) and the release of restrained shrinkage strains (see Fig. 5.22) reduce the influence of tension stiffening.
Discussion
116
0.1
0.2
0.3
0.4
0.5
σs, IIfct
200
150
100
w
0.1
0.2
0.3
0.4
0.5
0
crack formation
εeN
crack formation crack formation
crack formation
εsh
κ= 8
εci =εsi =
εΔTεΔT
εci
1.00.80.60.4
1.00.8
0 0.5 1.0 1.5 2.0
[%]ρ
crack formation
00000000
0.1
0.2
0.3
0.4
0.5
00000000
εci = εshεsi = 0
κ
εci =εsi =
εΔTεΔT
1.00.80.60.4
0 0.5 1.0 1.5 2.0
[%]ρ
+
1.00.80.60.4
= 0.05
1.00.80.6
κ= 0.05 κ = 0
crack formation
εe Es
fct10[ ]5
Es
f ct
104
Øw
Es
f ct
104
Øw
Es
f ct
104
Ø
(a) (b)
(c) (d)
(e) (f)
Es
fct10[ ]
5εci Es
fct10[ ]
5
εci Es
fct10[ ]
5 εci Es
fct10[ ]
5( ) εsi
Fig. 6.4 Crack widths: (a) axial load (Eq. (3.79)); (b) imposed deformations (Eqs. (4.77) and (4.79)); endrestrained deformations (Eqs. (4.46)) and (4.60)) due to (c) shrinkage/cooling with = ∞; (d) cooling with = 0.05; (e) shrinkage with = 0.05; (f) shrinkage with = 0. Note that n = 6 and = 1.The diagrams are valid as long as there is no steel yielding. Note that for fct = 2 MPa, Es = 200 GPaand = 10 mm the factor multiplying w equals 1.
Fig. 6.4 illustrates the maximum ( = 1) crack widths during the crack formation phase and stabilized cracking for imposed loads, imposed deformations and restrained deformations. The curves are valid for steel strains below the yield limit. During the crack formation phase the crack widths are identical in all illustrated cases and strongly dependent on the concrete tensile strength. The higher the concrete tensile strength, the larger is the crack width. This makes the concrete tensile strength an important parameter for tensile ties with extensive crack formation phases. After conclusion of the crack
Discussion
117
formation phase the crack widths increase (see also Fig. 5.8). During stabilized cracking, the influence of the concrete tensile strength decreases.
Fig. 6.5 illustrates minimum reinforcement ratios for limiting the crack widths illustrated in Fig. 6.4 (a) and Fig. 6.4 (c). According to Fig. 6.5 (b), a reinforcement ratio of 1.2 % ensures a related crack width wlim 104 Es / ( fct) below 0.1 (e.g. 0.2 mm for = 10 mm and fct = 2 MPa or 0.4 mm for = 10 mm and fct = 4 MPa) as long as the shrinkage and cooling induced concrete strains remain below 0.5 ‰.
00000000
50
100
150
200
250
σ s, II
f ct 0.2
0.3
0.4
0.1
=
0 0.5 1.0 1.5 2.0
[%]ρ
0.25
0.5
0.75
1.0
1.25
0.10.20.3=lim 0.4
εci = εsh + εΔT
min
00 0.5 1.0 1.5 2.0
[%]ρmin
N 0.05w Es
fct
104
Øε c
iEs f ct[
]

limw Es
fct
104
Ø
(a) (b)
105
Fig. 6.5 Minimum reinforcement ratios for crack width control: (a) axial load (Eq. (3.79)); (b) = ∞ endrestrained shrinkage and cooling strains (Eqs. (4.46) and (4.63)). Note that n = 6 and = 1. Forfct = 2 MPa and Es = 200 GPa the quotient 105 fct /Es equals 1.
Example Member
The dashed lines in Fig. 6.1 to Fig. 6.5 belong to an example member with = 1 %, fct = 2 MPa, = 10 mm, n = 6 and Es = 200 GPa.
Independent of the load case, the example member has a transfer length of 124 mm (Fig. 6.3 (a)) and a final crack spacing between 124 mm
( = 0.5) and 248 mm ( = 1). The concrete between the cracks reduces the steel and concrete strain difference responsible for the crack
width by 0.53 ‰ for = k = 1 (Fig. 6.3 (b)).
Under an axial load the example member cracks at N = Nr, causing the strains in the member to increase from 0.06 ‰ to 0.56 ‰
(Fig. 6.1 (a)). At N = Nr the State II steel stresses equal 210 MPa (Fig. 6.2 (a)) with a maximal crack width of 0.13 mm (Fig. 6.4 (a)).
Further loading up to a 400 MPa steel stress leads to maximum crack widths of 0.37 mm (Fig. 6.4 (a)).
Imposed deformations (Fig. 6.1 (b)) and fully endrestrained ( = ∞) (Fig. 6.1(c, d)) cooling/shrinkagestrains with absolute
values between 0.06 ‰ and 0.56 ‰ (crack formation phase) also lead to maximum crack widths of 0.13 mm (Fig. 6.4 (b, c)). After the
crack formation phase is concluded the crack widths increase, e.g. to 0.24 mm at 1 ‰.
Reducing the restraint stiffness shifts the crack formation phase, e.g. for shrinkageinduced strains to the limits of ci = 0.23 ‰
and 0.64 ‰ for = 0.05 or to ci = 1.05 ‰ for = 0 (Fig. 6.1 (d)). This does not affect the crack widths during the crack formation phase
(Fig. 6.4 (d to f)), but the crack widths during stabilized cracking decrease with decreasing restraint stiffness. Independent of the restraint
stiffness (for restrained cooling strains the maximum steel stress during the crack formation phase (Fig. 6.2 (a)) is 210 MPa. In
contrast, for restrained shrinkage strains (Fig. 6.2 (b)) the maximal steel stress during the crack formation phase depends on the length of
the tensile tie and the restraint stiffness.
Discussion
118
6.1.2 Bending Members
Fig. 6.6 illustrates the basic parameters of momentinduced cracking according to Chapter 4.2.1. The State II steel stresses at cracking (Fig. 6.6 (a)) are determined with the State II section properties.
l 0 Ø
5
10
15
20
25
00000000
50
100
150
200
250
σ s,
,rII f ct
00000000
00000000 0.5 1.0 1.5 2.0
[%]ρ
0
0000000
0 0.5 1.0 1.5 2.0
[%]ρ
0
2
4
6
8
10
[%]
ρ ef Schiessl
0.2
0.4
0.6
0.8
1
Frosch bottom
MC 2010MC 2010, EC 2
Es
f ctΔε
ts[
]
Tension Chord Model
Tension Chord Model
(a) (b)
(c) (d)
EC 2
105
Fig. 6.6 Momentinduced cracking: (a) steel stresses at cracking (M = Mr) acc. to Eq. (4.29); (b) effectivereinforcement ratio acc. to Eqs. (4.4) and (2.8); (c) contribution of tensile concrete acc. to Eq. (6.2)with = k = 1 and Eq. (2.6) with 3 = 0.6; and (d) transfer length acc. to Eq. (4.28), Eq. (2.5) withc = 30 mm and = 10 mm and Eq. (2.13) with s = 2/(4d), d = 250 mm, c = 30 mm and = 10 mm. Note that n = 6, ' = 0 and d/h = 0.9.
The effective reinforcement ratio (Fig. 6.6 (b)) is more controversial. However, regardless of whether Schiessl's (Eq. (2.8)) or the Tension Chord Model (Eq. (4.4)) expression is chosen, the effective reinforcement ratio soon reaches values, at which the influence of the tensile concrete is small (Fig. 6.6 (c)). As can also be seen in Fig. 5.14 and Fig. 5.17, for = As/(bd) above approximately 0.5 % it does not make any difference if the contribution of the tensile concrete
I II
II I2ct
tsc
f I d xk
E I h x
(6.2)
is considered (k = 1) or not (k = 0). Consequently, Frosch's (1999) crack width Eq. (2.12) does not consider the influence of the tensile concrete. However, the apparently small difference between effective reinforcement ratios has a large influence on the tensile concrete contribution (Fig. 6.6 (c)) at low reinforcement ratios. This can also be seen in Fig. 5.11 (d). The difference between the two effective reinforcement ratios most significantly influences the transfer length (Fig. 6.6 (d)). For the d, c and values assumed in Fig. 6.6 (d), Frosch's bottom face transfer length and the Tension Chord
Discussion
119
Model transfer length are similar. In contrast, Schiessl's effective reinforcement ratio used for the MC 2010 and EC 2 equations leads to larger transfer lengths. As a consequence, the MC 2010 steel stress vs. crack width relations in Figs. 5.14, 5.17, 5.18 are much steeper than the tension chord model relations. If an additional cover term is considered (EC 2), then an even larger transfer length results.
Fig. 6.7 illustrates related momentinduced crack widths determined with Eq. (4.27). For the shortterm crack widths ci = 0 with k = 1 are adopted, while the longterm crack widths assume shrinkage strains equal to 50 fct / Es as well as k = 0 and 1. Again, comparing the k = 0 and 1 curves in Fig. 6.7 (b) shows that for reinforcement ratios above approximately 0.5 % and certainly above 1 %, the contribution of the tensile concrete becomes insignificant. In contrast, the influence of shrinkage is clearly visible. This can also be seen in the crack width measurements illustrated in Fig. 5.14, Fig. 5.17 and Fig. 5.18.
Example Member
The dashed lines in Fig. 6.7 illustrate an example slab strip with = As/(bd) = 0.2 %, fct = 2 MPa, = 10 mm and Es = 200 GPa. In this
case the factor multiplying w equals 1. For the example member, the steel stresses at cracking (Fig. 6.6 (a)) are 100 · 2 MPa = 200 MPa and
the transfer length (Fig. 6.6 (d)) is 12 · 10 mm = 120 mm, implying a maximal crack spacing of 240 mm. This leads to an initial (at crack
ing) maximal crack width (Fig. 6.7 (a)) of 0.12 mm. Increasing the steel stresses up to 150 · 2 MPa = 300 MPa leads to 0.25 mm cracks
(Fig. 6.7 (a)). Alternatively (Fig. 6.7 (b)), if the cracking moment is maintained, shrinkage strains equal to 0.50 ‰ also lead to 0.25 mm
cracks or even 0.35 mm cracks, if tension stiffening is completely lost (k = 0).
0.1
0.2
0.3
0.4
0.5
00000000
kϕ= 1,
εsh fct
= 50Es
kϕ= 0,σs, II = 20015010050
0 0.5 1.0 1.5 2.0
[%]ρ0 0.5 1.0 1.5 2.0
[%]ρ0.20.2
at cracking
wE
s
f ct
104
Ø
(b)(a)
fct
σs, II = 20015010050
fct
kϕ= 1,σs, II = 20015010050
fct
Fig. 6.7 Maximum momentinduced crack widths (Eq. (4.27)) with n = 6, ' = 0, = 1 and d/h = 0.9: (a)k = 1 and ci = 0; (b) k = 0…1 and ciEs/fct = –50. With fct = 2 MPa, Es = 200 GPa, = 10 mm thefactor multiplying w equals 1.
Fig. 6.8 illustrates the minimum reinforcement ratios necessary for limiting the momentinduced crack widths in Fig. 6.7. For example, in order to limit bending crack widths below 0.15 fct / (Es 10
4) (e.g. 0.3 mm for = 10 mm and fct = 2 MPa or 0.6 mm for = 20 mm and fct = 2 MPa) at steel stresses equal to 150 fct (300 MPa for fct = 2 MPa) a minimal reinforcement ratio = As/(bd) of 0.4 % is necessary for shortterm loads (Fig. 6.8 (a)) or 0.7 % for sustained loads (Fig. 6.8 (b)).
Discussion
120
0.2
0.4
0.6
0.8
1
00000000100 125 150 175 200
σs, II
fct
ρ min
[%]
= 0.10
= 0.15
100 125 150 175 200σs, II
fct
= 0.10
= 0.30
= 0.35εsh
fct= 50Es
kϕ= 0
limw Es
fct
104
Ø
(a) (b)
= 0.20
= 0.25= 0.30= 0.35
= 0.15
= 0.20
= 0.25
limw Es
fct
104
Ø
Fig. 6.8 Minimum reinforcement ratio for limiting momentinduced crack widths: (a) k = 1 and ci = 0; (b)k = 0 and ciEs/fct = –50. Note that n = 6, ' = 0, = 1 and d/h = 0.9.
6.2 Deflections
There are a wide range of parameters influencing the deflections of RC bending members, such as the boundary conditions of the structural system, the loadhistory, the geometry and detailing of the individual sections as well as material parameters. The task of obtaining all of these input parameters at an accuracy level in line with our analytical models is already a challenge for uniformly reinforced simple beams tested under laboratory conditions, but hardly possible for the statically indeterminate members with curtailed reinforcement and unknown load histories used in practice. This means that strong simplifications are necessary. This chapter aims at identifying and discussing the decisive parameters for practical deflection estimates based on the equations presented in Chapter 4.3 and the test data validations discussed in Chapters 5.2 and 5.3.
6.2.1 Section Level
Influence of Cracking
Fig. 6.9 illustrates the ratio of the State I and II curvature for rectangular sections (Table 3.1), using the EMM (see Chapter 3.3.2) to consider creep. Both creep and additional tensile reinforcement reduce the difference between the uncracked and cracked section stiffness. If a lightly reinforced uncracked section is falsely modelled as a cracked section, then the immediate curvature is overestimated by over 90 %, while for a section with = 3 % and = 3, the curvature would only be overestimated by approximately 20 %. It is worth noting that the stiffness loss at cracking is larger for ' = than for ' = 0.
Discussion
121
ρ =ρ
’ 0d h,= 0.9
[%]ρ0 1 2 3
[%]ρ0 1 2 3
0ϕ = 3ϕ =
χ IIχ I
0
0.2
0.4
0.6
0.8
1.0
000
ρ =ρ
’ 0d h,= 0.8
ρ =ρ
’ 0d h,= 0.9
ρ =ρ
’ 0d h,= 0.8
(a) (b)
=
=
=
=
Fig. 6.9 Curvature ratio for rectangular sections with ≥ 0.15%: (a) without creep; (b) with creep according to the EMM. Note that n = 6 and d' = h – d.
Influence of Tension Stiffening
The reinforcement ratio has a much larger influence on the absolute tension stiffening curvature reduction (Fig. 6.10) than on the relative tension stiffening curvature reduction (Fig. 6.11). According to the Tension Chord Model (Eq. (4.14)), tension stiffening initially reduces the State II curvature by 50 to 20 % and by less than 20 % under sustained loads (Fig. 6.11). In comparison, Rao's semiempirical tension stiffening approach (Eq. (2.20)) features a larger tension stiffening influence at moment ratios below 2. It is likely that the average strain measurements from the constant moment zone of the 4point bending tests Rao used to derive his equation contained uncracked strains at low load levels due to the scatter in the concrete tensile strength.
[%]ρ0 1 2 3
0.5
1.0
1.5
0
[%]ρ0 1 2 3
χ Δts
d Es f ct
d h= 0.8h= 0.9 d h= 0.8
h= 0.90ϕ =
3ϕ =0.25k =ϕ
102
(a) (b)
Fig. 6.10 Influence of tension stiffening at section level according to Eq. (4.14). Note that ' = 0, n = 6 and = 1.
Discussion
122
Influence of Creep
According to the EMM, a creep coefficient of three increases the immediate uncracked section curvature by 100 to 300 % (Fig. 6.12 (a)). The creep curvature of uncracked sections can be reduced by increasing the tensile and compression reinforcement ratios or the effective depth. In a cracked section (Fig. 6.12 (b)) the creep curvature is much less sensitive to the tensile reinforcement ratio. However, in the presence of high tensile reinforcement ratios, the positive influence of the compression reinforcement is notable. For < 3 % the State II curvature is increased by up to 100 % in the case of = 3. For comparison, the dashed lines illustrate the curvature ratios determined with Ghali and Favre's (1986) curvature coefficients (Eq. (3.60)).
0
0.2
0.4
0.6
0.8
1.0
000
χ Δts
χ II
Rao 1β =χ II
Rao 0.5β =
= 0.25kϕ
0
0.2
0.4
0.6
0.8
1.0
0031.5 2 2.51
0
MrM
31.5 2 2.51
χ Δts
χ II
χ II
Rao 0.5β =
0ϕ =0.2 %ρ =
3ϕ =0.2 %ρ =
0ϕ =1.0 %ρ =
3ϕ =1.0 %ρ =
1=
Rao 1β =
= 0.25kϕ
kϕ
1=kϕ
(a)
(c)
(b)
(d)
MrM
Fig. 6.11 Relative influence of tension stiffening at section level according to Eq. (4.14). Rao's tension stiffening Eq. (2.20) is illustrated with dashed lines. Note that ' = 0, n = 6, = 1 und d = 0.85 h.
Influence of Shrinkage
The shrinkage curvatures (Eq. (3.67)) illustrated in Fig. 6.13 are related to the basic shrinkage curvature –sh/d. For a given shrinkage strain, the basic shrinkage curvature decreases linearly with increasing effective section depth. In an uncracked section (Fig. 6.13 (a, c)), the shrinkage curvature increases with increasing tensile reinforcement ratio, unless compression steel is provided. Under the given assumptions, shrinkage does not cause additional curvatures in uncracked symmetrically reinforced sections. In the absence of compression reinforcement, the shrinkage curvature of cracked sections (Fig. 6.13 (b, d)) approximately corresponds to the basic shrinkage curvature –sh/d. Compression reinforcement reduces the shrinkage curvature particularly in the case of large tensile rein
Discussion
123
forcement ratios. For comparison the curvature ratios determined with Ghali and Favre's (1986) curvature coefficients (Eq. (3.61)) are illustrated with dashed lines.
[%]ρ0 1 2 3
[%]ρ0 1 2 3
χχ ϕ=
3
ϕ=
0
0
4
3
2
1
0, d h= varρ =’d h= 0.8ρ =’
h= 0.9ρ,
State I State II
κϕϕ +1
κϕϕ +1
(b)(a)
EMM
d h= 0.8ρ =’
0,
h= 0.9
d h= 0.8ρ =’h= 0.9
ρ,
EMM
Fig. 6.12 Influence of creep at section level: (a) uncracked section; (b) cracked section. The reinforcementand effective depth parameters apply to the EMM (continuous lines) and Ghali and Favre's (1986)curvature coefficients (dashed lines according to Eq. (3.60)). Note that n = 6 and d' = h – d.
Comparison of Effects
For an uncracked rectangular cross section with a given moment M the initial curvature I is primarily a function of the section height h and the concrete elastic modulus Ec. If M is sustained until reaches 3, the resulting curvature is between 2 and 4 times the initial value. In nonsymmetrically reinforced sections shrinkage will further increase the curvature. The shrinkage curvature increases with increasing up to around –sh/d at = 3 %. An increasing section height has a positive influence on the initial curvature and the basic shrinkage curvature. Both tensile and compression reinforcement have a positive influence on the creep curvature. Assymmeterical reinforcement distributions have a negative influence on the shrinkage curvature.
If the same section is cracked, the initial curvature II is between 2 and 10 times larger depending on the reinforcement ratio. Creep maximally doubles II in absence of compression reinforcement. For sh = 1 ‰, Es = 200 GPa and fct = 2 MPa the multiplier of ts in Fig. 6.10 and of sh in Fig. 6.13 are equal and the influence of tension stiffening and shrinkage can be compared. In the absence of compression reinforcement, the initial tension stiffening curvature reduction at low reinforcement ratios (Fig. 6.10 (a)) is comparable with the shrinkage curvature for shrinkage strains sh = 1 ‰ (Fig. 6.13 (d)), while the influence of tension stiffening under sustained loads (Fig. 6.10 (b)) is much lower. An increasing section height has a positive influence on the basic shrinkage strains, while an increasing reinforcement ratio reduces the stiffness loss at cracking, the influence of tension stiffening and shrinkage.
Discussion
124
0
0, d h= 0.9ρ =’
0.5
1.0
1.5
χ Δsh
d ε sh

[%]ρ0 1 2 3
[%]ρ0 1 2 3
0
0.5
1.0
1.5
3ϕ = 3ϕ =
0, d h= varρ =’
d h= 0.8ρ =’
0, d h= varρ =’
ρ,State I State II
κ sh
κ sh
χ Δsh
d ε sh

(a) (b)
(c) (d)
EMM0, d h= 0.9ρ =’
EMMκ sh 0, d h= varρ =’
EMMd h= 0.8ρ =’ ρ,
d h= 0.9ρ =’ ρ,κ sh
EMMd h= 0.9ρ =’ ρ,
0, d h= 0.8ρ =’κ sh
EMM0, d h= 0.8ρ =’
0, d h= 0.9ρ =’EMM0, d h= 0.8ρ =’EMM
d h= 0.8ρ =’ ρ,EMMd h= 0.9ρ =’ ρ,EMM
1ϕ = 1ϕ =State I State II
Fig. 6.13 Influence of shrinkage at section level according to Eq. (3.67): (a) uncracked section with = 3;(b) cracked section with = 3; (c) uncracked section with = 1; (d) cracked section with = 1.The dashed lines illustrate Ghali and Favre's (1986) shrinkage curvature coefficient (Eq. (3.61)).Note that n = 6 and d' = h – d.
6.2.2 Member Level
Constant Stiffness
Fig. 6.14 shows the related deflections of a simple beam with uniformly reinforced rectangular sections. The illustrated deflections consider State I and II regions and optionally tension stiffening and creep. They are related to the corresponding State II deflections determined with either Ec ( = 0) or Ec,ef ( = 3). Before cracking (Ma/Mr ≤ 1) the ratio of the State I and II deflections corresponds to the curvature ratio (II/I) (Fig. 6.9). After initial cracking, the uncracked member regions are considered with the interpolation coefficients given in Table 4.2. For moment ratios above 1.5 the midspan deflections are reduced in comparison to the corresponding fully cracked deflections by up to 10 % due to remaining uncracked sections and by up to 30 % due to tension stiffening (upper limit with = 1). The loadindependency of the absolute tension stiffening term has the advantage that the interpolation coefficients can be combined with the moment ratio of the critical load case. The critical moment ratio occurs for example during construction if large loads are applied at an early age, making Ma large and Mr small.
Discussion
125
The uniformly loaded cantilever interpolation coefficient (simplified method) suggested by EC 2 (Eq. 2. 20) for all structural systems, leads to a stiffer deflection behaviour just after initial cracking and predictions between the Tension Chord Model limits ( = 1 and 0) above Ma / Mr = 1.25. Also under sustained loads the EC 2 longterm factor = 0.5 leads to predictions between the Tension Chord Model limits. The 4point bending tests illustrated in Chapter 5.2.1 show that the measured deflections are arbitrarily located between the limits of = 0 and 1.
0
0.2
0.4
0.6
0.8
1.0
a
000
IIa
0ϕ =
0.25k =ϕ
EC 2,
0.2 %ρ =
= 0
0
0.2
0.4
0.6
0.8
1.0
0031.5 2 2.51
0
MrM
31.5 2 2.51
a
3ϕ =0.2 %ρ =
0ϕ =1.0 %ρ =
3ϕ =1.0 %ρ =
Ia
Ia
1β =
EC 2, 0.5β =
Ia
Ia
EC 2, 1β =
EC 2, 0.5β =
kϕ
= 1kϕ= 0kϕ
= 0kϕ= 0kϕ
= 1kϕ
0.25k =ϕ
a IIa
(a) (b)
(c)
qa
(d)
qa
qa
qa
MrMa
Fig. 6.14 Deflections of a simple beam with n = 6, ' = 0, = 1 and d = 0.85 h for Ma ≤ My. The referenceState II deflections are determined with Ec ( = 0) or Ec,ef ( = 3).
Fig. 6.15 illustrates the related deflections of a symmetrically reinforced clampedended beam. The loadlevel is expressed by the ratio of the elastic support moment and the initial cracking moment. The related deflections consider cracking and arbitrarily creep and tension stiffening. They are determined with Eq. (4.82) in order to capture the moment redistributions that occur between support and span cracking. These moment redistributions are dependent on the ratio of the State I and II stiffness as well as the ratio of the support and span moment. They delay the extension of the cracked regions at the supports and preserve the overall stiffness until span cracking starts. In the two examples illustrated in Fig. 6.15, the span cracking load is reduced by approximately 25 %. The universal EC 2 interpolation coefficient does not consider moment redistributions and consequently overestimates the deflections between the cracking loads. The experimental loaddeflection curves of Alvarez and Marti's (1996) 2span slab strips feature an increased stiffness between support and span cracking, which is not quite as pronounced as predicted. Also the flat plates discussed in Chapter 5.3
Discussion
126
with elastic supporttospan cracking load ratios between 4 (edge panels) and 14 (internal panels) feature an uncracked deflection behaviour despite the presence of cracked regions.
0
0.2
0.4
0.6
0.8
1.0
a
000
IIa
0ϕ =
q
a
EC 2
0.2 %ρ =
0
0.2
0.4
0.6
0.8
1.0
0031.5 2 2.51
0
Mr,M
31.5 2 2.51
a,el
3ϕ =0.2 %ρ =
0ϕ =1.0 %ρ =
3ϕ =1.0 %ρ =
1
0
EC 2
1β =
EC 21β =
0.5β =
Ia
Ia
Ia
= 0kϕ
0.25= 0kϕ
1 = 0kϕ
0.25 = 0kϕ
EC 20.5β =
Ia
(a) (b)
(c) (d)
a IIa
q
a
q
a
q
a
Mr,Ma,el
0
Fig. 6.15 Deflections of a symmetrically reinforced clampedended beam for Ma ≤ My with n = 6, ' = =1and d = 0.85 h.
Variable Stiffness
Besides cracking also a nonuniform reinforcement detailing can lead to moment redistributions (see Fig. 4.11), which affect the deflections as well as the extent of the serviceability range (load range below steel yielding). Fig. 4.11 illustrates the influence of the supporttospan stiffness ratio on the State II deflections of a clampedended beam and a propped cantilever.
For a noncurtailed support and span tensile reinforcement, the State II deflections (Fig. 4.11 (b)) of the endrestrained example beam are approximately equal to the State II deflections determined with the average stiffness ratio, as long as the support stiffness is larger than the span stiffness (). In contrast a larger span stiffness can imply up to 2/3 larger State II deflections. The State II deflections of the propped cantilever exceed the average stiffness State II deflections for positive values, while a slightly larger span stiffness tends to have a favourable influence on the State II deflections. In both cases a reinforcement distribution, which is perfectly affine to the moment, increases the State II deflections by up to 50 %. The influence of the stiffness ratio can be appreciated for test specimens CB 1 to CB 3 shown in Fig. 5.32. Further, Fig. 5.33 shows that despite the significantly larger cracked stiffness, CB2 has the same deflections as CB4. This is most likely because of its unfavourable stiffness distribution.
Discussion
127
Fig. 6.16 compares the span to support stiffness and the moment ratios for the clampedended example member in Fig. 4.11. The dashed diagonal line stands for the case where the stiffness ratio coincides with the moment ratio. It can be seen that in general the provided support stiffness is too low for the corresponding moment. E.g. a uniform reinforcement distribution ( = 1) causes a moment ratio of 2, while the elastic reinforcement distribution ( = 2) causes a moment ratio of 3. The theoretical stiffness ratio of 5.6 corresponds to a moment ratio of 5.6 in a fully cracked member.
0 2 4 60
2
4
6
0
Msu
p
Msp
an
EIII,sup
EIII,span
q
a
Fig. 6.16 Support to span moment ratio vs. stiffness ratio
6.3 Summary
The cracking behaviour of tensile ties under axial loads as well as imposed or endrestrained deformations is strongly influenced by the extension of the crack formation phase:
In contrast to tensile ties with imposed or endrestrained deformations, axially loaded tensile ties have an instantaneous crack formation phase if a constant concrete tensile strength is assumed along the member.
During the crack formation phase the maximum crack widths are primarily defined by the reinforcement ratio and the concrete tensile strength (see Fig. 6.4). They are neither dependent on the magnitude of the imposed or restrained deformations (e.g. shrinkage or cooling strains) nor on the restraint stiffness.
Once the crack formation phase is concluded the crack widths increase with increasing load or deformation (see Fig. 6.4).
Lightly reinforced members are characterized by an extended crack formation phase (Fig. 6.1) and largely spaced cracks (Fig. 6.3 (a)) that are accordingly wide (Fig. 6.4). By increasing the reinforcement ratio the extension of the crack formation phase is reduced, causing a larger amount of thinner, closer spaced cracks.
The cracking behaviour of bending members is strongly dependent on the effective reinforcement ratio of the tension chord:
The parameter study carried out in this chapter (Fig. 6.6 (b)) shows that the bendingtheoryconform effective reinforcement ratio used by the Tension Chord Model is larger than the effec
Discussion
128
tive reinforcement ratio suggested by Schiessl (Eq. (2.8)). This leads to notably shorter transfer lengths (Fig. 6.6 (d)) and maximum crack spacings. This can also be seen in the test data comparisons in Chapter 5.2.1, where the gradient of the MC 2010 crack width vs. steel stress curves is larger than the Tension Chord Model gradient. Within these test data comparisons the predictions carried out with the Tension Chord Model effective reinforcement ratio are more consistent.
The large effective reinforcement ratios found in bending members make the influence of tension stiffening negligible for predicting momentinduced crack widths in members with reinforcement ratios over 0.5 % (Fig. 6.6 (c)). This is also clearly shown in the test data comparisons in Chapter 5, where, unless the reinforcement ratio is very small, the predicted crack width curves with k = 0 and 1 are close.
In terms of crack width, 0.25 ‰ shrinkage strains are approximately equivalent to 50 MPa additional State II steel stresses.
Section deformations are strongly influenced by cracking:
In lightly reinforced sections cracking reduces the section stiffness by up to 90 % (see Fig. 6.9 (a)). Creep evens out the State I and II stiffness difference.
For fct = 2 MPa and = k = 1 the tension stiffening curvature reduction reaches 1 ‰ /d at low reinforcement ratios (see Fig. 6.10 (a)). This is in the range of the curvature caused by shrinkage strainssh = 1 ‰ ( = 3) in strongly reinforced uncracked sections or singularly reinforced cracked sections (Fig. 6.13 (a)).
Moment redistributions have a strong influence on beam deflections:
The deflections of partially cracked statically determinate beams approximate the State II deflections with increasing reinforcement ratio and creep coefficient (Fig. 6.14).
The deflections of statically indeterminate beams are strongly influenced by the moment redistributions. Supporttospan moment redistributions due to cracking (Fig. 6.15) have a positive influence on the global stiffness between the support and span cracking loads, but reduce the span cracking load considerably.
The optimum supporttospan stiffness ratio for deflections (e.g. Fig. 4.11 (b)) does not necessarily coincide with the optimum supporttospan stiffness ratio for preventing early yielding (e.g. Fig. 6.16).
129
7 Conclusions and Outlook
7.1 Conclusions
Serviceability design is a topic of growing importance. This is mainly due to the increasing slenderness of our structures, which is driven by aesthetical and economical concerns and made possible by increasing material strengths. The service life spans of most structures require longterm serviceability approaches.
In most practical applications the accuracy of serviceability limit state predictions is limited by the complex and hardly known load history and the highly variable concrete properties. Nevertheless, reasonably reliable estimates of the magnitude of both integral and local deformations are required.
In contrast to the semiempirical cracking and deflection approaches illustrated in Chapter 2, the Tension Chord Model (Chapter 3.4) is an analytical model, which is suitable for both cracking and deflection predictions. The only empirical parameter in the model is the magnitude of the constant bond stress adopted between the steel and concrete. This makes the model applicable for a broad range of boundary conditions. The assumption of a constant bond stress is reasonable in view of the large scatter (e.g. concrete tensile strength) or the unknown components (e.g. load history) of the input parameters. The magnitude of the bond stress is in agreement with the findings of a parameter study involving 250 tests reported by König and Fehling.
Within the scope of this work the cracking and deformation behaviour of tensile ties and beams is modelled using the Tension Chord Model:
 new expressions are provided for determining the tension stiffening curvature reduction and the transfer length in bending members. They are based on an effective bendingtheoryconform reinforcement ratio (see Chapter 4.1.1).
 a factor k [1...0] is introduced (Eq. (4.11)) to express the effective contribution of the tensile concrete for a given crack spacing defined according to Eq. (4.25) by factor [1...0.5].
 the approach for describing the cracking behaviour of endrestrained tensile ties is extended to account for the combined presence of shrinkage and coolinginduced strains as well as elastic endrestraint conditions. This approach can also be used for estimating the cracking behaviour of baserestrained walls.
 deflection interpolation coefficients and spantodepth ratios are given for basic static systems. The interpolation coefficients can also be used to determine deflection reductions due to tension stiffening as well as additional shrinkage deflections. The universal interpolation coefficient provided in EC 2 (2004) represents a uniformly loaded cantilever.
The State I and II section behaviour forms the basis for all crack width and deformation predictions. Reliable predictions can be provided for the State I and II section deformations due to shortterm or sustained moments and/or axial forces. For standardly reinforced concrete sections creep can be considered with the Effective Modulus Method ( = 1).
Conclusions and Outlook
130
The State I and II section deformations lead to good upper limit deflection predictions for partially cracked statically determinate beams. However, for statically indeterminate beams the prediction quality for the deformations decreases due to the challenge of predicting the moment distribution. The influence of moment redistributions can be significant for statically indeterminate beams and slabs. The latter are further affected by membrane action.
Besides the State II steel strains, the maximum crack spacing is the crucial parameter for determining crack widths. With the bendingtheoryconform effective reinforcement ratio introduced in Chapter 4, the Tension Chord Model provides reasonable maximum crack spacings for bending members. This applies to beams without stirrups or with stirrups, which are spaced further apart than the theoretical maximum crack spacing.
With the Tension Chord Model ( = k = 1) good lower limits for the average steel strains and section curvatures as well as crack widths and integral deformations are obtained. However, depending on a number of parameters, such as load duration, crack spacing and section detailing, the effective influence of tension stiffening can be anywhere between this upper limit ( = k = 1) and zero (k = 0). Fortunately, crack width predictions in bending members with reinforcement ratios above 0.5 % are not sensitive to k. Also the deflections of heavily reinforced beams (which feature service load levels well above the cracking load level) and the deflections under sustained loads (where bond creep reduces the influence of tension stiffening) are insensitive to k. Further, it must be taken into account that tension stiffening can be present but this is not necessarily the case.
The Tension Chord Model represents an excellent tool for understanding and describing the shrinkage and coolinginduced cracking and deformation behaviour of elastically endrestrained tension ties. Good upper limits are predicted for the steel stress, deformation and crack widths during the crack formation phase. They are primarily defined by the concrete tensile strength and the reinforcement ratio and do not depend on the magnitude of the induced strains or the restraint stiffness.
7.2 Outlook
A better understanding of the moment redistributions under service loads is necessary to improve the prediction quality of statically indeterminate beam deflections. This would also provide valuable information for slab deflections.
The application of the endrestraint cracking approach described in Chapter 4.2.2 for baserestrained walls needs to be verified with largescale tests.
In this work Eqs. (4.66) & (4.63) and Eqs. (4.67) to (4.70) are suggested for modelling the cracking behaviour of concrete overlays and ground slabs. These equations need to be verified with test data and possibly further developed.
131
Notation
Alphabetic Characters
a = deflection A = transformed section area Ac = net concrete section area As = tensile reinforcement area A'
s = compression reinforcement area b = width of section c = depth of neutral axis of the strain plane, concrete cover, cement content d = effective depth of tensile reinforcement d' = effective depth of compression reinforcement E = modulus of elasticity f = material strength, related section property g = permanent load (dead load), related section property h = height of section I = second moment of area of transformed section j = crack number k = integration coefficient for elastic deflection equations, endrestraint stiffness l = length of member, span l0 = transfer length (American English) or transmission length (British English) m = related bending moment M = bending moment M = bending moment of equivalent statical system n = modular ratio (= Es/Ec) N = axial force q = variable load (live load), uniformly distributed load Q = single load R = degree of restraint, axial force s = crack spacing, bar spacing t = time in days T = temperature u = displacement V = shear force w = crack width, water content x = (horizontal) coordinate; depth of centroid of transformed section y = coordinate z = (vertical) coordinate
Greek Letters
= related deflections = fib and EC 2 tension stiffening factor, time factor creep/shrinkage = moment redistribution coefficient
Notation
132
= integral member deformation (e.g. deflection or rotation), bond slip = difference = strain (compression negative, tension positive) sh = free shrinkage strains sh (t, tsh) = deflection interpolation coefficient = factor = endrestraint stiffness factor, cracked stiffness ratio, curvature coefficient = tension stiffening coefficient = Poisson's ratio = related (horizontal) coordinate, ACI longterm coefficient = tensile reinforcement ratio As/(bd) of a bending member,
reinforcement ratio As/(bh) of a tensile member ' = compression reinforcement ratio As'/(bd) of a bending member TC = total reinforcement ratio (As + As')/(bh) of a bending member = stress (compression negative, tension positive) b = bond stress = creep coefficient (t, t0) = aging coefficient = curvature = moment ratio Mr/Ma,el I, II = uncracked state, cracked state = nominal diameter
Subscripts
a = ageadjusted, maximum (e.g. midspan), loadintroduction length b = bond between steel and concrete c = concrete, at restrained edge ct = tensile concrete e = imposed deformation ef = effective g = gross area of concrete section i = induced strains M = momentinduced r = cracking s = reinforcing steel sh = shrinkage t = time ts = tension stiffening u = unloading y = yielding = creep = curvature 0 = at loading, shortterm, construction, at origin of coordinates (z = 0) 1 = surcharge I, II = uncracked state, cracked state
Abbreviations
ACI = American Concrete Institute AAEMM = AgeAdjusted Elastic Modulus Method
Notation
133
EC = Eurocode EMM = Elastic Modulus Method fib = Fédération Internationale du Béton MC = Model Code RC = Reinforced Concrete TCM = Tension Chord Model
135
Literature
ACI Committee 207, 1990, ‘‘Effect of Restraint, Volume Change, and Reinforcement on Cracking of Mass Concrete’’, ACI Materials Journal, V. 87, No. 3, pp. 271–295.
ACI Committee 209, 1992, Prediction of Creep, Shrinkage, and Temperature Effects in Concrete Structures, ACI Committee Report, No. 209R92 (Reapproved 2008), American Concrete Institute, Farmington Hills, 47 pp.
ACI Committee 318, 2008, Building Code Requirements for Structural Concrete and Commentary, ACI Standard, American Concrete Institute, Farmington Hills, 473 pp.
Al Rawi, R.S., and Kheder, G.F., 1990, ‘‘Control of Cracking Due to Volume Change in BaseRestrained Concrete Members’’, ACI Structural Journal, V. 87, No. 4, pp. 397–405.
Alvarez, M., 1998, Einfluss des Verbundverhaltens auf das Verformungsvermögen von Stahlbeton, IBKBericht Nr. 236, ETH, Zürich, 182 pp.
Alvarez, M., and Marti, P., 1996, Versuche zum Verbundverhalten von Bewehrungsstahl bei plastischen Verformungen, IBKBericht Nr. 222, ETH, Zürich, 135 pp.
American Society for Testing and Materials, 2011, Standard Specification for Portland Cement, No. C150/C150M – 11, ASTM, Pennsylvania, 9 pp.
Bachmann, H., 1967, Zur plastizitätstheoretischen Berechnung statisch unbestimmter Stahlbetonbalken, IBKBericht Nr. 13, No. 13, ETH, Zürich, 188 pp.
Bakoss, S.L., Gilbert, R.I., Faulkes, K.A., and Pulmano, V.A., 1982a, ‘‘LongTerm Deflections of Reinforced Concrete Beams’’, Magazine of Concrete Research, V. 34, No. 121, pp. 203–212.
Bakoss, S.L., Gilbert, R.I., Faulkes, K.A., and Pulmano, V.A., 1982b, LongTerm Tests on Reinforced Concrete Beams, UNICIV Report, No. R204, University of New South Wales, Kensington, 43 pp.
Balázs, G.L., 1993, ‘‘Cracking Analysis Based on Slip and Bond Stresses’’, ACI Materials Journal, V. 90, No. 4, pp. 340–348.
Bareš, R., 1971, Berechnungstafeln für Platten und Wandscheiben, 2. Aufl., Bauverlag, Wiesbaden, 626 pp.
Base, G.D., Read, J.B., Beeby, A., and Taylor, H.P.J., 1966, An Investigation of the Crack Control Characteristics of Various Types of Bar in Reinforced Concrete Beams, Research Report, No. 18, Cement and Concrete Association, 44 pp.
Bažant, Z., 1972, ‘‘Prediction of Concrete Creep Effects Using AgeAdjusted Effective Modulus Method’’, ACI Journal Proceedings, V. 69, No. 4, pp. 212–217.
Bažant, Z., and Baweja, S., 1995, ‘‘Creep and Shrinkage Prediction Model for Analysis and Design of Concrete Structures  Model B3’’, Materials and Structures (RILEM), V. 28, No. 6, pp. 357–365.
Bažant, Z., and Najjar, L., 1973, ‘‘Comparison of Approximate Linear Methods for Concrete Creep’’, ASCE Journal of the Structural Division, V. 99, No. 9, pp. 1851–1874.
Literature
136
Beeby, A., 1999, ‘‘Serviceability Limit States  4.3.1 General’’, in Structural Concrete Textbook, Vol. 2, fib Bulletin No. 2, Fédération Internationale du Béton, Lausanne, pp. 67–74.
Beeby, A., and Scott, R., 2006, ‘‘Mechanisms of LongTerm Decay of Tension Stiffening’’, Magazine of Concrete Research, V. 58, No. 5, pp. 255–266.
Boltzmann, L., 1874, Zur Theorie der elastischen Nachwirkung, Sitzungsbericht der kaiserlichen Akademie der Wissenschaften, No. LXX, Band XXI, Sitzung vom 08. Oktober 1874, Wien, 275–306 pp.
Borosnyói, A., and Balázs, G.L., 2005, ‘‘Models for Flexural Cracking in Concrete: the State of the Art’’, Structural Concrete, V. 6, No. 2, pp. 53–62.
Branson, D., 1971, ‘‘Compression Steel Effect on LongTime Deflections’’, ACI Journal Proceedings, V. 68, No. 8, pp. 555–559.
Branson, D., 1977, ‘‘Deflection of Reinforced Concrete Beams and OneWay Slabs, and both Steel and Reinforced Concrete Composite Beams’’, in Deformation of Concrete Structures, McGrawHill, New York, pp. 111–262.
Branson, D., and Christiason, M.., 1971, ‘‘Time Dependent Concrete Properties Related to Design Strength and Elastic Properties, Creep, and Shrinkage’’, ACI Special Publication, V. 27, No. 13, pp. 257–278.
Broms, B., 1965, ‘‘Crack Width and Crack Spacing in Reinforced Concrete Members’’, ACI Journal Proceedings, V. 62, No. 10, pp. 1237–1256.
BuffoLacarriere, L., Rospars, C., Delaplace, A., Vu Duong, A., and Jason, L., 2011, International Benchmark, CONCRACK, Synthesis of the results, Workshop Report ConCrack 2, Paris, 120 pp.
Burns, C., 2008, ‘‘Deflection Prediction of OneWay RC Members’’, in Proceedings 7th International PhD Symposium in Civil Engineering, University of Stuttgart, pp. 203–204 and CD–ROM Part 14: Structural design, pp. 13–22.
Burns, C., Seelhofer, H., and Marti, P., 2008, ‘‘Discussion of ‘Tension Stiffening in Lightly Reinforced Concrete Slabs’ by R. Ian Gilbert’’, ASCE Journal of Structural Engineering, V. 134, No. 7, pp. 1262–1264.
Comité EuroInternational du Béton, 1985, CEB Design Manual on Cracking and Deformations, Bulletin, No. 158, EPFL, Lausanne, 250 pp.
Comité EuroInternational du Béton, 1993, CEBFIP Model Code 1990, Telford, London, 437 pp.
Considère, A., 1902, ExperimentalUntersuchungen über die Eigenschaften der ZementEisenKonstruktionen, Lehmann & Wentzel (Paul Krebs), Wien, 32 pp.
Dykes, A.R., 1978, ‘‘Chairman’s Address to the Scottish Branch of the Institution of Structural Engineers’’, in The Structural Engineer No. 5, Vol. 56A, pp. 150–151.
Espion, B., 1988, Long Term Sustained Loading Tests on Reinforced Concrete Beams, Bulletin du Service Génie Civil, No. 881, Service Génie Civil, Université Libre de Bruxelles, 62 pp.
Espion, B., and Halleux, P., 1990, ‘‘LongTerm Deflections of Reinforced Concrete Beams: Reconsideration of their Variability’’, ACI Structural Journal, V. 87, No. 2, pp. 232–236.
European Committee for Standardization, 2000, EN 1971, Cement  Part 1: Composition, Specifications and Conformity Criteria for Common Cements, European Committee for Standardization, Brussels, 17 pp.
European Committee for Standardization, 2004, Eurocode 2, Part 11: Design of Concrete Structures  General Rules and Rules for Buildings, European Committee for Standardization, Brussels, 246 pp.
Literature
137
European Committee for Standardization, 2011, Eurocode 2, Part 3: Design of Concrete Structures  Liquid Retaining and Containment Structures, European Committee for Standardization, Brussels, 30 pp.
Favre, R., Koprna, M., and Putallaz, J.C., 1981, ‘‘Deformation of Concrete Structures: Theoretical Basis for the Calculation’’, IABSE Surveys, No. S16/81, pp. 1–24.
Fédération Internationale du Béton, 2010a, Model Code 2010  First Complete Draft, Vol. 1, fib Bulletin, No. 55, Fédération Internationale du Béton, Lausanne, 318 pp.
Fédération Internationale du Béton, 2010b, Model Code 2010  First Complete Draft, Vol. 2, fib Bulletin, No. 56, Fédération Internationale du Béton, Lausanne, 312 pp.
Fédération Internationale du Béton, 1999, Structural Concrete Textbook, Vol. 1, fib Bulletin, No. 1, Fédération Internationale du Béton, Lausanne, 244 pp.
Frosch, R., 1999, ‘‘Another Look at Cracking and Crack Control in Reinforced Concrete’’, ACI Structural Journal, V. 96, No. 3, pp. 437–442.
Fürst, A., 2001, Vorgespannte Betonzugglieder im Brückenbau, IBKBericht Nr. 267, ETH, Zürich, 124 pp.
Gardner, J., 2004, ‘‘Comparison of Prediction Provisions for Drying Shrinkage and Creep of NormalStrength Concretes’’, Canadian Journal of Civil Engineering, V. 31, No. 5, pp. 767–775.
Gardner, J., and Lockman, M.J., 2001, ‘‘Design Provisions for Drying Shrinkage and Creep of NormalStrength Concrete’’, ACI Materials Journal, V. 98, No. 2, pp. 159–167.
Gergely, P., and Lutz, L., 1968, ‘‘Maximum Crack Width in Reinforced Concrete Flexural Members’’, ACI Special Publication, No. SP20, pp. 87–117.
Ghali, A., and Favre, R., 1986, Concrete Structures  Stresses and Deformations, Chapman & Hall, London, 352 pp.
Gilbert, R.I., 2007, ‘‘Tension Stiffening in Lightly Reinforced Concrete Slabs’’, ASCE Journal of Structural Engineering, V. 133, No. 6, pp. 899–903.
Gilbert, R.I., and Guo, X.H., 2005, ‘‘TimeDependent Deflection and Deformation of Reinforced Concrete Flat Slabs  An Experimental Study’’, ACI Structural Journal, V. 102, No. 3, pp. 363–373.
Gilbert, R.I., and Nejadi, S., 2004, An Experimental Study of Flexural Cracking in Reinforced Concrete Members under Sustained Loads, UNICIV Report, No. R435, School of Civil and Environmental Engineering, University of New South Wales, Sydney, 59 pp.
Goto, Y., 1971, ‘‘Cracks Formed in Concrete around Deformed Tension Bars’’, ACI Journal Proceedings, V. 68, No. 4, pp. 244–251.
Günther, G., and Mehlhorn, G., 1989, Langzeitverformungsverhalten von Stahlbetonzugkörpern, Forschungsbericht Nr. 8 aus dem Fachgebiet Massivbau, Gesamthochschule Kassel, 15 pp.
Guo, X.H., and Gilbert, R.I., 2002, An Experimental Study of Reinforced Concrete Flat Slabs under Sustained Service Loads, UNICIV Report, No. R407, School of Civil and Environmental Engineering, University of New South Wales, Sydney, 185 pp.
Heinzmann, D., 2006, Rissbildung und zugversteifende Mitwirkung des Betons, Diplomarbeit, IBK, ETH, Zürich, 122 pp.
Jaccoud, J.P., and Favre, R., 1982, ‘‘Flèche des structures en béton armé, vérification expérimentale d’une méthode de calcul’’, Annales de l’institut technique du bâtiment et des travaux publics, Série: Béton, V. 406, No. 208, pp. 21–66.
Literature
138
Jaccoud, J.P., Francou, B., and Camara, J.M., 1984, Armature minimale pour le contrôle de la fissuration des structures en béton, Projet de recherche, No. 8213, EPFL, Lausanne, 69 pp.
Kaufmann, W., 1998, Strength and Deformations of Structural Concrete Subjected to InPlane Shear and Normal Forces, IBKBericht Nr. 234, ETH, Zürich, 147 pp.
Kenel, A., 2002, Biegetragverhalten und Mindestbewehrung von Stahlbetonbauteilen, IBKBericht Nr. 277, ETH, Zürich, 114 pp.
Kenel, A., and Marti, P., 2002, Faseroptische Dehnungsmessungen an einbetonierten Bewehrungsstäben, IBKBericht Nr. 271, ETH, Zürich, 93 pp.
Kenel, A., Nellen, P., Frank, A., and Marti, P., 2005, ‘‘Reinforcing Steel Strains Measured by Bragg Grating Sensors’’, ASCE Journal of Materials in Civil Engineering, V. 17, No. 4, pp. 423–431.
Kheder, G.F., 1997, ‘‘A New Look at the Control of Volume Change Cracking of Base Restrained Concrete Walls’’, ACI Structural Journal, V. 94, No. 3, pp. 262–271.
König, G., and Fehling, E., 1988, ‘‘Zur Rißbreitenbeschränkung im Stahlbetonbau’’, Beton und Stahlbetonbau, V. 83, No. 3, pp. 161–167, 199–204.
Kuuskoski, V., 1950, Über die Haftung zwischen Beton und Stahl, Valtioneuvoston Kirjapaino, Helsinki, 203 pp.
Lohmeyer, G., and Ebeling, K., 2009, Weisse Wannen  einfach und sicher, Konstruktion und Ausführung wasserundurchlässiger Bauwerke aus Beton, 9., überarb. Aufl., Bau + Technik, Düsseldorf, 461 pp.
Marí, A.R., Bairán, J.M., and Duarte, N., 2010, ‘‘Longterm Deflections in Cracked Reinforced Concrete Flexural Members’’, Engineering Structures, V. 32, No. 3, pp. 829–842.
Marti, P., 1983, ‘‘Balken II: Verformungen’’, in Anwendung der Plastizitätstheorie auf Stahlbeton, ETH, Zürich, pp. 45–59.
Marti, P., 2004, Reinforced Concrete I Lecture Notes, Department of Civil, Environmental and Geomatic Engineering, ETH, Zürich, 92 pp.
Marti, P., Alvarez, M., Kaufmann, W., and Sigrist, V., 1998, ‘‘Tension Chord Model for Structural Concrete’’, Structural Engineering International, V. 8, No. 4, pp. 287–298.
Marti, P., Alvarez, M., and Sigrist, V., 1997, ‘‘Rissbildung und Mindestbewehrung’’, Schweizer Ingenieur und Architekt, V. 115, No. 41, pp. 832–838.
Marti, P., Sigrist, V., and Alvarez, M., 1997, Mindestbewehrung von Betonbauten, Bericht Nr. 529, Forschungsauftrag Nr. 82/95, Bundesamt für Strassenbau, Zürich, 55 pp.
McMillan, F.R., 1916, ‘‘Discussion of ‘Method of Designing Reinforced Concrete Slabs’ by A.C. Janni’’, Transactions ASCE, V. 80, pp. 1738–1754.
Mörsch, E., 1908, Der Eisenbetonbau, seine Theorie und Anwendung, 3rd ed., Konrad Wittwer, Stuttgart, 376 pp.
Mourachev, V., Sigalov, E., and Baïkov, V., 1971, ‘‘Etudes expérimentales et bases de calcul des constructions en béton armé’’, in Constructions en béton armé, Mir, Moscow, pp. 79–104.
Müller, H.S., and Hilsdorf, H.K., 1990, Evaluation of the Time Dependent Behavior of Concrete  Summary Report on the Work of General Task Group 9, CEB Bulletin d’information, No. 199, Comité EuroInternational du Béton, Lausanne, 201 pp.
NECS, 2010, ‘‘ConCrack.org’’, http://www.concrack.org/.
Literature
139
Nejadi, S., and Gilbert, R.I., 2003, Shrinkage Cracking in Restrained Reinforced Concrete Members, UNICIV Report, No. R433, School of Civil Engineering, University of New South Wales, Sydney, 92 pp.
Noakowski, P., 1985, ‘‘Verbundorientierte, kontinuierliche Theorie zur Ermittlung der Rißbreite  Wirklichkeitsnaher und einfacher Nachweis unter Berücksichtigung der Verbundgesetze und der Betonzugfestigkeit sowie unter Verknüpfung des Erstriss und Endrisszustands’’, Beton und Stahlbetonbau, V. 80, pp. 185–190, 215–221.
Pfyl, T., 2003, Tragverhalten von Stahlfaserbeton, IBKBericht Nr. 279, ETH, Zürich, 139 pp.
Pfyl, T., and Marti, P., 2001, Versuche an stahlfaserverstärkten Stahlbetonelementen, IBKBericht Nr. 268, ETH, Zürich, 137 pp.
Polak, M.A., and Killen, D., 1998, ‘‘The Influence of the Reinforcing Bar Diameter on the Behavior of Members in Bending and InPlane Tension’’, ACI Structural Journal, V. 95, No. 5, pp. 471–479.
Randl, N., and Wicke, M., 2000, ‘‘Schubübertragung zwischen Alt und Neubeton: Experimentelle Untersuchungen, theoretischer Hintergrund und Bemessungsansatz’’, Beton und Stahlbetonbau, V. 95, No. 8, pp. 461– 473.
Rao, P.S., 1966, Die Grundlagen zur Berechnung der bei statisch unbestimmten Stahlbetonkonstruktionen im plastischen Bereich auftretenden Umlagerungen der Schnittkräfte, DAfStb Heft Nr. 177, Ernst & Sohn, Berlin, 99 pp.
Rehm, G., 1961, Über die Grundlagen des Verbundes zwischen Stahl und Beton, DAfStb Heft Nr. 138, Ernst & Sohn, Berlin, 59 pp.
Rostásy, F., Koch, R., and Leonhardt, F., 1976, Zur Mindestbewehrung für Zwang von Aussenwänden aus Stahlleichtbeton, DAfStb Heft Nr. 267, Ernst & Sohn, Berlin, 83 pp.
Saliger, R., 1936, ‘‘HighGrade Steel in Reinforced Concrete’’, IABSE Congress Report, V. 2, pp. 293–315.
Sargin, M., 1971, StressStrain Relationships for Concrete and the Analysis of Structural Concrete Sections, University of Waterloo, Ontario, 167 pp.
Schiessl, P., 1989, ‘‘Grundlagen der Neuregelung zur Beschränkung der Rissbreite’’, in Erläuterungen zu DIN 1045 Betonund Stahlbeton, DAfStb Heft Nr. 400, Beuth, Berlin, pp. 157–175.
Scott, R., and Gill, P., 1990, ‘‘TimeDependent Distributions of Strain and Bond Stress along Tension Reinforcement’’, Proceedings of the Institution of Civil Engineers, V. 89, No. 2, pp. 301–312.
Seelhofer, H., 2009, Ebener Spannungszustand im Betonbau: Grundlagen und Anwendungen, IBKBericht Nr. 320, ETH, Zürich, 236 pp.
Sigrist, V., 1995, Zum Verformungsvermögen von Stahlbetonträgern, IBKBericht Nr. 210, ETH, Zürich, 159 pp.
Sigrist, V., and Marti, P., 1993, Versuche zum Verformungsvermögen von Stahlbetonträgern, IBKBericht Nr. 202, ETH, Zürich, 90 pp.
Taerwe, L., 1981, ‘‘Doorlopende Liggers van Gewapend Beton’’, Annales des Travaux Publics de Belgique, No. 5, pp. 423–441.
Tellenbach, A., 1984, Déformation à long terme des dalles en béton à l’état fissuré, Thèse, No. 544, EPFL, Lausanne, 256 pp.
Thoma, K.H., 2004, Stochastische Betrachtung von Modellen für vorgespannte Zugelemente, IBKBericht Nr. 287, ETH, Zürich, 118 pp.
Literature
140
Trost, H., 1967, ‘‘Auswirkungen des Superpositionsprinzips auf Kriech und Relaxationsprobleme bei Beton und Spannbeton’’, Beton und Stahlbetonbau, V. 62, No. 10, 11, pp. 230–238, 261–269.
Trost, H., and Mainz, B., 1968, ‘‘Verformungen von Stahlbetonbalken unter besonderer Berücksichtigung von Kriechen und Schwinden’’, VDIZeitschrift, V. 110, No. 11, pp. 432–440.
Vollum, R.L., Moss, R.., and Hossain, T.R., 2002, ‘‘Slab Deflections in the Cardington insitu Concrete Frame Building’’, Magazine of Concrete Research, V. 54, No. 1, pp. 23–34.
Watstein, D., and Parsons, D., 1943, ‘‘Width and Spacing of Tensile Cracks in Axially Reinforced Concrete Cylinders’’, Journal of Research of the National Bureau of Standards, V. 31, pp. 1–24.
Appendix A – Test Data Used in Chapter 5
141
Appendix A – Test Data Used in Chapter 5
Tensile Tests
Table A. 1: Longterm loadcontrolled tensile tests. Spec. l; b; h
As; Av =
As/bhfcm fctm
Es
fy
t0 t – t0
LS sm t0 t
srm t0
t unit mm % MPa GPa
MPad
kN ‰ mm
Günther & Mehlhorn (1989)
D1 1200; 70; 70 1Ø10; 
1.63 21a)
n/a 202 29
146 1 16.0 0.58 c)
0.74 c) 142 142
D4 " " 22 a)
n/a 202 29
144 1 16.0 0.73 c)
0.93 c) 113 113
D2 " " 22 a)
n/a 203 25
148 1 18.8 0.99 c)
1.16 c) 111 111
D5 " " 33 a)
n/a 203 157
180 1 18.8 0.96 c)
1.16 c) 141 141
D3 " " 28 a)
n/a 203 275
175 1 22.0 1.16 c)
1.36 c) 129 129
D8 " " 32 a)
n/a 198 158
179 1 22.0 1.09 c)
1.29 c) 129 129
D6 1200; 90; 90 1Ø10; 
0.98 20 a) n/a
203 49 176
1 21.8 1.16 c) 1.41 c)
114 114
D7 " " 20 a)
n/a 203 49
179 1 21.8 1.17 c)
1.42 c) 106 106
Scott & Gill (1990)
ST1 885; 100; 100 1Ø12; 
1.13 42a) 2.7b)
n/a 40 73
1 26.0
0.696 d) 0.883 d)
single crack
ST2 " " 42a)
3.4b) n/a 116
27 1 32.5 0.970 d)
1.095 d) single crack
ST3 " " 43a)
2.5b) n/a 35
36 1 15.0 0.509 d)
0.612 d) single crack
Beeby & Scott (2006)
T16B1 1200; 120; 120 1Ø16; 
1.4 19a) 1.7b)
n/a 28 e) 127
1 74.0 1.507 1.550
T16B2 " " 55a)
3.2b) n/a 28 e)
50 1 71.5 1.492
1.590
T16B3 " " 99a)
5.0b) n/a 28 e)
119 1 78.0 1.442
1.607
T20B1 1200; 120; 120 1Ø20; 
2.18 27a) 2.3b)
n/a 28 e) 133
1 74.0 1.050 1.097
T20B2 " " 71a)
3.1b) n/a 28 e)
56 1 72.8 1.020
1.109
T20B3 " " 94a)
3.9b) n/a 28 e)
48 1 70.5 0.901
0.976
Note that a) 80% of concrete cube strength; b) 90 % of splitting tensile strength; c) measured with inductive displacement transducers; d) straingauged reinforcement bar; and (e) assumed. When not given Es is assumed to be 205 GPa.
Appendix A – Test Data Used in Chapter 5
142
Table A. 2: Endrestrained shrinkage tests (Nejadi and Gilbert 2003). Spec. l; b; h
As; Av =
As/bhfcm fctm
Ecm
n Es
fy
t0 t – t0
sh
LS s,II wmax
srm
unit mm % MPa GPa GPa
MPad
 MPa mm mm
S1a a) S1b a)
2000 c); 600; 100 3Ø12; 
0.565 24.3 1.97 d)
22.8 9
n/a 3 150
457 0.98
1 1
AIIIe) 0.37 0.21
n/a
S2a a) 2000 c); 600; 100 3Ø10; 
0.393 " " " " " 1 AIIIe) 0.43 n/a
S2b b) " " 28.4
2.10 d) 23.2 8.8
" 3 150
495 1.16
1 AIIIe) 0.45 n/a
S3a a) S3b a)
2000 c); 600; 100 2Ø10; 
0.262 24.3 1.97 d)
22.8 9
n/a 3 150
457 0.98
1 1
AIIIe) 0.84 0.78
n/a
S4a a) S4b a)
2000 c); 600; 100 4Ø10; 
0.523 " " " " " 1 1
AIIIe) 0.29 0.21
n/a
a) concrete properties at 28 d batch I; b) concrete properties at 28 d batch II; c) tested length d) indirect tensile strength (brazil test); e) strain gauge measurements Nejadi & Gilbert (2003) Appendix III.
Table A. 3: Deformation controlled tensile tests (Jaccoud et al. 1984). The deformations were controlled over a length of 1 m (B1 series) or 1.2 m (B2 series)
Spec. l; b; h As; Av
fcm fctm
Ecm
n Es
fy
t0
e s,II b) wmax
srm
unit mm % MPa GPa GPa
MPad
 MPa mm mm
B11 2500; 450; 150 6Ø8; 
0.45 32.9 2.43
32.0 a)
6.4 a) n/a
617 36
Fig.
4.2 c) Fig.
4.2 c) Fig.
4.2 c) 365
B12 " 8Ø8; 
0.60 " " n/a 617
" Fig. 4.4 c)
Fig. 4.4 c)
Fig. 4.4 c)
158
B13 " 6Ø10; 
0.70 " " n/a 564
" Fig. 4.6 c)
Fig. 4.6 c)
Fig. 4.6 c)
150
B14 " 8Ø10; 
0.93 " " n/a 564
" Fig. 4.8 c)
Fig. 4.8 c)
Fig. 4.8 c)
154
B17 " 4Ø10; 
0.47 " " n/a 685
" Fig. 4.14 c)
Fig. 4.14 c)
Fig. 4.14 c)
234
B21 2500; 450; 150 6Ø8; 
0.45 43.5 2.71
35.2a) 5.8 a)
n/a 617
33
Fig. 4.16 c)
Fig. 4.16 c)
Fig. 4.16 c)
n/a
B22 " 8Ø8; 
0.60 " " n/a 617
" Fig. 4.18 c)
Fig. 4.18 c)
Fig. 4.18 c)
555
B23 " 6Ø10; 
0.70 " " n/a 564
" Fig. 4.20 c)
Fig. 4.20 c)
Fig. 4.20 c)
184
B24 " 8Ø10; 
0.93 " " n/a 564
" Fig. 4.22 c)
Fig. 4.22 c)
Fig. 4.22 c)
173
B25 " 4Ø10; 
0.47 " " n/a 685
" Fig. 4.24 c)
Fig. 4.24 c)
Fig. 4.24 c)
250
B26 " 6Ø10; 
0.70 " " n/a 685
" Fig. 4.26 c)
Fig. 4.26 c)
Fig. 4.26 c)
220
B27 " 8Ø10; 
0.93 " " n/a 685
" Fig. 4.28 c)
Fig. 4.28 c)
Fig. 4.28 c)
150
a) calculated from fcm assuming Es = 205 GPa; b) determined from measured axial force N/As; c) in Jaccoud et al. (1984).
Appendix A – Test Data Used in Chapter 5
143
Bending Tests
Table A. 4: Statically determinate bending members. Spec. l; b; h; d
As; As'; Av s; cside; cbot
a)' a)
fcm fctm
Ecm n
Es
fy
t0
tt0sh
LS M m
t0
t
wmax t0 t
srm
t0 t
unit m % MPa GPa 
GPa MPa
d
 kNm mra
d/m mm mm
Kenel & Marti (2002)
1.2 1.2 1.2m
a
Q Q
support section
d) d)
B1
3.6; 1.0; 0.2; 0.167 8Ø10; n/a; Ø8@300 0.125; 0.0575; 0.028
0.38
40 3.2b)
34 6.1
208 563
c)
27 n/a
n/a n/a
1 2 3 4 5
21.4 23.5 27.4 39.7 51.7
2.2 4.2 6.8
12.2 17.8
0.05 0.10 0.20 0.40 0.60
n/a n/a
150 150 150
B3
" 0.38
81 4.8b)
40 5.2
"
31 n/a
"
1 2 3 4 5 9
28.1 29.6 33.1 35.7 44.0
51.8
2.6 3.6 6.1 8.9
13.1 16.1
0.05 0.08 0.15 0.20 0.30 0.40
n/a n/a n/a
140 140 140
B4
3.6; 1.0; 0.2; 0.167 4Ø10; n/a; Ø8@300 0.250; 0.118; 0.028
0.19
37 3.1b)
34 6.2
"
27 n/a
"
1 2 3 4 5 6 7 8
16.8 16.3 17.1 21.0 20.7 20.7 25.2
25.4
1.9 3.6 5.1 7.5 9.5
11.0 13.0 14.9
0.20 0.30 0.30 0.40 0.45 0.50 0.55 0.70
n/a n/a n/a n/a n/a
280 280 280
B5
3.6; 1.0; 0.2; 0.165 4Ø14; n/a; Ø8@300 0.250; 0.118; 0.028
0.38
36 2.7 b)
36 5.7
202 508
27 n/a
"
3 4 5
10
23.5 30.1 39.6 41.8
0.20 0.30 0.40 0.45
n/a n/a
150 150
Jaccoud & Favre (1982)
1.0
a
1.1 1.0m
Q Q
midspan
C11 3.1; 0.75; 0.16; 0.131; 5Ø12; 2Ø6; Ø8@200 0.150; 0.069; 0.023
0.58 0.05
8
31 2.8f)
30 6.9
n/a n/a
28 360
0.35 2.31
6.42 0.2 3.5
n/a n/a
C12 " " " " " " " 9.63 1.8
7.9 0.05 0.11
n/a
C22 " " " " " " " 9.63 1.3
6.1 0.03 0.08
n/a
C13 " " " " " " " 12.84 5.6
12.3 0.14 0.25
200
C14 " " " " " " " 16.05 7.4
16.4 0.20 0.32
200
C24 " " " " " " " 16.05 7.8
15.6 0.19 0.30
200
C15 " " " " " " " 19.26 11.7
21.2 0.27 0.40
200
Appendix A – Test Data Used in Chapter 5
144
Spec. l; b; h; d As; As'; Av s; cside; cbot
a)' a)
fcm fctm
Ecm n
Es
fy
t0
tt0sh
LS M m
t0
t
wmax t0 t
srm
t0 t
unit m % MPa GPa 
GPa MPa
d
 kNm mra
d/m mm mm
Gilbert & Nejadi (2004) Q Q
1.17 1.17 1.17m
a
midspan
B1a 3.5; 0.25; 0.348; 0.3 2Ø16; n/a; n/a 0.15; 0.042; 0.04
0.53 18 1.8e)
23 9
n/a n/a
14 386
0.825 1.71
24.9 0.13 0.38
231 165
B1b " "
"
"
"
"
"
17.0
0.05 0.18
227 194
B2a 3.5; 0.25; 0.333; 0.3 2Ø16; n/a; n/a 0.18; 0.027; 0.025
"
"
"
"
"
"
24.8
0.10 0.36
201 129
B2b " "
"
"
"
"
"
16.8 0.05 0.18
315 181
B3a 3.5; 0.25; 0.333; 0.3 3Ø16; n/a; n/a 0.09; 0.027; 0.025
0.80 "
"
"
"
"
34.6 0.08 0.28
230 130
B3b " "
"
"
"
"
"
20.8 0.05 0.13
232 133
S1a 3.5; 0.40; 0.161; 0.13 2Ø12; n/a; n/a 0.308; 0.04; 0.025
0.42 18 1.8e)
23 9
n/a n/a
14 386
0.825 1.71
6.81 0.13 0.20
136 121
S1b " "
"
"
"
"
"
5.28
0.08 0.15
189 115
S2a 3.5; 0.40; 0.161; 0.13 2Ø12; n/a; n/a 0.154; 0.04; 0.025
0.63 "
"
"
"
"
9.87
0.130.23
136 97
S2b " "
"
"
"
"
"
6.81 0.080.18
138 95
S3a 3.5; 0.40; 0.161; 0.13 2Ø12; n/a; n/a 0.103; 0.04; 0.025
0.84 "
"
"
"
"
11.35 0.100.25
144 111
S3b " "
"
"
"
"
"
8.34 0.080.20
142 128
ConCrack (2010)
Q
1.75 0.8m
CL
RL1
2.55; 1.6; 0.8; 0.722 1632; 825; 16@350/310 var; 0.083; 0.038
1.11 0.34
60 4.65g)
39 5.1
200 n/a
63
0.490 1.1
RG8
2.55; 0.5; 0.8; 0.725 532; 532; 16@220/200 var; 0.046; 0.046
1.10 1.10
60 4.65g)
39 5.1
200 n/a
30
0.433 1.1
a) the reinforcement ratios refer to the effective depth (As/bd); b) direct tensile strength; c) static yield strength; d) averaged AB and ME; e) 90% of splitting tensile strength; f) 50% of flexural tensile strength; g) splitting tensile strength.
Appendix A – Test Data Used in Chapter 5
145
Table A. 5: Statically indeterminate beams. Spec. l; b; h; d
As,a; As,b; Av
aa)
b a)
c a)
fcm fctm
Ecm n
Es
fy
t0
tt0sh
t0
t
a t0 t
unit m % MPa GPa 
GPa MPa
d
 mrad/
m mm
Taerwe (1981)
exact splice lengths unknown
a
M 2 3m
ab cc
CB1 5; 0.198; 0.4; 0.365 n/a; n/a; n/a splice lengths unknown
0.78 0.78 0.31
27 3.6b) 30 c) 6.8
205 c) 500 c)
CB2 " 1.36
0.53 0.31
" " "
CB3 " 0.31
0.95 0.31
" " "
CB4 " 0.66
0.75 0.31
" " "
Alvarez and Marti (1996)
Q QQQ
a1 3.6m
M
+
2.4 2.6
ab
ZP1 6; 1; 0.24; 0.21 1012; 1010; 8@200d)
0.54 0.37
49.3 3.5e)
33.6 6.5
217 600
26 Fig. 4.49bf)
Fig. 4.49cf)
ZP2 6; 1; 0.24; 0.21 1012; 1014; 8@200d)
0.54 0.73
51.2 3.6e)
31.0 7.0
217 600
32 Fig. 4.54bf)
Fig. 4.54cf)
ZP3 6; 1; 0.24; 0.21 108; 1010; 8@200d)
0.23 0.37
50.2 4.5e)
32.6 6.7
217 600
36 Fig. 4.59bf)
Fig. 4.59cf)
Bakoss et al. (1982b; 1982a) tested horizontally
a
M
3.5 m
aa
2B1 2B2
3.5; 0.1; 0.15 212; 212; n/a
1.7 1.7
33.1 4.9 b)
27.3 7.5
205 c) 500 c)
22 400
640 2.3
Table 6 g)
a) the reinforcement ratios refer to the effective depth (As/bd); b) flexural tensile strength; c) estimated; d) transverse reinforcement; e) splitting tensile strength; f) in Alvarez and Marti (1996); g) in Bakoss et al. (1982b; 1982a).
Appendix A – Test Data Used in Chapter 5
146
Table A. 6: Slabs.
Spec. lx ly h
span x, y, avg dx, dy, davg
fc, fct, Ec Es, n,, sh
t0
t t0
g+q
atest at / a0
bottom surface
top surface
unit m %, mm MPa, GPa, 106 d kN/m2 mm
Simply supported slabs with clamped corners from Jaccoud & Favre (1982)
B1 4 4
0.12
0.52, 0.58, 0.55 100, 90, 95
3.1, 28.0 205a), 7.3 2.55, 434
13 360
10.850
4.2 13.3
3.2 no cracks t0; part cracked t
B2 " " " " 18.757
28.1 47.9
1.7 well cracked
B3 " 0.76, 0.38, 0.57
99, 89, 94 " " " 24.3
46.3 1.9 well cracked
Simply supported slabs with clamped corners from Tellenbach (1984)
D1 2.7 2.7
0.11
0.55, 0.62, 0.59 95, 85, 90
2.5, 29.6 205a), 6.9
2.4, 396
21 365
26.6
6.6 16.3
2.5 well cracked
D2 " "
Skew reinf. " " 26.6
4.6
14.6 3.2 well cracked
Slab on corner columns from Tellenbach (1984)
D3 " "
" " 8.9
10.2 27.2
2.7 fully cracked
Corner panels with base pined (S6) or base fixed (S2, S4, S5, S7) columns from Guo & Gilbert (2002)
S2 3 3
0.1
0.46, 0.41, 0.44 77, 87, 82
2.7b), 29.1 219, 7.5
2.9 c), 854d)
14 456
5.72 2.09e) 12.1e)
5.8 no cracks 14d 2 cracks 180 d
crac
ks a
bove
col
umns
aft
er lo
adin
g
S4
3 3
0.09
0.53, 0.46, 0.50 67, 77, 72
2.8 c), 22.0 219, 10
3.6, 780d)
15 761
8.39 4.51e) 25.9 e)
5.7 no cracks 15d 2 cracks 17d well cracked
776d
S5
"
" " 14 15 15
733
2.16 8.39 2.16 2.16
2.02e) 3.91e) 2.27e) 7.37 e)
3.2 no cracks 15d some cracks 45 d
S6 "
0.39, 0.34, 0.37 67, 77, 72
2.4b), 19.0, 219, 11.5,
2.7c), 512d)
14 494
5.26 3.68e) 19.6e)
5.3 no cracks at 14d some cracks 42 d
S7 "
" " 14 494
5.55 3.14e) 20.6e)
6.6 no cracks at 14d some cracks 45 d
Cardington insitu building (Vollum et al. 2002) with flat plates
1 edge panels
7.5 7.5
250
0.3f) 200f)
63g), 2.5h) i), 24i) 205a), 8.5i)
2.6j) k), 535j) k)
27 ≈ 360 ≈ 360 ≈ 800
6.25 6.25 9.25 9.25
4.9k) 12.5 k) 14.7 k) 17.9 k)
2.6
2 edge panels
"
58g), 2.4h) i), 26i) 205a), 7.9 i)
2.3 j) k), 624 j) k)
1 ≈ 360 ≈ 360 ≈ 800
6.25 6.25 9.25 9.25
5.5 k) 15.2 k) 17.9 k) 22.5 k)
2.8
Appendix A – Test Data Used in Chapter 5
147
Spec. lx ly h
span x, y, avg dx, dy, davg
fc, fct, Ec Es, n,, sh
t0
t t0
g+q
atest at / a0
bottom surface
top surface
unit m %, mm MPa, GPa, 106 d kN/m2 mm
3 edge panels
"
57g), 2.7h) i), 33i) 205a), 6.2i)
2.0j) k), 521j) k)
2 ≈ 360 ≈ 360 ≈ 800
6.25 6.25 9.25 9.25
5.3 k) 17.1 k) 20.1 k) 24.9 k)
3.2
4N edge panels
"
72g), 2.5h) i)), 29i) 205a),7.1i)
2.1j) k), 449j) k)
2 ≈ 360 ≈ 360 ≈ 800
6.25 6.25 9.25 9.25
4.3 l) 13.8 l) 15.9 l) 19.5 l)
3.2
4S edge panels
"
72g), 2.5h) i)), 29i) 205a),7.1i)
2.1j) k), 449j) k)
2 ≈ 360 ≈ 360 ≈ 800
6.25 6.25 9.25 9.25
4.8 l) 14.0 l) 16.5 l) 19.7 l)
2.9
5 edge panels
"
47g), 2.5h) i), 26i) 205a), 7.9i)
2.1j) k), 503j) k)
2 ≈ 360 ≈ 360 ≈ 800
6.25 6.25 9.25 9.25
5.1 k) 16.6 k) 18.9 k) 23.5 k)
3.3
6 edge panels
"
56 g), 2.0h) i), 23i) 205a), 8.9i)
1.8 j) k), 370 j) k)
3 ≈ 360 ≈ 360 ≈ 800
6.25 6.25 9.25 9.25
6.3 k) 18.6 k) 21.4 k) 26.3 k)
3.0
1 int. panels
7.5 7.5
250
0.3f) 200f)
63g), 2.5h) i), 24i) 205a), 8.5i)
2.6j) k), 535j) k)
27 ≈ 360 ≈ 360 ≈ 800
6.25 6.25 9.25 9.25
2.9 l) 5.7 l) 7.4 l) 9.5 l)
2.0
2 int. panels
"
58g), 2.4h) i), 26i) 205a), 7.9 i)
2.3 j) k), 624 j) k)
1 ≈ 360 ≈ 360 ≈ 800
6.25 6.25 9.25 9.25
3.5 l) 9.0 l)
10.7 l) 14.2 l)
2.6
3 int. panels
"
57g), 2.7h) i), 33i) 205a), 6.2i)
2.0j) k), 521j) k)
2 ≈ 360 ≈ 360 ≈ 800
6.25 6.25 9.25 9.25
3.5 l) 9.9 l)
12.1 l) 15.5 l)
2.8
4N int. panel
"
72g), 2.5h) i)), 29i) 205a),7.1i)
2.1j) k), 449j) k)
2 ≈ 360 ≈ 360 ≈ 800
6.25 6.25 9.25 9.25
3.2 8.2
10.2 13.3
2.6
4S int. panel
"
72g), 2.5h) i)), 29i) 205a),7.1i)
2.1j) k), 449j) k)
2 ≈ 360 ≈ 360 ≈ 800
6.25 6.25 9.25 9.25
2.4 7.8 9.9
11.8
3.3
5 int. panels
"
47g), 2.5h) i), 26i) 205a), 7.9i)
2.1j) k), 503j) k)
2 ≈ 360 ≈ 360 ≈ 800
6.25 6.25 9.25 9.25
2.0 l) 10.1 l) 11.9 l) 15.0 l)
5.1
6 int. panels
"
56 g), 2.0h) i), 23i) 205a), 8.9i)
1.8 j) k), 370 j) k)
3 ≈ 360 ≈ 360 ≈ 800
6.25 6.25 9.25 9.25
3.0 l) 8.6 l)
10.6 l) 13.6 l)
2.9
a) assumed; b) flexural tensile strength; c) values from Gilbert & Guo (2005); d) shrinkage specimen 600/600 mm with same thickness as slabs e) average of 4 bays; f) assuming davg = 0.8 h; g) 28day; h) splitting strength; i) at striking; k) 600 d; j) measured on specimens 102 mm, l = 254 mm; k) average of 4 panels; l) average of two panels.
149
Curriculum vitae
Clare Burns Born on the 25 July 1977 Citizen of Effingen, AG
Education
1984 – 1997 Primary School in Effingen, Grammar School in Frick and Aarau, Matura Type C
1997 – 2002 Civil Engineering Studies at ETH in Zurich, graduated Dipl. Bauingenieur ETH
Work Experience
2000 – 2001 Trainee (part time), Engineering Office Wolfseher und Partner AG, Zurich
2002 – 2005 Site Engineer, Building Companies SERPREC Ltda. und Quiroga Ltda., Cochabamba, Bolivia
2005 – 2011 Assistant and Research Associate of Prof. Dr. P. Marti at the Institute of Structural Engineering, ETH Zurich